# Electronic Supplementary Material (ESI) for ChemComm.
# This journal is © The Royal Society of Chemistry 2018

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_ma18010_0m
_database_code_depnum_ccdc_archive 'CCDC 1857777'
_audit_update_record             
;
2018-07-24 deposited with the CCDC.
2018-08-23 downloaded from the CCDC.
;
_audit_creation_date             2018-06-24
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'C13 Dy1.45 K6 N2 O63.75 Si W11'
_chemical_formula_sum            'C13 Dy1.45 K6 N2 O63.75 Si W11'
_chemical_formula_weight         3724.81
_chemical_absolute_configuration unk
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_H-M_alt        'P 1 21 1'
_space_group_name_Hall           'P 2yb'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   10.6779(5)
_cell_length_b                   20.1665(9)
_cell_length_c                   15.5021(8)
_cell_angle_alpha                90
_cell_angle_beta                 103.3465(19)
_cell_angle_gamma                90
_cell_volume                     3248.0(3)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    9179
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      36.23
_cell_measurement_theta_min      2.62
_shelx_estimated_absorpt_T_max   0.182
_shelx_estimated_absorpt_T_min   0.099
_exptl_absorpt_coefficient_mu    21.561
_exptl_absorpt_correction_T_max  0.7471
_exptl_absorpt_correction_T_min  0.3205
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1411 before and 0.0783 after correction.
The Ratio of minimum to maximum transmission is 0.4290.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.809
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             3279
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.12
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0575
_diffrn_reflns_av_unetI/netI     0.0383
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            70843
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.680
_diffrn_reflns_theta_min         3.575
_diffrn_ambient_temperature      149.98
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.942
_reflns_Friedel_fraction_full    0.998
_reflns_Friedel_fraction_max     0.998
_reflns_number_gt                11532
_reflns_number_total             12297
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_refine_diff_density_max         1.843
_refine_diff_density_min         -2.915
_refine_diff_density_rms         0.282
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.51(2)
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.078
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     448
_refine_ls_number_reflns         12297
_refine_ls_number_restraints     67
_refine_ls_R_factor_all          0.0291
_refine_ls_R_factor_gt           0.0262
_refine_ls_restrained_S_all      1.075
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+52.3712P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0633
_refine_ls_wR_factor_ref         0.0652
_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.49(2)
 0.51(2)
2. Uiso/Uaniso restraints and constraints
: with sigma of 0.1 and sigma for terminal atoms of 0.2
Uanis(W11) \\sim Ueq: with sigma of 0.1 and sigma for terminal atoms of 0.2
Uanis(W1) \\sim Ueq, Uanis(W2) \\sim Ueq, Uanis(W3) \\sim Ueq, Uanis(W4) \\sim
Ueq, Uanis(W5) \\sim Ueq, Uanis(W6) \\sim Ueq, Uanis(W7) \\sim Ueq, Uanis(W8)
\\sim Ueq, Uanis(W9) \\sim Ueq, Uanis(W10) \\sim Ueq, Uanis(W11) \\sim Ueq:
with sigma of 0.2 and sigma for terminal atoms of 0.4
3. Others
 Fixed Sof: K4(0.5) K6(0.5) K8(0.5) K0A(0.5) Dy2(0.45) O0AA(0.75)
 Fixed Uiso: O20(0.02) O24(0.02) O33(0.02) O37(0.02) O38(0.02) C1(0.02)
 C2(0.02) C3(0.02) N1(0.02) C4(0.02) C5(0.02) C6(0.02) C7(0.02) O39(0.02)
 K4(0.02) K6(0.02) C8(0.02) O0AA(0.02)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.50483(12) 0.12935(6) 0.98392(10) 0.0069(3) Uani 1 1 d . U . . .
W2 W 0.06686(13) 0.13743(6) 1.00973(10) 0.0076(3) Uani 1 1 d . U . . .
W3 W 0.13772(4) 0.21916(10) 0.64162(3) 0.00908(10) Uani 1 1 d . U . . .
W4 W -0.04032(13) 0.13503(6) 0.75950(10) 0.0083(3) Uani 1 1 d . U . . .
W5 W -0.04107(13) 0.30260(6) 0.75932(10) 0.0074(3) Uani 1 1 d . U . . .
W6 W 0.06688(13) 0.30014(6) 1.00981(10) 0.0072(3) Uani 1 1 d . U . . .
W7 W 0.50474(12) 0.30902(6) 0.98400(10) 0.0084(3) Uani 1 1 d . U . . .
W8 W 0.25049(13) 0.39271(6) 0.87122(10) 0.0082(3) Uani 1 1 d . U . . .
W9 W 0.43127(13) 0.12677(6) 0.75609(10) 0.0083(3) Uani 1 1 d . U . . .
W10 W 0.43071(13) 0.31146(6) 0.75582(10) 0.0095(3) Uani 1 1 d . U . . .
Dy1 Dy 0.35679(5) 0.21880(11) 1.16682(3) 0.00851(11) Uani 1 1 d . . . . .
W11 W 0.25053(14) 0.04527(6) 0.87138(10) 0.0082(3) Uani 1 1 d . U . . .
Si1 Si 0.2342(3) 0.2179(7) 0.87453(19) 0.0055(6) Uiso 1 1 d . U . . .
O1 O 0.1720(7) 0.2194(15) 0.9597(5) 0.0052(14) Uiso 1 1 d . . . . .
O2 O -0.0285(7) 0.2219(12) 1.0189(5) 0.0080(18) Uiso 1 1 d . . . . .
O3 O 0.1708(19) 0.3589(10) 0.9557(14) 0.011(5) Uiso 1 1 d . . . . .
O4 O 0.4772(7) 0.2160(13) 0.7537(5) 0.0107(19) Uiso 1 1 d . . . . .
O5 O -0.039(2) 0.2985(11) 0.8797(15) 0.012(6) Uiso 1 1 d . . . . .
O6 O -0.0367(19) 0.1407(10) 0.8761(14) 0.008(5) Uiso 1 1 d . . . . .
O7 O 0.1694(17) 0.0770(9) 0.9630(12) 0.006(5) Uiso 1 1 d . . . . .
O8 O -0.0395(17) 0.0822(9) 1.0384(13) 0.006(5) Uiso 1 1 d . . . . .
O9 O 0.5496(7) 0.2199(16) 0.9653(5) 0.0101(16) Uiso 1 1 d . . . . .
O10 O 0.1157(7) 0.2211(13) 0.7862(5) 0.0081(17) Uiso 1 1 d . . . . .
O11 O 0.2620(18) 0.2812(10) 0.6799(14) 0.011(5) Uiso 1 1 d . . . . .
O12 O -0.1659(18) 0.3528(9) 0.7157(13) 0.013(5) Uiso 1 1 d . . . . .
O13 O -0.1333(7) 0.2201(15) 0.7380(5) 0.0098(16) Uiso 1 1 d . . . . .
O14 O 0.5139(16) 0.3437(8) 0.6822(12) 0.007(4) Uiso 1 1 d . . . . .
O15 O 0.1011(19) 0.3606(10) 0.7846(14) 0.009(5) Uiso 1 1 d . . . . .
O16 O 0.103(2) 0.0740(10) 0.7901(14) 0.011(5) Uiso 1 1 d . . . . .
O17 O 0.3245(17) 0.2860(9) 0.8729(13) 0.001(4) Uiso 1 1 d . . . . .
O18 O 0.5502(18) 0.1121(11) 0.8608(14) 0.012(5) Uiso 1 1 d . . . . .
O19 O 0.6545(17) 0.1013(9) 1.0386(12) 0.010(4) Uiso 1 1 d . . . . .
O20 O 0.221(2) -0.0378(11) 0.8708(14) 0.020 Uiso 1 1 d . . . . .
O21 O 0.4985(18) 0.0970(10) 0.6763(13) 0.018(5) Uiso 1 1 d . . . . .
O22 O 0.2152(16) 0.4755(9) 0.8787(11) 0.006(2) Uiso 1 1 d . . . . .
O23 O 0.322(2) 0.1550(11) 0.8718(17) 0.017(6) Uiso 1 1 d . . . . .
O24 O 0.411(2) 0.0485(12) 0.9517(17) 0.020 Uiso 1 1 d . . . . .
O25 O 0.2360(8) 0.2178(16) 1.2815(6) 0.0159(18) Uiso 1 1 d . . . . .
O26 O 0.3350(16) 0.0456(8) 0.7804(12) 0.010(4) Uiso 1 1 d . . . . .
O27 O 0.3467(16) 0.3887(8) 0.7747(12) 0.008(4) Uiso 1 1 d . . . . .
O28 O 0.4198(17) 0.3061(9) 1.2652(13) 0.006(2) Uiso 1 1 d . . . . .
O29 O 0.4173(16) 0.2885(8) 1.0674(12) 0.007(4) Uiso 1 1 d . . . . .
O30 O 0.010(2) 0.2853(11) 0.6488(15) 0.010(5) Uiso 1 1 d . . . . .
O31 O 0.4296(17) 0.1515(9) 1.0643(13) 0.013(5) Uiso 1 1 d . . . . .
O32 O 0.1314(8) 0.2240(10) 0.5301(6) 0.014(2) Uiso 1 1 d . . . . .
O33 O 0.427(2) 0.1298(12) 1.2650(16) 0.020 Uiso 1 1 d . . . . .
O34 O 0.1714(19) 0.1487(10) 1.1124(15) 0.018(5) Uiso 1 1 d . . . . .
O35 O 0.1847(16) 0.2894(8) 1.1115(12) 0.003(4) Uiso 1 1 d . . . . .
O36 O 0.5913(8) 0.2222(15) 1.2122(6) 0.020(2) Uiso 1 1 d . . . . .
O37 O 0.4480(19) 0.0440(10) 1.3552(14) 0.020 Uiso 1 1 d . . . . .
O38 O 0.167(2) 0.0936(12) 1.3189(16) 0.020 Uiso 1 1 d . . . . .
C1 C 0.185(3) -0.0559(14) 1.0899(19) 0.020 Uiso 1 1 d . . . . .
C2 C 0.378(3) 0.0007(16) 1.153(2) 0.020 Uiso 1 1 d . . . . .
C3 C 0.404(3) 0.0725(18) 1.285(2) 0.020 Uiso 1 1 d . . . . .
N1 N 0.3068(18) -0.0444(10) 1.0887(14) 0.020 Uiso 1 1 d . . . . .
C4 C 0.197(3) 0.0142(18) 1.206(2) 0.020 Uiso 1 1 d . . . . .
C5 C 0.325(3) 0.0296(17) 1.211(2) 0.020 Uiso 1 1 d . . . . .
C6 C 0.110(3) 0.0489(17) 1.265(3) 0.020 Uiso 1 1 d . . . . .
C7 C 0.139(3) -0.0311(13) 1.141(2) 0.020 Uiso 1 1 d . . . . .
O39 O -0.0029(19) 0.0332(9) 1.2593(13) 0.020 Uiso 1 1 d . . . . .
K1 K 0.7423(2) 0.2176(6) 0.87981(17) 0.0161(6) Uiso 1 1 d . . . . .
K4 K 0.1635(15) 0.5860(7) 0.8493(12) 0.020 Uiso 0.5 1 d . . P . .
O40 O 0.2637(18) -0.1730(9) 0.7344(13) 0.020(5) Uiso 1 1 d . . . . .
O41 O 0.1536(10) -0.2856(15) 0.8460(7) 0.034(3) Uiso 1 1 d . . . . .
O42 O 0.689(2) 0.0009(12) 1.5884(16) 0.025(6) Uiso 1 1 d . . . . .
O43 O 0.6835(19) 0.4350(10) 0.5812(14) 0.012(5) Uiso 1 1 d . . . . .
O44 O 0.3655(9) 0.2135(12) 1.4638(7) 0.028(3) Uiso 1 1 d . . . . .
O45 O 0.6346(9) 0.2157(15) 0.6149(6) 0.025(2) Uiso 1 1 d . . . . .
O46 O 0.8486(17) 0.1026(9) 1.4934(12) 0.034(5) Uiso 1 1 d . . . . .
O47 O 0.2578(16) 0.0694(8) 1.5049(11) 0.019(4) Uiso 1 1 d . . . . .
O48 O 0.2293(18) 0.3723(10) 0.5017(13) 0.037(6) Uiso 1 1 d . . . . .
O49 O 0.6581(16) 0.2316(12) 0.4178(12) 0.069(6) Uiso 1 1 d . . . . .
K5 K 0.3236(6) -0.0542(3) 0.6527(4) 0.0541(14) Uiso 1 1 d . . . . .
K6 K 0.8268(14) -0.0158(8) 1.4883(11) 0.020 Uiso 0.5 1 d . . P . .
K7 K 0.1742(11) -0.0451(6) 1.5122(8) 0.0502(13) Uiso 1 1 d . . . . .
O50 O -0.049(2) 0.3552(11) 1.0379(15) 0.013(5) Uiso 1 1 d . . . . .
O51 O 0.2723(18) 0.1527(9) 0.6826(13) 0.010(5) Uiso 1 1 d . . . . .
O52 O 0.4156(16) 0.3930(9) 0.9546(13) 0.003(2) Uiso 1 1 d . . . . .
O53 O 0.5506(17) 0.3201(10) 0.8616(13) 0.007(4) Uiso 1 1 d . . . . .
O54 O 0.011(2) 0.1525(12) 0.6460(16) 0.012(5) Uiso 1 1 d . . . . .
O55 O -0.1672(19) 0.0798(9) 0.7217(14) 0.013(5) Uiso 1 1 d . . . . .
O56 O 0.6492(18) 0.3386(10) 1.0469(13) 0.014(5) Uiso 1 1 d . . . . .
K8 K 0.0409(8) -0.2138(4) 0.6330(6) 0.0287(18) Uiso 0.5 1 d . . P A .
K9 K 0.1655(11) -0.1474(5) 0.8470(8) 0.0454(13) Uiso 1 1 d . . . . .
O57 O 0.9728(17) -0.0481(9) 1.3976(12) 0.018(5) Uiso 1 1 d . . . . .
O58 O 1.0301(18) -0.0037(10) 1.6068(13) 0.022(5) Uiso 1 1 d . . . . .
O59 O -0.0020(17) -0.0881(8) 0.7484(11) 0.013(3) Uiso 1 1 d . . . . .
O60 O 0.1767(15) -0.1730(8) 1.5033(10) 0.019(4) Uiso 1 1 d . . . . .
O61 O 0.2720(19) 0.6025(10) 0.7314(14) 0.025(5) Uiso 1 1 d . . . . .
O62 O -0.168(2) -0.1554(10) 0.6866(14) 0.011(2) Uiso 1 1 d . . . . .
O63 O 0.4369(15) 0.3913(8) 1.3608(12) 0.010(3) Uiso 1 1 d . . . . .
C8 C 0.396(3) 0.3641(18) 1.285(2) 0.020 Uiso 1 1 d . . . . .
C9 C 0.391(2) 0.4363(14) 1.153(2) 0.013(4) Uiso 1 1 d . . . . .
C10 C 0.318(2) 0.4082(13) 1.2145(19) 0.004(3) Uiso 1 1 d . . . . .
C11 C 0.189(2) 0.4220(14) 1.2075(19) 0.006(3) Uiso 1 1 d . . . . .
N2 N 0.1995(15) 0.4954(9) 1.0835(12) 0.002(3) Uiso 1 1 d . . . . .
C12 C 0.1239(19) 0.4651(10) 1.1446(16) 0.006(3) Uiso 1 1 d . . . . .
C13 C 0.3329(17) 0.4785(10) 1.0885(15) 0.013(4) Uiso 1 1 d . . . . .
K0A K 0.5682(9) 0.3225(4) 1.5076(6) 0.0177(18) Uiso 0.5 1 d . . P . .
Dy2 Dy 0.5283(3) 0.11122(15) 1.5109(2) 0.0475(8) Uiso 0.45 1 d . . P . .
O0AA O -0.116(3) -0.1098(15) 0.737(2) 0.020 Uiso 0.75 1 d . . P A 1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O9 1.93(3) . ?
W1 O18 2.10(2) . ?
W1 O19 1.723(19) . ?
W1 O23 2.35(2) . ?
W1 O24 1.92(2) . ?
W1 O31 1.692(19) . ?
W1 K1 3.755(6) . ?
W1 K4 3.970(17) 2_647 ?
W2 O1 2.23(2) . ?
W2 O2 2.01(2) . ?
W2 O6 2.11(2) . ?
W2 O7 1.890(18) . ?
W2 O8 1.721(18) . ?
W2 O34 1.73(2) . ?
W2 K1 3.932(6) 1_455 ?
W2 K4 3.793(15) 2_547 ?
W3 O10 2.308(7) . ?
W3 O11 1.821(19) . ?
W3 O30 1.93(2) . ?
W3 O32 1.718(8) . ?
W3 O51 1.960(19) . ?
W3 O54 1.92(2) . ?
W4 O6 1.80(2) . ?
W4 O10 2.37(2) . ?
W4 O13 1.97(3) . ?
W4 O16 1.93(2) . ?
W4 K1 3.693(6) 1_455 ?
W4 O54 1.99(2) . ?
W4 O55 1.75(2) . ?
W5 O5 1.86(2) . ?
W5 O10 2.31(2) . ?
W5 O12 1.69(2) . ?
W5 O13 1.92(3) . ?
W5 O15 1.88(2) . ?
W5 O30 1.95(2) . ?
W5 K1 3.710(6) 1_455 ?
W6 O1 2.22(2) . ?
W6 O2 1.90(2) . ?
W6 O3 1.94(2) . ?
W6 O5 2.07(2) . ?
W6 O35 1.789(18) . ?
W6 K1 3.951(6) 1_455 ?
W6 O50 1.79(2) . ?
W6 K9 3.840(11) 2_557 ?
W7 O9 1.90(3) . ?
W7 O17 2.314(19) . ?
W7 O29 1.809(17) . ?
W7 K1 3.786(7) . ?
W7 O52 1.944(18) . ?
W7 O53 2.078(19) . ?
W7 O56 1.73(2) . ?
W7 K9 3.971(12) 2_657 ?
W8 O3 1.850(19) . ?
W8 O15 1.94(2) . ?
W8 O17 2.292(18) . ?
W8 O22 1.721(17) . ?
W8 O27 2.002(17) . ?
W8 K4 4.003(15) . ?
W8 O52 1.930(18) . ?
W9 O4 1.87(3) . ?
W9 O18 1.84(2) . ?
W9 O21 1.68(2) . ?
W9 O23 2.42(2) . ?
W9 O26 2.014(16) . ?
W9 K1 3.890(6) . ?
W9 K5 4.044(6) . ?
W9 O51 1.887(19) . ?
W10 O4 1.99(3) . ?
W10 O11 2.006(19) . ?
W10 O14 1.727(16) . ?
W10 O17 2.407(19) . ?
W10 O27 1.855(16) . ?
W10 K1 3.924(6) . ?
W10 O53 1.84(2) . ?
Dy1 O25 2.426(8) . ?
Dy1 O28 2.324(19) . ?
Dy1 O29 2.287(17) . ?
Dy1 O31 2.354(19) . ?
Dy1 O33 2.36(2) . ?
Dy1 O34 2.42(2) . ?
Dy1 O35 2.327(16) . ?
Dy1 O36 2.440(9) . ?
W11 O7 1.936(18) . ?
W11 O16 1.87(2) . ?
W11 O20 1.70(2) . ?
W11 O23 2.34(2) . ?
W11 O24 1.87(2) . ?
W11 O26 1.841(17) . ?
W11 K9 3.987(11) . ?
Si1 O1 1.609(7) . ?
Si1 O10 1.637(8) . ?
Si1 O17 1.68(2) . ?
Si1 O23 1.59(3) . ?
O2 K1 2.865(8) 1_455 ?
O4 K1 3.047(8) . ?
O5 K1 2.85(2) 1_455 ?
O6 K1 2.83(2) 1_455 ?
O8 K4 2.42(2) 2_547 ?
O9 K1 2.693(8) . ?
O13 K1 2.818(8) 1_455 ?
O14 K0A 2.926(19) 1_554 ?
O18 K1 2.92(2) . ?
O19 K4 2.31(3) 2_647 ?
O20 K9 2.30(2) . ?
O21 Dy2 2.67(2) 1_554 ?
O22 K4 2.32(2) . ?
O26 K5 2.806(18) . ?
O28 C8 1.25(4) . ?
O32 K8 3.033(15) 2_556 ?
O33 C3 1.23(4) . ?
O37 C3 1.23(4) . ?
O37 Dy2 2.73(2) . ?
O38 C6 1.28(4) . ?
C1 N1 1.32(3) . ?
C1 C7 1.14(4) . ?
C2 N1 1.43(4) . ?
C2 C5 1.30(4) . ?
C3 C5 1.52(5) . ?
C4 C5 1.39(5) . ?
C4 C6 1.61(4) . ?
C4 C7 1.39(5) . ?
C6 O39 1.23(4) . ?
C6 K4 3.14(4) 2_547 ?
O39 K4 2.36(3) 2_547 ?
K1 W4 3.693(6) 1_655 ?
K1 W5 3.710(6) 1_655 ?
K1 O2 2.865(8) 1_655 ?
K1 O5 2.85(2) 1_655 ?
K1 O6 2.83(2) 1_655 ?
K1 O13 2.819(8) 1_655 ?
K1 O53 2.88(2) . ?
K4 W1 3.970(17) 2_657 ?
K4 W2 3.793(15) 2_557 ?
K4 O8 2.42(2) 2_557 ?
K4 O19 2.31(3) 2_657 ?
K4 C6 3.14(4) 2_557 ?
K4 O39 2.36(3) 2_557 ?
K4 K1 4.873(18) 2_657 ?
K4 O41 2.59(3) 1_565 ?
K4 O61 2.40(2) . ?
O40 K5 2.85(2) . ?
O40 K8 2.66(2) . ?
O40 K9 2.29(2) . ?
O41 K4 2.59(3) 1_545 ?
O41 K9 2.79(3) . ?
O42 K6 2.39(3) . ?
O42 Dy2 2.90(2) . ?
O43 K7 2.36(2) 2_657 ?
O43 K0A 2.71(2) 1_554 ?
O44 K0A 3.05(2) . ?
O44 Dy2 2.69(2) . ?
O45 K0A 2.71(3) 1_554 ?
O45 Dy2 2.74(2) 1_554 ?
O46 K6 2.40(2) . ?
O47 K5 3.348(17) 1_556 ?
O47 K7 2.489(19) . ?
O48 K6 2.35(2) 2_657 ?
O49 K0A 2.61(2) 1_554 ?
K5 O47 3.348(17) 1_554 ?
K5 K7 2.391(14) 1_554 ?
K5 K8 4.376(10) . ?
K5 K9 4.220(13) . ?
K5 O58 3.21(2) 1_454 ?
K5 O63 2.835(16) 2_647 ?
K5 C8 3.36(4) 2_647 ?
K5 K0A 3.877(10) 2_647 ?
K6 O48 2.35(3) 2_647 ?
K6 K7 3.690(7) 1_655 ?
K6 K8 4.882(18) 1_656 ?
K6 O57 2.42(2) . ?
K6 O58 2.51(2) . ?
K6 Dy2 4.167(15) . ?
K7 O43 2.36(2) 2_647 ?
K7 K5 2.391(14) 1_556 ?
K7 K6 3.690(8) 1_455 ?
K7 K8 4.283(15) 1_556 ?
K7 O57 2.45(2) 1_455 ?
K7 O58 2.50(2) 1_455 ?
K7 O60 2.58(2) . ?
K7 K0A 3.896(14) 2_648 ?
O50 K9 2.40(2) 2_557 ?
O56 K9 2.28(2) 2_657 ?
K8 O32 3.033(15) 2_546 ?
K8 K6 4.882(18) 1_454 ?
K8 K7 4.283(15) 1_554 ?
K8 K9 3.541(15) . ?
K8 O59 3.198(17) . ?
K8 O60 2.857(17) 1_554 ?
K8 O62 2.81(2) . ?
K8 O0AA 3.32(3) . ?
K9 W6 3.840(11) 2_547 ?
K9 W7 3.971(12) 2_647 ?
K9 O50 2.40(2) 2_547 ?
K9 O56 2.28(2) 2_647 ?
K9 O59 2.39(2) . ?
K9 O0AA 3.18(3) . ?
O57 K7 2.45(2) 1_655 ?
O58 K5 3.21(2) 1_656 ?
O58 K7 2.50(2) 1_655 ?
O59 O0AA 1.26(3) . ?
O60 K8 2.857(17) 1_556 ?
O60 K0A 2.770(18) 2_648 ?
O62 O0AA 1.25(4) . ?
O63 K5 2.835(16) 2_657 ?
O63 C8 1.28(4) . ?
O63 K0A 2.76(2) . ?
C8 K5 3.36(4) 2_657 ?
C8 C10 1.50(5) . ?
C9 C10 1.48(3) . ?
C9 C13 1.35(4) . ?
C10 C11 1.39(3) . ?
C11 C12 1.37(4) . ?
C11 O0AA 1.44(4) 2_557 ?
N2 C12 1.51(2) . ?
N2 C13 1.45(2) . ?
K0A O14 2.926(19) 1_556 ?
K0A O43 2.71(2) 1_556 ?
K0A O45 2.71(3) 1_556 ?
K0A O49 2.61(2) 1_556 ?
K0A K5 3.877(10) 2_657 ?
K0A K7 3.896(15) 2_658 ?
K0A O60 2.770(18) 2_658 ?
K0A Dy2 4.283(7) . ?
Dy2 O21 2.67(2) 1_556 ?
Dy2 O45 2.74(2) 1_556 ?
O0AA C11 1.44(4) 2_547 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O9 W1 O18 84.5(6) . . ?
O9 W1 O23 82.7(6) . . ?
O9 W1 K1 43.1(4) . . ?
O9 W1 K4 95.2(3) . 2_647 ?
O18 W1 O23 72.0(8) . . ?
O18 W1 K1 50.9(6) . . ?
O18 W1 K4 101.3(6) . 2_647 ?
O19 W1 O9 98.7(7) . . ?
O19 W1 O18 90.6(8) . . ?
O19 W1 O23 162.4(8) . . ?
O19 W1 O24 102.6(10) . . ?
O19 W1 K1 74.0(6) . . ?
O19 W1 K4 11.6(6) . 2_647 ?
O23 W1 K1 96.1(6) . . ?
O23 W1 K4 173.2(6) . 2_647 ?
O24 W1 O9 154.1(8) . . ?
O24 W1 O18 80.7(9) . . ?
O24 W1 O23 72.6(9) . . ?
O24 W1 K1 130.9(7) . . ?
O24 W1 K4 108.4(7) . 2_647 ?
O31 W1 O9 92.1(7) . . ?
O31 W1 O18 163.8(9) . . ?
O31 W1 O19 105.6(9) . . ?
O31 W1 O23 91.9(9) . . ?
O31 W1 O24 96.3(9) . . ?
O31 W1 K1 132.4(6) . . ?
O31 W1 K4 94.7(7) . 2_647 ?
K1 W1 K4 78.2(2) . 2_647 ?
O1 W2 K1 88.4(4) . 1_455 ?
O1 W2 K4 147.9(6) . 2_547 ?
O2 W2 O1 72.6(6) . . ?
O2 W2 O6 83.3(6) . . ?
O2 W2 K1 44.4(3) . 1_455 ?
O2 W2 K4 77.5(4) . 2_547 ?
O6 W2 O1 80.1(6) . . ?
O6 W2 K1 44.3(5) . 1_455 ?
O6 W2 K4 108.1(6) . 2_547 ?
O7 W2 O1 87.8(8) . . ?
O7 W2 O2 157.3(6) . . ?
O7 W2 O6 82.1(8) . . ?
O7 W2 K1 126.1(6) . 1_455 ?
O7 W2 K4 123.7(6) . 2_547 ?
O8 W2 O1 169.3(7) . . ?
O8 W2 O2 98.9(7) . . ?
O8 W2 O6 92.7(9) . . ?
O8 W2 O7 99.0(8) . . ?
O8 W2 O34 99.8(9) . . ?
O8 W2 K1 80.9(7) . 1_455 ?
O8 W2 K4 28.3(7) . 2_547 ?
O34 W2 O1 87.3(7) . . ?
O34 W2 O2 93.1(7) . . ?
O34 W2 O6 167.4(9) . . ?
O34 W2 O7 97.4(9) . . ?
O34 W2 K1 136.1(6) . 1_455 ?
O34 W2 K4 82.7(7) . 2_547 ?
K4 W2 K1 78.2(3) 2_547 1_455 ?
O11 W3 O10 84.4(8) . . ?
O11 W3 O30 88.7(9) . . ?
O11 W3 O51 86.6(3) . . ?
O11 W3 O54 159.5(10) . . ?
O30 W3 O10 72.6(8) . . ?
O30 W3 O51 158.3(9) . . ?
O32 W3 O10 171.1(5) . . ?
O32 W3 O11 98.4(8) . . ?
O32 W3 O30 98.9(9) . . ?
O32 W3 O51 102.7(8) . . ?
O32 W3 O54 102.2(9) . . ?
O51 W3 O10 85.9(8) . . ?
O54 W3 O10 75.3(9) . . ?
O54 W3 O30 88.1(3) . . ?
O54 W3 O51 88.9(9) . . ?
O6 W4 O10 85.8(7) . . ?
O6 W4 O13 90.4(7) . . ?
O6 W4 O16 87.8(9) . . ?
O6 W4 K1 48.3(6) . 1_455 ?
O6 W4 O54 158.2(9) . . ?
O10 W4 K1 94.6(4) . 1_455 ?
O13 W4 O10 72.5(7) . . ?
O13 W4 K1 48.9(3) . 1_455 ?
O13 W4 O54 85.8(7) . . ?
O16 W4 O10 86.5(8) . . ?
O16 W4 O13 159.0(8) . . ?
O16 W4 K1 135.8(6) . 1_455 ?
O16 W4 O54 88.1(9) . . ?
O54 W4 O10 72.6(7) . . ?
O54 W4 K1 134.3(7) . 1_455 ?
O55 W4 O6 102.3(9) . . ?
O55 W4 O10 169.3(7) . . ?
O55 W4 O13 100.2(8) . . ?
O55 W4 O16 100.6(9) . . ?
O55 W4 K1 85.9(6) . 1_455 ?
O55 W4 O54 99.5(9) . . ?
O5 W5 O10 87.0(7) . . ?
O5 W5 O13 91.2(7) . . ?
O5 W5 O15 89.8(9) . . ?
O5 W5 O30 159.0(9) . . ?
O5 W5 K1 48.7(7) . 1_455 ?
O10 W5 K1 95.2(4) . 1_455 ?
O12 W5 O5 104.7(9) . . ?
O12 W5 O10 166.1(7) . . ?
O12 W5 O13 97.2(8) . . ?
O12 W5 O15 103.6(9) . . ?
O12 W5 O30 96.3(9) . . ?
O12 W5 K1 87.3(6) . 1_455 ?
O13 W5 O10 74.7(7) . . ?
O13 W5 O30 86.0(7) . . ?
O13 W5 K1 48.1(3) . 1_455 ?
O15 W5 O10 83.6(8) . . ?
O15 W5 O13 158.3(8) . . ?
O15 W5 O30 85.4(9) . . ?
O15 W5 K1 138.4(6) . 1_455 ?
O30 W5 O10 72.2(7) . . ?
O30 W5 K1 134.0(7) . 1_455 ?
O1 W6 K1 88.1(4) . 1_455 ?
O1 W6 K9 148.4(6) . 2_557 ?
O2 W6 O1 74.9(7) . . ?
O2 W6 O3 155.2(7) . . ?
O2 W6 O5 83.0(6) . . ?
O2 W6 K1 42.8(3) . 1_455 ?
O2 W6 K9 76.0(4) . 2_557 ?
O3 W6 O1 84.9(8) . . ?
O3 W6 O5 80.1(9) . . ?
O3 W6 K1 123.9(6) . 1_455 ?
O3 W6 K9 126.3(6) . 2_557 ?
O5 W6 O1 81.6(6) . . ?
O5 W6 K1 43.9(6) . 1_455 ?
O5 W6 K9 106.6(6) . 2_557 ?
O35 W6 O1 84.9(5) . . ?
O35 W6 O2 96.6(6) . . ?
O35 W6 O3 95.6(8) . . ?
O35 W6 O5 166.1(8) . . ?
O35 W6 K1 139.0(5) . 1_455 ?
O35 W6 O50 104.3(9) . . ?
O35 W6 K9 86.6(5) . 2_557 ?
O50 W6 O1 167.1(8) . . ?
O50 W6 O2 94.8(8) . . ?
O50 W6 O3 103.0(9) . . ?
O50 W6 O5 89.6(9) . . ?
O50 W6 K1 79.0(7) . 1_455 ?
O50 W6 K9 27.5(7) . 2_557 ?
K9 W6 K1 78.6(2) 2_557 1_455 ?
O9 W7 O17 83.8(5) . . ?
O9 W7 K1 42.0(4) . . ?
O9 W7 O52 156.2(6) . . ?
O9 W7 O53 80.9(6) . . ?
O9 W7 K9 95.4(3) . 2_657 ?
O17 W7 K1 96.2(5) . . ?
O17 W7 K9 173.5(5) . 2_657 ?
O29 W7 O9 94.7(7) . . ?
O29 W7 O17 90.4(7) . . ?
O29 W7 K1 134.5(6) . . ?
O29 W7 O52 93.5(8) . . ?
O29 W7 O53 161.2(8) . . ?
O29 W7 K9 96.0(6) . 2_657 ?
K1 W7 K9 79.04(17) . 2_657 ?
O52 W7 O17 73.9(7) . . ?
O52 W7 K1 131.6(6) . . ?
O52 W7 O53 84.2(8) . . ?
O52 W7 K9 105.9(5) . 2_657 ?
O53 W7 O17 70.9(7) . . ?
O53 W7 K1 48.7(5) . . ?
O53 W7 K9 102.6(5) . 2_657 ?
O56 W7 O9 100.9(7) . . ?
O56 W7 O17 165.7(8) . . ?
O56 W7 O29 102.5(8) . . ?
O56 W7 K1 79.1(6) . . ?
O56 W7 O52 99.0(8) . . ?
O56 W7 O53 96.3(8) . . ?
O56 W7 K9 9.0(7) . 2_657 ?
O3 W8 O15 85.9(9) . . ?
O3 W8 O17 81.9(8) . . ?
O3 W8 O27 156.0(8) . . ?
O3 W8 K4 106.5(7) . . ?
O3 W8 O52 91.4(8) . . ?
O15 W8 O17 85.5(7) . . ?
O15 W8 O27 87.2(8) . . ?
O15 W8 K4 97.4(6) . . ?
O17 W8 K4 171.3(5) . . ?
O22 W8 O3 99.6(8) . . ?
O22 W8 O15 102.3(8) . . ?
O22 W8 O17 172.2(8) . . ?
O22 W8 O27 104.3(7) . . ?
O22 W8 K4 8.6(6) . . ?
O22 W8 O52 97.6(8) . . ?
O27 W8 O17 74.7(7) . . ?
O27 W8 K4 97.1(5) . . ?
O52 W8 O15 160.1(8) . . ?
O52 W8 O17 74.7(7) . . ?
O52 W8 O27 87.3(7) . . ?
O52 W8 K4 102.3(6) . . ?
O4 W9 O23 87.8(6) . . ?
O4 W9 O26 159.1(6) . . ?
O4 W9 K1 50.0(3) . . ?
O4 W9 K5 156.0(3) . . ?
O4 W9 O51 85.7(7) . . ?
O18 W9 O4 92.4(7) . . ?
O18 W9 O23 74.7(8) . . ?
O18 W9 O26 89.0(8) . . ?
O18 W9 K1 45.9(7) . . ?
O18 W9 K5 106.2(7) . . ?
O18 W9 O51 156.8(8) . . ?
O21 W9 O4 99.9(7) . . ?
O21 W9 O18 105.5(9) . . ?
O21 W9 O23 172.3(8) . . ?
O21 W9 O26 99.8(8) . . ?
O21 W9 K1 94.0(7) . . ?
O21 W9 K5 61.0(7) . . ?
O21 W9 O51 97.6(9) . . ?
O23 W9 K1 91.5(6) . . ?
O23 W9 K5 111.4(6) . . ?
O26 W9 O23 72.5(7) . . ?
O26 W9 K1 134.8(5) . . ?
O26 W9 K5 39.7(5) . . ?
K1 W9 K5 138.84(18) . . ?
O51 W9 O23 82.1(8) . . ?
O51 W9 O26 84.9(8) . . ?
O51 W9 K1 135.5(6) . . ?
O51 W9 K5 82.9(6) . . ?
O4 W10 O11 83.7(6) . . ?
O4 W10 O17 88.2(5) . . ?
O4 W10 K1 49.9(3) . . ?
O11 W10 O17 82.1(7) . . ?
O11 W10 K1 133.3(6) . . ?
O14 W10 O4 100.6(6) . . ?
O14 W10 O11 104.8(8) . . ?
O14 W10 O17 169.2(7) . . ?
O14 W10 O27 97.5(7) . . ?
O14 W10 K1 89.9(6) . . ?
O14 W10 O53 101.3(8) . . ?
O17 W10 K1 91.2(4) . . ?
O27 W10 O4 161.2(6) . . ?
O27 W10 O11 86.9(8) . . ?
O27 W10 O17 74.4(7) . . ?
O27 W10 K1 135.6(6) . . ?
O53 W10 O4 88.9(6) . . ?
O53 W10 O11 153.8(8) . . ?
O53 W10 O17 72.6(7) . . ?
O53 W10 O27 92.4(8) . . ?
O53 W10 K1 43.3(6) . . ?
O25 Dy1 O36 118.2(3) . . ?
O28 Dy1 O25 69.4(8) . . ?
O28 Dy1 O31 142.1(6) . . ?
O28 Dy1 O33 98.8(3) . . ?
O28 Dy1 O34 139.5(6) . . ?
O28 Dy1 O35 82.1(6) . . ?
O28 Dy1 O36 70.5(7) . . ?
O29 Dy1 O25 141.3(9) . . ?
O29 Dy1 O28 83.8(7) . . ?
O29 Dy1 O31 73.2(3) . . ?
O29 Dy1 O33 143.6(7) . . ?
O29 Dy1 O34 117.3(7) . . ?
O29 Dy1 O35 72.4(6) . . ?
O29 Dy1 O36 75.3(6) . . ?
O31 Dy1 O25 143.5(9) . . ?
O31 Dy1 O33 83.8(7) . . ?
O31 Dy1 O34 78.4(6) . . ?
O31 Dy1 O36 74.6(6) . . ?
O33 Dy1 O25 70.4(8) . . ?
O33 Dy1 O34 83.9(8) . . ?
O33 Dy1 O36 71.5(8) . . ?
O34 Dy1 O25 73.7(7) . . ?
O34 Dy1 O36 145.0(8) . . ?
O35 Dy1 O25 76.5(6) . . ?
O35 Dy1 O31 117.4(6) . . ?
O35 Dy1 O33 144.0(6) . . ?
O35 Dy1 O34 73.5(3) . . ?
O35 Dy1 O36 139.4(8) . . ?
O7 W11 O23 83.5(8) . . ?
O7 W11 K9 105.1(6) . . ?
O16 W11 O7 86.6(8) . . ?
O16 W11 O23 86.2(8) . . ?
O16 W11 O24 159.7(10) . . ?
O16 W11 K9 95.7(6) . . ?
O20 W11 O7 102.5(9) . . ?
O20 W11 O16 100.1(10) . . ?
O20 W11 O23 171.5(9) . . ?
O20 W11 O24 100.2(10) . . ?
O20 W11 O26 97.0(9) . . ?
O20 W11 K9 5.2(8) . . ?
O23 W11 K9 171.2(6) . . ?
O24 W11 O7 89.9(9) . . ?
O24 W11 O23 73.5(9) . . ?
O24 W11 K9 104.5(7) . . ?
O26 W11 O7 160.5(7) . . ?
O26 W11 O16 88.2(8) . . ?
O26 W11 O23 77.4(8) . . ?
O26 W11 O24 88.5(9) . . ?
O26 W11 K9 94.1(5) . . ?
O1 Si1 O10 107.4(4) . . ?
O1 Si1 O17 110.2(13) . . ?
O10 Si1 O17 107.0(12) . . ?
O23 Si1 O1 113.3(14) . . ?
O23 Si1 O10 110.9(13) . . ?
O23 Si1 O17 107.9(4) . . ?
W6 O1 W2 94.9(3) . . ?
Si1 O1 W2 127.4(15) . . ?
Si1 O1 W6 129.7(15) . . ?
W2 O2 K1 106.3(7) . 1_455 ?
W6 O2 W2 114.2(3) . . ?
W6 O2 K1 110.4(7) . 1_455 ?
W8 O3 W6 159.0(12) . . ?
W9 O4 W10 149.8(4) . . ?
W9 O4 K1 101.9(7) . . ?
W10 O4 K1 100.2(7) . . ?
W5 O5 W6 148.4(11) . . ?
W5 O5 K1 101.9(9) . 1_455 ?
W6 O5 K1 105.8(8) . 1_455 ?
W2 O6 K1 104.3(8) . 1_455 ?
W4 O6 W2 150.1(11) . . ?
W4 O6 K1 103.3(9) . 1_455 ?
W2 O7 W11 153.0(11) . . ?
W2 O8 K4 132.0(11) . 2_547 ?
W1 O9 K1 107.6(10) . . ?
W7 O9 W1 142.6(4) . . ?
W7 O9 K1 109.8(10) . . ?
W3 O10 W4 92.5(6) . . ?
W3 O10 W5 93.9(6) . . ?
W5 O10 W4 92.2(3) . . ?
Si1 O10 W3 125.4(4) . . ?
Si1 O10 W4 119.6(12) . . ?
Si1 O10 W5 124.4(12) . . ?
W3 O11 W10 152.6(12) . . ?
W4 O13 K1 99.4(8) . 1_455 ?
W5 O13 W4 120.4(4) . . ?
W5 O13 K1 101.3(8) . 1_455 ?
W10 O14 K0A 142.9(8) . 1_554 ?
W5 O15 W8 147.5(12) . . ?
W11 O16 W4 149.2(12) . . ?
W7 O17 W10 93.6(6) . . ?
W8 O17 W7 92.6(7) . . ?
W8 O17 W10 90.7(6) . . ?
Si1 O17 W7 122.3(10) . . ?
Si1 O17 W8 124.7(10) . . ?
Si1 O17 W10 123.9(10) . . ?
W1 O18 K1 95.2(7) . . ?
W9 O18 W1 121.2(10) . . ?
W9 O18 K1 107.3(9) . . ?
W1 O19 K4 159.8(11) . 2_647 ?
W11 O20 K9 171.0(13) . . ?
W9 O21 Dy2 146.6(10) . 1_554 ?
W8 O22 K4 165.0(10) . . ?
W1 O23 W9 92.1(8) . . ?
W11 O23 W1 90.5(8) . . ?
W11 O23 W9 89.3(8) . . ?
Si1 O23 W1 123.5(13) . . ?
Si1 O23 W9 126.6(13) . . ?
Si1 O23 W11 124.2(13) . . ?
W11 O24 W1 123.0(12) . . ?
W9 O26 K5 113.1(7) . . ?
W11 O26 W9 120.5(9) . . ?
W11 O26 K5 126.1(8) . . ?
W10 O27 W8 120.1(9) . . ?
C8 O28 Dy1 146(2) . . ?
W7 O29 Dy1 153.5(9) . . ?
W3 O30 W5 121.3(12) . . ?
W1 O31 Dy1 159.5(11) . . ?
W3 O32 K8 137.5(6) . 2_556 ?
C3 O33 Dy1 145(2) . . ?
W2 O34 Dy1 134.2(11) . . ?
W6 O35 Dy1 137.2(9) . . ?
C3 O37 Dy2 122(2) . . ?
C7 C1 N1 121(3) . . ?
C5 C2 N1 122(3) . . ?
O33 C3 C5 117(3) . . ?
O37 C3 O33 127(4) . . ?
O37 C3 C5 116(3) . . ?
C1 N1 C2 118(2) . . ?
C5 C4 C6 124(3) . . ?
C7 C4 C5 117(3) . . ?
C7 C4 C6 119(3) . . ?
C2 C5 C3 122(3) . . ?
C2 C5 C4 116(3) . . ?
C4 C5 C3 122(3) . . ?
O38 C6 C4 116(3) . . ?
O38 C6 K4 116(2) . 2_547 ?
C4 C6 K4 111(2) . 2_547 ?
O39 C6 O38 123(3) . . ?
O39 C6 C4 122(3) . . ?
O39 C6 K4 41.3(16) . 2_547 ?
C1 C7 C4 127(3) . . ?
C6 O39 K4 119(2) . 2_547 ?
W1 K1 W7 57.44(4) . . ?
W4 K1 W1 124.7(3) 1_655 . ?
W4 K1 W5 54.32(4) 1_655 1_655 ?
W4 K1 W7 174.99(17) 1_655 . ?
W5 K1 W1 175.37(11) 1_655 . ?
W5 K1 W7 123.2(3) 1_655 . ?
O2 K1 W1 103.6(3) 1_655 . ?
O2 K1 W4 82.3(3) 1_655 1_655 ?
O2 K1 W5 80.9(3) 1_655 1_655 ?
O2 K1 W7 101.8(3) 1_655 . ?
O2 K1 O4 171.5(2) 1_655 . ?
O2 K1 O18 123.7(7) 1_655 . ?
O2 K1 O53 121.2(6) 1_655 . ?
O4 K1 W1 69.6(3) . . ?
O4 K1 W4 105.7(3) . 1_655 ?
O4 K1 W5 106.1(3) . 1_655 ?
O4 K1 W7 70.4(3) . . ?
O5 K1 W1 155.1(5) 1_655 . ?
O5 K1 W4 69.3(4) 1_655 1_655 ?
O5 K1 W5 29.4(5) 1_655 1_655 ?
O5 K1 W7 110.6(5) 1_655 . ?
O5 K1 O2 54.9(6) 1_655 1_655 ?
O5 K1 O4 130.3(6) 1_655 . ?
O5 K1 O18 166.7(6) 1_655 . ?
O5 K1 O53 98.8(7) 1_655 . ?
O6 K1 W1 113.4(5) 1_655 . ?
O6 K1 W4 28.4(4) 1_655 1_655 ?
O6 K1 W5 67.9(4) 1_655 1_655 ?
O6 K1 W7 156.6(5) 1_655 . ?
O6 K1 O2 57.4(6) 1_655 1_655 ?
O6 K1 O4 129.5(6) 1_655 . ?
O6 K1 O5 68.1(2) 1_655 1_655 ?
O6 K1 O18 99.6(6) 1_655 . ?
O6 K1 O53 165.4(6) 1_655 . ?
O9 K1 W1 29.3(7) . . ?
O9 K1 W4 153.7(8) . 1_655 ?
O9 K1 W5 151.1(8) . 1_655 ?
O9 K1 W7 28.2(7) . . ?
O9 K1 O2 104.2(2) . 1_655 ?
O9 K1 O4 67.3(2) . . ?
O9 K1 O5 135.3(8) . 1_655 ?
O9 K1 O6 138.9(8) . 1_655 ?
O9 K1 O13 159.2(3) . 1_655 ?
O9 K1 O18 57.6(7) . . ?
O9 K1 O53 55.2(7) . . ?
O13 K1 W1 146.1(6) 1_655 . ?
O13 K1 W4 31.8(6) 1_655 1_655 ?
O13 K1 W5 30.5(6) 1_655 1_655 ?
O13 K1 W7 143.8(6) 1_655 . ?
O13 K1 O2 96.4(2) 1_655 1_655 ?
O13 K1 O4 92.0(2) 1_655 . ?
O13 K1 O5 57.0(6) 1_655 1_655 ?
O13 K1 O6 56.6(6) 1_655 1_655 ?
O13 K1 O18 112.3(7) 1_655 . ?
O13 K1 O53 111.3(7) 1_655 . ?
O18 K1 W1 33.9(4) . . ?
O18 K1 W4 97.4(5) . 1_655 ?
O18 K1 W5 142.2(4) . 1_655 ?
O18 K1 W7 82.7(4) . . ?
O18 K1 O4 53.2(6) . . ?
O53 K1 W1 81.2(4) . . ?
O53 K1 W4 142.2(4) . 1_655 ?
O53 K1 W5 97.5(5) . 1_655 ?
O53 K1 W7 32.9(4) . . ?
O53 K1 O4 53.8(6) . . ?
O53 K1 O18 92.6(2) . . ?
W1 K4 W8 90.3(3) 2_657 . ?
W1 K4 K1 48.95(19) 2_657 2_657 ?
W2 K4 W1 99.5(4) 2_557 2_657 ?
W2 K4 W8 112.7(4) 2_557 . ?
W2 K4 K1 52.2(2) 2_557 2_657 ?
W8 K4 K1 117.4(4) . 2_657 ?
O8 K4 W1 95.3(7) 2_557 2_657 ?
O8 K4 W2 19.7(5) 2_557 2_557 ?
O8 K4 W8 93.6(6) 2_557 . ?
O8 K4 C6 78.9(9) 2_557 2_557 ?
O8 K4 K1 55.6(6) 2_557 2_657 ?
O8 K4 O41 91.1(7) 2_557 1_565 ?
O19 K4 W1 8.6(5) 2_657 2_657 ?
O19 K4 W2 94.3(6) 2_657 2_557 ?
O19 K4 W8 85.9(7) 2_657 . ?
O19 K4 O8 88.2(8) 2_657 2_557 ?
O19 K4 O22 81.9(9) 2_657 . ?
O19 K4 C6 165.8(10) 2_657 2_557 ?
O19 K4 O39 160.6(10) 2_657 2_557 ?
O19 K4 K1 46.2(5) 2_657 2_657 ?
O19 K4 O41 84.5(7) 2_657 1_565 ?
O19 K4 O61 94.8(9) 2_657 . ?
O22 K4 W1 87.0(6) . 2_657 ?
O22 K4 W2 107.9(6) . 2_557 ?
O22 K4 W8 6.4(4) . . ?
O22 K4 O8 88.5(8) . 2_557 ?
O22 K4 C6 91.8(9) . 2_557 ?
O22 K4 O39 78.9(8) . 2_557 ?
O22 K4 K1 111.2(7) . 2_657 ?
O22 K4 O41 166.4(9) . 1_565 ?
O22 K4 O61 98.5(8) . . ?
C6 K4 W1 174.1(8) 2_557 2_657 ?
C6 K4 W2 75.5(7) 2_557 2_557 ?
C6 K4 W8 89.1(7) 2_557 . ?
C6 K4 K1 126.7(7) 2_557 2_657 ?
O39 K4 W1 162.8(7) 2_557 2_657 ?
O39 K4 W2 94.2(6) 2_557 2_557 ?
O39 K4 W8 74.8(6) 2_557 . ?
O39 K4 O8 94.0(8) 2_557 2_557 ?
O39 K4 C6 20.1(8) 2_557 2_557 ?
O39 K4 K1 146.2(7) 2_557 2_657 ?
O39 K4 O41 114.6(8) 2_557 1_565 ?
O39 K4 O61 85.3(9) 2_557 . ?
O41 K4 W1 79.6(5) 1_565 2_657 ?
O41 K4 W2 73.1(4) 1_565 2_557 ?
O41 K4 W8 169.2(6) 1_565 . ?
O41 K4 C6 101.4(9) 1_565 2_557 ?
O41 K4 K1 58.1(4) 1_565 2_657 ?
O61 K4 W1 87.2(6) . 2_657 ?
O61 K4 W2 153.0(8) . 2_557 ?
O61 K4 W8 93.2(6) . . ?
O61 K4 O8 172.7(10) . 2_557 ?
O61 K4 C6 98.7(10) . 2_557 ?
O61 K4 K1 122.7(7) . 2_657 ?
O61 K4 O41 82.6(7) . 1_565 ?
K8 O40 K5 105.0(7) . . ?
K9 O40 K5 109.7(8) . . ?
K9 O40 K8 90.9(7) . . ?
K4 O41 K9 175.2(5) 1_545 . ?
K6 O42 Dy2 103.5(9) . . ?
K7 O43 K0A 100.3(8) 2_657 1_554 ?
Dy2 O44 K0A 96.4(3) . . ?
K0A O45 Dy2 103.6(4) 1_554 1_554 ?
K7 O47 K5 45.5(4) . 1_556 ?
W9 K5 K8 145.09(19) . . ?
W9 K5 K9 104.0(2) . . ?
O26 K5 W9 27.3(3) . . ?
O26 K5 O40 105.5(5) . . ?
O26 K5 O47 85.3(5) . 1_554 ?
O26 K5 K8 119.6(4) . . ?
O26 K5 K9 77.0(4) . . ?
O26 K5 O58 79.1(5) . 1_454 ?
O26 K5 O63 115.9(5) . 2_647 ?
O26 K5 C8 105.0(8) . 2_647 ?
O26 K5 K0A 160.4(4) . 2_647 ?
O40 K5 W9 130.9(4) . . ?
O40 K5 O47 153.7(5) . 1_554 ?
O40 K5 K8 36.0(4) . . ?
O40 K5 K9 30.8(4) . . ?
O40 K5 O58 93.3(5) . 1_454 ?
O40 K5 C8 74.7(7) . 2_647 ?
O40 K5 K0A 82.9(4) . 2_647 ?
O47 K5 W9 66.1(3) 1_554 . ?
O47 K5 K8 117.9(4) 1_554 . ?
O47 K5 K9 139.9(4) 1_554 . ?
O47 K5 C8 126.4(6) 1_554 2_647 ?
O47 K5 K0A 94.9(3) 1_554 2_647 ?
K7 K5 W9 111.2(3) 1_554 . ?
K7 K5 O26 120.0(5) 1_554 . ?
K7 K5 O40 107.3(5) 1_554 . ?
K7 K5 O47 47.9(4) 1_554 1_554 ?
K7 K5 K8 71.8(3) 1_554 . ?
K7 K5 K9 113.1(4) 1_554 . ?
K7 K5 O58 50.4(4) 1_554 1_454 ?
K7 K5 O63 112.7(5) 1_554 2_647 ?
K7 K5 C8 131.4(7) 1_554 2_647 ?
K7 K5 K0A 72.5(3) 1_554 2_647 ?
K9 K5 K8 48.6(2) . . ?
O58 K5 W9 88.6(4) 1_454 . ?
O58 K5 O47 64.7(5) 1_454 1_554 ?
O58 K5 K8 66.2(4) 1_454 . ?
O58 K5 K9 76.6(4) 1_454 . ?
O58 K5 C8 168.0(7) 1_454 2_647 ?
O58 K5 K0A 118.8(4) 1_454 2_647 ?
O63 K5 W9 101.5(4) 2_647 . ?
O63 K5 O40 90.3(5) 2_647 . ?
O63 K5 O47 106.8(5) 2_647 1_554 ?
O63 K5 K8 109.2(4) 2_647 . ?
O63 K5 K9 113.3(4) 2_647 . ?
O63 K5 O58 163.0(6) 2_647 1_454 ?
O63 K5 C8 21.7(7) 2_647 2_647 ?
O63 K5 K0A 45.3(4) 2_647 2_647 ?
C8 K5 W9 100.1(7) 2_647 . ?
C8 K5 K8 102.3(6) 2_647 . ?
C8 K5 K9 93.1(6) 2_647 . ?
C8 K5 K0A 59.4(7) 2_647 2_647 ?
K0A K5 W9 137.2(2) 2_647 . ?
K0A K5 K8 77.6(2) 2_647 . ?
K0A K5 K9 113.5(2) 2_647 . ?
O42 K6 O46 84.7(9) . . ?
O42 K6 K7 135.3(7) . 1_655 ?
O42 K6 K8 96.3(7) . 1_656 ?
O42 K6 O57 171.7(10) . . ?
O42 K6 O58 93.9(9) . . ?
O42 K6 Dy2 42.5(6) . . ?
O46 K6 K7 93.9(6) . 1_655 ?
O46 K6 K8 140.1(7) . 1_656 ?
O46 K6 O57 102.5(8) . . ?
O46 K6 O58 79.5(8) . . ?
O46 K6 Dy2 57.0(5) . . ?
O48 K6 O42 83.6(9) 2_647 . ?
O48 K6 O46 168.0(10) 2_647 . ?
O48 K6 K7 96.1(6) 2_647 1_655 ?
O48 K6 K8 44.2(6) 2_647 1_656 ?
O48 K6 O57 89.4(8) 2_647 . ?
O48 K6 O58 103.6(9) 2_647 . ?
O48 K6 Dy2 111.9(7) 2_647 . ?
K7 K6 K8 58.0(2) 1_655 1_656 ?
K7 K6 Dy2 149.4(3) 1_655 . ?
O57 K6 K7 41.1(6) . 1_655 ?
O57 K6 K8 75.5(6) . 1_656 ?
O57 K6 O58 83.5(7) . . ?
O57 K6 Dy2 145.4(7) . . ?
O58 K6 K7 42.5(5) . 1_655 ?
O58 K6 K8 60.6(6) . 1_656 ?
O58 K6 Dy2 115.3(7) . . ?
Dy2 K6 K8 138.6(4) . 1_656 ?
O43 K7 O47 80.9(7) 2_647 . ?
O43 K7 K5 99.1(7) 2_647 1_556 ?
O43 K7 K6 137.7(6) 2_647 1_455 ?
O43 K7 K8 117.3(6) 2_647 1_556 ?
O43 K7 O57 97.6(8) 2_647 1_455 ?
O43 K7 O58 170.3(9) 2_647 1_455 ?
O43 K7 O60 77.4(7) 2_647 . ?
O43 K7 K0A 43.1(5) 2_647 2_648 ?
O47 K7 K6 102.1(5) . 1_455 ?
O47 K7 K8 156.4(6) . 1_556 ?
O47 K7 O58 89.6(7) . 1_455 ?
O47 K7 O60 156.4(7) . . ?
O47 K7 K0A 111.4(5) . 2_648 ?
K5 K7 O47 86.6(6) 1_556 . ?
K5 K7 K6 123.2(3) 1_556 1_455 ?
K5 K7 K8 76.1(3) 1_556 1_556 ?
K5 K7 O57 161.1(7) 1_556 1_455 ?
K5 K7 O58 82.1(6) 1_556 1_455 ?
K5 K7 O60 87.7(5) 1_556 . ?
K5 K7 K0A 71.6(3) 1_556 2_648 ?
K6 K7 K8 75.1(2) 1_455 1_556 ?
K6 K7 K0A 144.4(2) 1_455 2_648 ?
O57 K7 O47 104.7(7) 1_455 . ?
O57 K7 K6 40.4(5) 1_455 1_455 ?
O57 K7 K8 88.4(5) 1_455 1_556 ?
O57 K7 O58 82.9(7) 1_455 1_455 ?
O57 K7 O60 87.4(7) 1_455 . ?
O57 K7 K0A 116.3(6) 1_455 2_648 ?
O58 K7 K6 42.7(5) 1_455 1_455 ?
O58 K7 K8 72.4(5) 1_455 1_556 ?
O58 K7 O60 112.3(7) 1_455 . ?
O58 K7 K0A 144.7(6) 1_455 2_648 ?
O60 K7 K6 100.2(4) . 1_455 ?
O60 K7 K8 40.4(4) . 1_556 ?
O60 K7 K0A 45.2(4) . 2_648 ?
K0A K7 K8 78.6(3) 2_648 1_556 ?
W6 O50 K9 132.4(12) . 2_557 ?
W9 O51 W3 151.1(11) . . ?
W8 O52 W7 118.5(9) . . ?
W7 O53 K1 98.4(7) . . ?
W10 O53 W7 122.8(9) . . ?
W10 O53 K1 110.6(8) . . ?
W3 O54 W4 119.6(12) . . ?
W7 O56 K9 164.2(12) . 2_657 ?
O32 K8 K5 129.7(4) 2_546 . ?
O32 K8 K6 80.0(5) 2_546 1_454 ?
O32 K8 K7 99.4(4) 2_546 1_554 ?
O32 K8 K9 164.1(4) 2_546 . ?
O32 K8 O59 131.1(5) 2_546 . ?
O32 K8 O0AA 112.9(7) 2_546 . ?
O40 K8 O32 155.2(5) . 2_546 ?
O40 K8 K5 39.0(4) . . ?
O40 K8 K6 106.2(5) . 1_454 ?
O40 K8 K7 70.8(5) . 1_554 ?
O40 K8 K9 40.4(4) . . ?
O40 K8 O59 69.4(5) . . ?
O40 K8 O60 78.3(6) . 1_554 ?
O40 K8 O62 110.9(7) . . ?
O40 K8 O0AA 90.0(7) . . ?
K5 K8 K6 70.9(2) . 1_454 ?
K7 K8 K5 32.03(19) 1_554 . ?
K7 K8 K6 46.92(18) 1_554 1_454 ?
K9 K8 K5 63.4(2) . . ?
K9 K8 K6 99.0(3) . 1_454 ?
K9 K8 K7 91.0(3) . 1_554 ?
O59 K8 K5 64.1(3) . . ?
O59 K8 K6 59.7(4) . 1_454 ?
O59 K8 K7 73.7(4) . 1_554 ?
O59 K8 K9 41.1(4) . . ?
O59 K8 O0AA 22.2(6) . . ?
O60 K8 O32 80.9(4) 1_554 2_546 ?
O60 K8 K5 51.9(3) 1_554 . ?
O60 K8 K6 72.6(4) 1_554 1_454 ?
O60 K8 K7 35.9(4) 1_554 1_554 ?
O60 K8 K9 114.1(4) 1_554 . ?
O60 K8 O59 109.1(5) 1_554 . ?
O60 K8 O0AA 123.6(7) 1_554 . ?
O62 K8 O32 92.9(5) . 2_546 ?
O62 K8 K5 104.6(5) . . ?
O62 K8 K6 58.2(5) . 1_454 ?
O62 K8 K7 99.3(5) . 1_554 ?
O62 K8 K9 73.5(5) . . ?
O62 K8 O59 43.6(5) . . ?
O62 K8 O60 130.8(6) . 1_554 ?
O62 K8 O0AA 21.5(7) . . ?
O0AA K8 K5 85.3(6) . . ?
O0AA K8 K6 58.2(6) . 1_454 ?
O0AA K8 K7 88.1(6) . 1_554 ?
O0AA K8 K9 55.1(6) . . ?
W6 K9 W7 98.7(3) 2_547 2_647 ?
W6 K9 W11 112.2(3) 2_547 . ?
W6 K9 K5 162.5(3) 2_547 . ?
W7 K9 W11 90.3(2) 2_647 . ?
W7 K9 K5 97.5(2) 2_647 . ?
W11 K9 K5 60.91(17) . . ?
O20 K9 W6 110.5(6) . 2_547 ?
O20 K9 W7 87.1(6) . 2_647 ?
O20 K9 W11 3.8(6) . . ?
O20 K9 O41 166.5(8) . . ?
O20 K9 K5 63.5(6) . . ?
O20 K9 O50 91.1(8) . 2_547 ?
O20 K9 K8 122.8(7) . . ?
O20 K9 O59 75.5(7) . . ?
O20 K9 O0AA 92.0(8) . . ?
O40 K9 W6 148.0(6) . 2_547 ?
O40 K9 W7 87.8(6) . 2_647 ?
O40 K9 W11 99.1(6) . . ?
O40 K9 O20 101.1(8) . . ?
O40 K9 O41 78.4(6) . . ?
O40 K9 K5 39.5(5) . . ?
O40 K9 O50 167.8(9) . 2_547 ?
O40 K9 K8 48.7(5) . . ?
O40 K9 O59 91.8(7) . . ?
O40 K9 O0AA 100.7(9) . . ?
O41 K9 W6 72.1(3) . 2_547 ?
O41 K9 W7 79.3(3) . 2_647 ?
O41 K9 W11 169.4(5) . . ?
O41 K9 K5 117.8(4) . . ?
O41 K9 K8 67.0(4) . . ?
O41 K9 O0AA 101.4(7) . . ?
O50 K9 W6 20.2(5) 2_547 2_547 ?
O50 K9 W7 92.6(6) 2_547 2_647 ?
O50 K9 W11 93.1(6) 2_547 . ?
O50 K9 O41 89.7(7) 2_547 . ?
O50 K9 K5 152.0(7) 2_547 . ?
O50 K9 K8 124.0(7) 2_547 . ?
O50 K9 O0AA 78.9(8) 2_547 . ?
O56 K9 W6 96.8(6) 2_647 2_547 ?
O56 K9 W7 6.8(5) 2_647 2_647 ?
O56 K9 W11 85.0(6) 2_647 . ?
O56 K9 O20 81.6(8) 2_647 . ?
O56 K9 O40 92.8(8) 2_647 . ?
O56 K9 O41 84.9(6) 2_647 . ?
O56 K9 K5 98.5(6) 2_647 . ?
O56 K9 O50 88.7(8) 2_647 2_547 ?
O56 K9 K8 134.8(7) 2_647 . ?
O56 K9 O59 157.1(8) 2_647 . ?
O56 K9 O0AA 166.0(9) 2_647 . ?
K8 K9 W6 106.5(3) . 2_547 ?
K8 K9 W7 128.2(3) . 2_647 ?
K8 K9 W11 119.0(3) . . ?
K8 K9 K5 68.0(3) . . ?
O59 K9 W6 91.1(5) . 2_547 ?
O59 K9 W7 162.2(6) . 2_647 ?
O59 K9 W11 72.1(5) . . ?
O59 K9 O41 118.0(6) . . ?
O59 K9 K5 71.6(5) . . ?
O59 K9 O50 91.5(7) . 2_547 ?
O59 K9 K8 61.7(5) . . ?
O59 K9 O0AA 20.5(7) . . ?
O0AA K9 W6 73.7(6) . 2_547 ?
O0AA K9 W7 171.5(7) . 2_647 ?
O0AA K9 W11 89.1(6) . . ?
O0AA K9 K5 89.7(6) . . ?
O0AA K9 K8 58.9(6) . . ?
K6 O57 K7 98.5(8) . 1_655 ?
K6 O58 K5 139.9(8) . 1_656 ?
K7 O58 K5 47.4(4) 1_655 1_656 ?
K7 O58 K6 94.8(8) 1_655 . ?
K9 O59 K8 77.2(5) . . ?
O0AA O59 K8 84.5(15) . . ?
O0AA O59 K9 117.9(18) . . ?
K7 O60 K8 103.7(6) . 1_556 ?
K7 O60 K0A 93.3(6) . 2_648 ?
K0A O60 K8 134.4(6) 2_648 1_556 ?
O0AA O62 K8 103.0(17) . . ?
C8 O63 K5 103.0(17) . 2_657 ?
C8 O63 K0A 123(2) . . ?
K0A O63 K5 87.8(5) . 2_657 ?
O28 C8 K5 108(2) . 2_657 ?
O28 C8 O63 126(3) . . ?
O28 C8 C10 119(3) . . ?
O63 C8 K5 55.3(15) . 2_657 ?
O63 C8 C10 115(3) . . ?
C10 C8 K5 102.9(19) . 2_657 ?
C13 C9 C10 120(2) . . ?
C9 C10 C8 115(2) . . ?
C11 C10 C8 123(2) . . ?
C11 C10 C9 122(2) . . ?
C10 C11 O0AA 122(3) . 2_557 ?
C12 C11 C10 121(2) . . ?
C12 C11 O0AA 117(2) . 2_557 ?
C13 N2 C12 122.1(17) . . ?
C11 C12 N2 116.7(18) . . ?
C9 C13 N2 117.9(19) . . ?
O14 K0A O44 91.7(4) 1_556 . ?
O14 K0A K5 130.6(4) 1_556 2_657 ?
O14 K0A K7 105.5(4) 1_556 2_658 ?
O14 K0A Dy2 95.3(4) 1_556 . ?
O43 K0A O14 69.9(6) 1_556 1_556 ?
O43 K0A O44 158.3(6) 1_556 . ?
O43 K0A O45 112.2(7) 1_556 1_556 ?
O43 K0A K5 63.7(5) 1_556 2_657 ?
O43 K0A K7 36.6(5) 1_556 2_658 ?
O43 K0A O60 68.9(6) 1_556 2_658 ?
O43 K0A O63 91.2(6) 1_556 . ?
O43 K0A Dy2 150.0(5) 1_556 . ?
O44 K0A K5 128.4(3) . 2_657 ?
O44 K0A K7 162.6(4) . 2_658 ?
O44 K0A Dy2 38.6(4) . . ?
O45 K0A O14 68.2(5) 1_556 1_556 ?
O45 K0A O44 68.7(5) 1_556 . ?
O45 K0A K5 145.9(4) 1_556 2_657 ?
O45 K0A K7 120.2(4) 1_556 2_658 ?
O45 K0A O60 86.7(5) 1_556 2_658 ?
O45 K0A O63 156.5(6) 1_556 . ?
O45 K0A Dy2 38.4(4) 1_556 . ?
O49 K0A O14 140.4(6) 1_556 1_556 ?
O49 K0A O43 128.7(7) 1_556 1_556 ?
O49 K0A O44 72.9(5) 1_556 . ?
O49 K0A O45 72.2(6) 1_556 1_556 ?
O49 K0A K5 84.7(5) 1_556 2_657 ?
O49 K0A K7 94.9(5) 1_556 2_658 ?
O49 K0A O60 60.2(5) 1_556 2_658 ?
O49 K0A O63 95.3(6) 1_556 . ?
O49 K0A Dy2 50.2(5) 1_556 . ?
K5 K0A K7 35.8(2) 2_657 2_658 ?
K5 K0A Dy2 133.7(2) 2_657 . ?
K7 K0A Dy2 139.2(3) 2_658 . ?
O60 K0A O14 117.4(6) 2_658 1_556 ?
O60 K0A O44 131.9(5) 2_658 . ?
O60 K0A K5 59.8(4) 2_658 2_657 ?
O60 K0A K7 41.5(4) 2_658 2_658 ?
O60 K0A Dy2 97.8(4) 2_658 . ?
O63 K0A O14 121.2(6) . 1_556 ?
O63 K0A O44 88.8(5) . . ?
O63 K0A K5 47.0(3) . 2_657 ?
O63 K0A K7 79.8(4) . 2_658 ?
O63 K0A O60 104.6(5) . 2_658 ?
O63 K0A Dy2 118.5(4) . . ?
O21 Dy2 O37 135.5(6) 1_556 . ?
O21 Dy2 O42 73.1(6) 1_556 . ?
O21 Dy2 O44 97.5(5) 1_556 . ?
O21 Dy2 O45 69.0(5) 1_556 1_556 ?
O21 Dy2 K6 106.1(5) 1_556 . ?
O21 Dy2 K0A 98.8(4) 1_556 . ?
O37 Dy2 O42 91.2(6) . . ?
O37 Dy2 O45 155.1(6) . 1_556 ?
O37 Dy2 K6 73.1(5) . . ?
O37 Dy2 K0A 119.7(5) . . ?
O42 Dy2 K6 34.0(5) . . ?
O42 Dy2 K0A 135.9(5) . . ?
O44 Dy2 O37 95.2(5) . . ?
O44 Dy2 O42 170.6(5) . . ?
O44 Dy2 O45 73.9(5) . 1_556 ?
O44 Dy2 K6 155.3(3) . . ?
O44 Dy2 K0A 45.0(4) . . ?
O45 Dy2 O42 102.8(7) 1_556 . ?
O45 Dy2 K6 107.6(4) 1_556 . ?
O45 Dy2 K0A 38.0(4) 1_556 . ?
K6 Dy2 K0A 122.0(2) . . ?
K9 O0AA K8 65.9(6) . . ?
O59 O0AA K8 73.3(14) . . ?
O59 O0AA K9 41.5(14) . . ?
O59 O0AA C11 113(3) . 2_547 ?
O62 O0AA K8 55.5(14) . . ?
O62 O0AA K9 112.9(19) . . ?
O62 O0AA O59 128(3) . . ?
O62 O0AA C11 119(3) . 2_547 ?
C11 O0AA K8 167(2) 2_547 . ?
C11 O0AA K9 111(2) 2_547 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Dy1 O28 C8 K5 -139(2) . . . 2_657 ?
Dy1 O28 C8 O63 161(2) . . . . ?
Dy1 O28 C8 C10 -23(5) . . . . ?
Dy1 O33 C3 O37 -162(2) . . . . ?
Dy1 O33 C3 C5 25(6) . . . . ?
O1 W2 O7 W11 -45(2) . . . . ?
O1 W2 O8 K4 -78(5) . . . 2_547 ?
O1 W2 O34 Dy1 -3.9(13) . . . . ?
O1 W6 O35 Dy1 -3.9(12) . . . . ?
O1 W6 O50 K9 83(4) . . . 2_557 ?
O1 Si1 O10 W3 -179.0(16) . . . . ?
O1 Si1 O10 W4 -61.4(17) . . . . ?
O1 Si1 O10 W5 54.9(18) . . . . ?
O1 Si1 O17 W7 62.3(13) . . . . ?
O1 Si1 O17 W8 -57.9(14) . . . . ?
O1 Si1 O17 W10 -176.7(9) . . . . ?
O1 Si1 O23 W1 -59.3(17) . . . . ?
O1 Si1 O23 W9 177.5(11) . . . . ?
O1 Si1 O23 W11 58.3(18) . . . . ?
O2 W2 O7 W11 -15(4) . . . . ?
O2 W2 O8 K4 -41.2(14) . . . 2_547 ?
O2 W2 O34 Dy1 -76.3(13) . . . . ?
O2 W6 O35 Dy1 70.2(12) . . . . ?
O2 W6 O50 K9 46.5(15) . . . 2_557 ?
O3 W6 O35 Dy1 -88.2(13) . . . . ?
O3 W6 O50 K9 -150.9(14) . . . 2_557 ?
O3 W8 O22 K4 -144(4) . . . . ?
O4 W9 O18 W1 86.9(11) . . . . ?
O4 W9 O18 K1 -20.6(7) . . . . ?
O4 W9 O21 Dy2 -49.0(19) . . . 1_554 ?
O4 W9 O51 W3 -29(2) . . . . ?
O4 W10 O14 K0A 46.5(14) . . . 1_554 ?
O4 W10 O27 W8 26(3) . . . . ?
O4 W10 O53 W7 -92.3(10) . . . . ?
O4 W10 O53 K1 23.0(7) . . . . ?
O5 W5 O15 W8 24(2) . . . . ?
O5 W6 O35 Dy1 -17(4) . . . . ?
O5 W6 O50 K9 129.4(15) . . . 2_557 ?
O6 W2 O7 W11 36(2) . . . . ?
O6 W2 O8 K4 -124.8(14) . . . 2_547 ?
O6 W2 O34 Dy1 -4(5) . . . . ?
O7 W2 O8 K4 152.8(14) . . . 2_547 ?
O7 W2 O34 Dy1 83.6(14) . . . . ?
O7 W11 O16 W4 30(2) . . . . ?
O7 W11 O24 W1 -77.9(14) . . . . ?
O7 W11 O26 W9 17(3) . . . . ?
O7 W11 O26 K5 -155.6(19) . . . . ?
O8 W2 O7 W11 127(2) . . . . ?
O8 W2 O34 Dy1 -175.9(13) . . . . ?
O9 W1 O19 K4 74(3) . . . 2_647 ?
O9 W1 O31 Dy1 -6(3) . . . . ?
O9 W7 O29 Dy1 13(2) . . . . ?
O9 W7 O56 K9 -53(4) . . . 2_657 ?
O10 W3 O11 W10 63(2) . . . . ?
O10 W4 O6 W2 -57(2) . . . . ?
O10 W4 O6 K1 99.9(7) . . . 1_455 ?
O10 W5 O5 W6 51(2) . . . . ?
O10 W5 O5 K1 -99.6(7) . . . 1_455 ?
O10 W5 O15 W8 -63.4(19) . . . . ?
O10 Si1 O1 W2 73.4(16) . . . . ?
O10 Si1 O1 W6 -67.4(17) . . . . ?
O10 Si1 O17 W7 178.8(9) . . . . ?
O10 Si1 O17 W8 58.6(14) . . . . ?
O10 Si1 O17 W10 -60.3(13) . . . . ?
O10 Si1 O23 W1 179.9(11) . . . . ?
O10 Si1 O23 W9 56.6(17) . . . . ?
O10 Si1 O23 W11 -62.6(17) . . . . ?
O11 W3 O32 K8 -101.7(13) . . . 2_556 ?
O11 W10 O14 K0A -39.7(15) . . . 1_554 ?
O11 W10 O27 W8 85.5(11) . . . . ?
O11 W10 O53 W7 -19(3) . . . . ?
O11 W10 O53 K1 96.3(18) . . . . ?
O12 W5 O5 W6 -137(2) . . . . ?
O12 W5 O5 K1 72.8(9) . . . 1_455 ?
O12 W5 O15 W8 129(2) . . . . ?
O13 W4 O6 W2 -129(2) . . . . ?
O13 W4 O6 K1 27.5(8) . . . 1_455 ?
O13 W5 O5 W6 126(2) . . . . ?
O13 W5 O5 K1 -24.9(8) . . . 1_455 ?
O13 W5 O15 W8 -69(3) . . . . ?
O14 W10 O27 W8 -170.0(10) . . . . ?
O14 W10 O53 W7 167.1(11) . . . . ?
O14 W10 O53 K1 -77.6(9) . . . . ?
O15 W5 O5 W6 -33(2) . . . . ?
O15 W5 O5 K1 176.8(8) . . . 1_455 ?
O15 W8 O3 W6 34(3) . . . . ?
O15 W8 O22 K4 -56(4) . . . . ?
O16 W4 O6 W2 30(2) . . . . ?
O16 W4 O6 K1 -173.4(8) . . . 1_455 ?
O16 W11 O24 W1 2(4) . . . . ?
O16 W11 O26 W9 91.7(11) . . . . ?
O16 W11 O26 K5 -80.9(11) . . . . ?
O17 W7 O9 W1 -72.1(8) . . . . ?
O17 W7 O9 K1 106.5(5) . . . . ?
O17 W7 O29 Dy1 97(2) . . . . ?
O17 W7 O56 K9 -161(3) . . . 2_657 ?
O17 W8 O3 W6 -52(3) . . . . ?
O17 W10 O14 K0A -169(3) . . . 1_554 ?
O17 W10 O27 W8 2.8(9) . . . . ?
O17 W10 O53 W7 -3.9(10) . . . . ?
O17 W10 O53 K1 111.5(8) . . . . ?
O17 Si1 O1 W2 -170.4(9) . . . . ?
O17 Si1 O1 W6 48.8(10) . . . . ?
O17 Si1 O10 W3 62.7(19) . . . . ?
O17 Si1 O10 W4 -179.6(9) . . . . ?
O17 Si1 O10 W5 -63.3(10) . . . . ?
O17 Si1 O23 W1 63.0(12) . . . . ?
O17 Si1 O23 W9 -60.3(13) . . . . ?
O17 Si1 O23 W11 -179.5(17) . . . . ?
O18 W1 O19 K4 158(3) . . . 2_647 ?
O18 W1 O31 Dy1 -84(5) . . . . ?
O18 W9 O4 W10 -117.0(10) . . . . ?
O18 W9 O4 K1 19.2(6) . . . . ?
O18 W9 O21 Dy2 -144.3(17) . . . 1_554 ?
O18 W9 O51 W3 57(4) . . . . ?
O19 W1 O31 Dy1 93(3) . . . . ?
O20 W11 O16 W4 132(2) . . . . ?
O20 W11 O24 W1 179.5(14) . . . . ?
O20 W11 O26 W9 -168.3(11) . . . . ?
O20 W11 O26 K5 19.1(12) . . . . ?
O21 W9 O4 W10 136.8(11) . . . . ?
O21 W9 O4 K1 -87.0(7) . . . . ?
O21 W9 O18 W1 -172.2(11) . . . . ?
O21 W9 O18 K1 80.4(10) . . . . ?
O21 W9 O51 W3 -128(2) . . . . ?
O22 W8 O3 W6 135(3) . . . . ?
O23 W1 O19 K4 167(2) . . . 2_647 ?
O23 W1 O31 Dy1 -89(3) . . . . ?
O23 W9 O4 W10 -42.5(10) . . . . ?
O23 W9 O4 K1 93.8(6) . . . . ?
O23 W9 O18 W1 -0.2(11) . . . . ?
O23 W9 O18 K1 -107.6(9) . . . . ?
O23 W9 O51 W3 60(2) . . . . ?
O23 W11 O16 W4 -53(2) . . . . ?
O23 W11 O24 W1 5.4(13) . . . . ?
O23 W11 O26 W9 5.2(10) . . . . ?
O23 W11 O26 K5 -167.4(11) . . . . ?
O23 Si1 O1 W2 -49.4(12) . . . . ?
O23 Si1 O1 W6 169.8(11) . . . . ?
O23 Si1 O10 W3 -55(2) . . . . ?
O23 Si1 O10 W4 62.9(11) . . . . ?
O23 Si1 O10 W5 179.2(11) . . . . ?
O23 Si1 O17 W7 -61.8(10) . . . . ?
O23 Si1 O17 W8 178.0(17) . . . . ?
O23 Si1 O17 W10 59.1(10) . . . . ?
O24 W1 O19 K4 -121(3) . . . 2_647 ?
O24 W1 O31 Dy1 -162(3) . . . . ?
O24 W11 O16 W4 -50(4) . . . . ?
O24 W11 O26 W9 -68.3(11) . . . . ?
O24 W11 O26 K5 119.2(11) . . . . ?
O26 W9 O4 W10 -24(2) . . . . ?
O26 W9 O4 K1 112.6(16) . . . . ?
O26 W9 O18 W1 -72.3(12) . . . . ?
O26 W9 O18 K1 -179.7(8) . . . . ?
O26 W9 O21 Dy2 124.1(18) . . . 1_554 ?
O26 W9 O51 W3 133(2) . . . . ?
O26 W11 O16 W4 -131(2) . . . . ?
O26 W11 O24 W1 82.7(14) . . . . ?
O27 W8 O3 W6 -40(5) . . . . ?
O27 W8 O22 K4 34(4) . . . . ?
O27 W10 O14 K0A -128.5(14) . . . 1_554 ?
O27 W10 O53 W7 69.0(12) . . . . ?
O27 W10 O53 K1 -175.7(8) . . . . ?
O28 C8 C10 C9 -78(4) . . . . ?
O28 C8 C10 C11 103(4) . . . . ?
O29 W7 O9 W1 17.9(9) . . . . ?
O29 W7 O9 K1 -163.6(6) . . . . ?
O29 W7 O56 K9 44(4) . . . 2_657 ?
O30 W3 O11 W10 135(3) . . . . ?
O30 W3 O32 K8 -11.7(15) . . . 2_556 ?
O30 W5 O5 W6 44(4) . . . . ?
O30 W5 O5 K1 -107(2) . . . 1_455 ?
O30 W5 O15 W8 -136(2) . . . . ?
O31 W1 O19 K4 -21(3) . . . 2_647 ?
O32 W3 O11 W10 -126(2) . . . . ?
O33 C3 C5 C2 80(4) . . . . ?
O33 C3 C5 C4 -106(4) . . . . ?
O34 W2 O7 W11 -132(2) . . . . ?
O34 W2 O8 K4 53.5(15) . . . 2_547 ?
O35 W6 O50 K9 -51.5(16) . . . 2_557 ?
O37 C3 C5 C2 -93(4) . . . . ?
O37 C3 C5 C4 81(4) . . . . ?
O38 C6 O39 K4 93(4) . . . 2_547 ?
N1 C1 C7 C4 2(5) . . . . ?
N1 C2 C5 C3 174(3) . . . . ?
N1 C2 C5 C4 0(5) . . . . ?
C4 C6 O39 K4 -87(3) . . . 2_547 ?
C5 C2 N1 C1 0(4) . . . . ?
C5 C4 C6 O38 1(5) . . . . ?
C5 C4 C6 O39 -179(3) . . . . ?
C5 C4 C6 K4 135(3) . . . 2_547 ?
C5 C4 C7 C1 -2(6) . . . . ?
C6 C4 C5 C2 -174(3) . . . . ?
C6 C4 C5 C3 11(6) . . . . ?
C6 C4 C7 C1 174(3) . . . . ?
C7 C1 N1 C2 -1(4) . . . . ?
C7 C4 C5 C2 1(5) . . . . ?
C7 C4 C5 C3 -173(3) . . . . ?
C7 C4 C6 O38 -175(3) . . . . ?
C7 C4 C6 O39 5(5) . . . . ?
C7 C4 C6 K4 -40(4) . . . 2_547 ?
K1 W1 O19 K4 109(3) . . . 2_647 ?
K1 W1 O31 Dy1 11(4) . . . . ?
K1 W2 O7 W11 42(3) 1_455 . . . ?
K1 W2 O8 K4 -81.9(13) 1_455 . . 2_547 ?
K1 W2 O34 Dy1 -88.7(14) 1_455 . . . ?
K1 W4 O6 W2 -157(3) 1_455 . . . ?
K1 W5 O5 W6 151(3) 1_455 . . . ?
K1 W5 O15 W8 27(3) 1_455 . . . ?
K1 W6 O35 Dy1 77.2(14) 1_455 . . . ?
K1 W6 O50 K9 86.5(14) 1_455 . . 2_557 ?
K1 W7 O9 W1 -178.6(9) . . . . ?
K1 W7 O29 Dy1 -2(3) . . . . ?
K1 W7 O56 K9 -89(4) . . . 2_657 ?
K1 W9 O4 W10 -136.3(10) . . . . ?
K1 W9 O18 W1 107.4(14) . . . . ?
K1 W9 O21 Dy2 -99.1(18) . . . 1_554 ?
K1 W9 O51 W3 -24(3) . . . . ?
K1 W10 O14 K0A 95.5(13) . . . 1_554 ?
K1 W10 O27 W8 -72.5(11) . . . . ?
K1 W10 O53 W7 -115.3(14) . . . . ?
K4 W1 O31 Dy1 89(3) 2_647 . . . ?
K4 W2 O7 W11 142(2) 2_547 . . . ?
K4 W2 O34 Dy1 -153.3(14) 2_547 . . . ?
K4 W8 O3 W6 130(3) . . . . ?
K5 W9 O4 W10 101.5(10) . . . . ?
K5 W9 O4 K1 -122.2(6) . . . . ?
K5 W9 O18 W1 -108.5(10) . . . . ?
K5 W9 O18 K1 144.1(5) . . . . ?
K5 W9 O21 Dy2 115.5(19) . . . 1_554 ?
K5 W9 O51 W3 172(2) . . . . ?
K5 O63 C8 O28 88(3) 2_657 . . . ?
K5 O63 C8 C10 -88(2) 2_657 . . . ?
K5 C8 C10 C9 42(3) 2_657 . . . ?
K5 C8 C10 C11 -138(2) 2_657 . . . ?
O50 W6 O35 Dy1 166.8(12) . . . . ?
O51 W3 O11 W10 -23(2) . . . . ?
O51 W3 O32 K8 170.0(12) . . . 2_556 ?
O51 W9 O4 W10 39.8(10) . . . . ?
O51 W9 O4 K1 176.0(6) . . . . ?
O51 W9 O18 W1 2(3) . . . . ?
O51 W9 O18 K1 -105(2) . . . . ?
O51 W9 O21 Dy2 37.9(19) . . . 1_554 ?
O52 W7 O9 W1 -92.0(17) . . . . ?
O52 W7 O9 K1 86.5(16) . . . . ?
O52 W7 O29 Dy1 171(2) . . . . ?
O52 W7 O56 K9 140(4) . . . 2_657 ?
O52 W8 O3 W6 -127(3) . . . . ?
O52 W8 O22 K4 123(4) . . . . ?
O53 W7 O9 W1 -143.7(9) . . . . ?
O53 W7 O9 K1 34.9(6) . . . . ?
O53 W7 O29 Dy1 89(3) . . . . ?
O53 W7 O56 K9 -135(4) . . . 2_657 ?
O53 W10 O14 K0A 137.5(14) . . . 1_554 ?
O53 W10 O27 W8 -68.3(11) . . . . ?
O54 W3 O11 W10 54(4) . . . . ?
O54 W3 O32 K8 78.3(15) . . . 2_556 ?
O54 W4 O6 W2 -50(4) . . . . ?
O54 W4 O6 K1 107(2) . . . 1_455 ?
O55 W4 O6 W2 130(2) . . . . ?
O55 W4 O6 K1 -73.0(9) . . . 1_455 ?
O56 W7 O9 W1 121.6(9) . . . . ?
O56 W7 O9 K1 -59.8(7) . . . . ?
O56 W7 O29 Dy1 -89(2) . . . . ?
K8 O59 O0AA K9 72.3(11) . . . . ?
K8 O59 O0AA O62 -10(3) . . . . ?
K8 O59 O0AA C11 168(3) . . . 2_547 ?
K8 O62 O0AA K9 -34.1(19) . . . . ?
K8 O62 O0AA O59 11(4) . . . . ?
K8 O62 O0AA C11 -167(2) . . . 2_547 ?
K9 W6 O35 Dy1 145.6(12) 2_557 . . . ?
K9 W7 O9 W1 114.4(7) 2_657 . . . ?
K9 W7 O9 K1 -67.1(3) 2_657 . . . ?
K9 W7 O29 Dy1 -83(2) 2_657 . . . ?
K9 W11 O16 W4 135(2) . . . . ?
K9 W11 O24 W1 176.5(11) . . . . ?
K9 W11 O26 W9 -172.7(9) . . . . ?
K9 W11 O26 K5 14.7(9) . . . . ?
K9 O59 O0AA K8 -72.3(11) . . . . ?
K9 O59 O0AA O62 -82(4) . . . . ?
K9 O59 O0AA C11 96(3) . . . 2_547 ?
O63 C8 C10 C9 99(3) . . . . ?
O63 C8 C10 C11 -81(4) . . . . ?
C8 C10 C11 C12 177(3) . . . . ?
C8 C10 C11 O0AA -6(5) . . . 2_557 ?
C9 C10 C11 C12 -3(4) . . . . ?
C9 C10 C11 O0AA 175(3) . . . 2_557 ?
C10 C9 C13 N2 1(4) . . . . ?
C10 C11 C12 N2 1(4) . . . . ?
C12 N2 C13 C9 -3(3) . . . . ?
C13 C9 C10 C8 -178(3) . . . . ?
C13 C9 C10 C11 2(4) . . . . ?
C13 N2 C12 C11 2(3) . . . . ?
K0A O63 C8 O28 -8(4) . . . . ?
K0A O63 C8 K5 -95.8(15) . . . 2_657 ?
K0A O63 C8 C10 175.8(16) . . . . ?
Dy2 O37 C3 O33 26(5) . . . . ?
Dy2 O37 C3 C5 -161(2) . . . . ?
O0AA C11 C12 N2 -177(2) 2_557 . . . ?


_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.49(2)
2 0.51(2)

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_mar18053_0m
_database_code_depnum_ccdc_archive 'CCDC 1857779'
_audit_update_record             
;
2018-07-24 deposited with the CCDC.
2018-08-23 downloaded from the CCDC.
;
_audit_creation_date             2018-06-17
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'C14 K4 N2 O59.75 Pr2 Si W11, 4(O)'
_chemical_formula_sum            'C14 K4 N2 O63.75 Pr2 Si W11'
_chemical_formula_weight         3704.82
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pr Pr -0.2180 2.8214 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   11.4529(13)
_cell_length_b                   30.495(3)
_cell_length_c                   17.907(2)
_cell_angle_alpha                90
_cell_angle_beta                 101.994(4)
_cell_angle_gamma                90
_cell_volume                     6117.5(12)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    9885
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      ?
_cell_measurement_theta_min      ?
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    22.570
_exptl_absorpt_correction_T_max  0.7454
_exptl_absorpt_correction_T_min  0.2977
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1568 before and 0.1134 after correction.
The Ratio of minimum to maximum transmission is 0.3994.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    4.023
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plates
_exptl_crystal_F_000             6520
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.02
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.1495
_diffrn_reflns_av_unetI/netI     0.0707
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       37
_diffrn_reflns_limit_k_min       -37
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            102527
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.682
_diffrn_reflns_theta_min         3.537
_diffrn_ambient_temperature      150.04
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                9174
_reflns_number_total             11556
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_refine_diff_density_max         4.265
_refine_diff_density_min         -4.214
_refine_diff_density_rms         0.704
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.148
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     458
_refine_ls_number_reflns         11556
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1066
_refine_ls_R_factor_gt           0.0846
_refine_ls_restrained_S_all      1.148
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0563P)²+1534.4174P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2064
_refine_ls_wR_factor_ref         0.2213
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
: with sigma of 0.2 and sigma for terminal atoms of 0.4
2. Others
 Fixed Sof: O18(0.75)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.40200(11) 0.47913(4) 0.30410(6) 0.0126(3) Uani 1 1 d . . . . .
W2 W 0.68185(11) 0.44704(4) 0.35966(7) 0.0138(3) Uani 1 1 d . . . . .
W3 W 0.29367(11) 0.36597(4) 0.34257(7) 0.0140(3) Uani 1 1 d . . . . .
W4 W 0.19490(11) 0.41641(4) 0.15380(7) 0.0147(3) Uani 1 1 d . . . . .
W5 W 0.39611(11) 0.43387(4) 0.04232(7) 0.0150(3) Uani 1 1 d . . . . .
W6 W 0.57675(11) 0.33347(4) 0.40008(7) 0.0156(3) Uani 1 1 d . . . . .
W7 W 0.29479(12) 0.32988(4) 0.06806(7) 0.0181(3) Uani 1 1 d . . . . .
W8 W 0.39419(12) 0.27872(4) 0.25907(7) 0.0175(3) Uani 1 1 d . . . . .
W9 W 0.70370(12) 0.39893(4) 0.10363(7) 0.0178(3) Uani 1 1 d . . . . .
W10 W 0.78836(12) 0.34784(4) 0.27262(7) 0.0189(3) Uani 1 1 d . . . . .
W11 W 0.60886(13) 0.29436(4) 0.13084(8) 0.0201(3) Uani 1 1 d . . . . .
Pr1 Pr 0.61828(15) 0.51994(6) 0.17870(9) 0.0146(3) Uani 1 1 d . . . . .
Pr2 Pr 0.10999(18) 0.64406(7) 0.27719(11) 0.0245(4) Uani 1 1 d . . . . .
K1 K 0.7051(14) 0.2312(5) 0.3407(9) 0.076(4) Uiso 1 1 d . . . . .
K2 K 0.0480(11) 0.3069(4) 0.1904(7) 0.055(3) Uiso 1 1 d . . . . .
K3 K -0.256(2) 0.6440(7) 0.1488(13) 0.117(6) Uiso 1 1 d . . . . .
K4 K 1.138(2) 0.2740(7) 0.4272(13) 0.123(7) Uiso 1 1 d . . . . .
Si2 Si 0.4932(6) 0.3853(2) 0.2212(4) 0.0026(13) Uiso 1 1 d . . . . .
O1 O 0.322(2) 0.6457(8) 0.3332(14) 0.027(5) Uiso 1 1 d . . . . .
O2 O 0.462(2) 0.5808(8) 0.1323(14) 0.024(5) Uiso 1 1 d . . . . .
O3 O 0.442(2) 0.6381(8) 0.2555(15) 0.030(6) Uiso 1 1 d . . . . .
O4 O 0.185(3) 0.5711(9) 0.2461(17) 0.038(7) Uiso 1 1 d . . . . .
O5 O 0.985(5) 0.3348(18) 0.498(3) 0.104(16) Uiso 1 1 d . . . . .
O6 O 0.709(2) 0.6478(8) 0.3235(15) 0.030(6) Uiso 1 1 d . . . . .
O7 O -0.004(4) 0.2604(16) 0.057(3) 0.089(14) Uiso 1 1 d . . . . .
O8 O 0.7096(19) 0.4905(7) 0.2996(12) 0.017(4) Uiso 1 1 d . . . . .
O9 O 0.1657(19) 0.3634(7) 0.0925(12) 0.014(4) Uiso 1 1 d . . . . .
O10 O 0.221(2) 0.6476(8) 0.1650(15) 0.028(6) Uiso 1 1 d . . . . .
O11 O 0.148(2) 0.6918(8) 0.3956(13) 0.023(5) Uiso 1 1 d . . . . .
O12 O -0.169(2) 0.5367(8) 0.1848(14) 0.027(5) Uiso 1 1 d . . . . .
O13 O -0.069(3) 0.5909(9) 0.2493(16) 0.038(7) Uiso 1 1 d . . . . .
O14 O -0.042(3) 0.5836(10) 0.4436(17) 0.040(7) Uiso 1 1 d . . . . .
O15 O 0.112(2) 0.5977(9) 0.3873(16) 0.034(6) Uiso 1 1 d . . . . .
O16 O 0.2022(18) 0.3804(7) 0.2421(12) 0.013(4) Uiso 1 1 d . . . . .
O17 O -0.078(3) 0.6789(9) 0.2990(17) 0.039(7) Uiso 1 1 d . . . . .
O18 O 0.074(7) 0.236(2) 0.283(4) 0.11(2) Uiso 0.75 1 d . . P . .
O19 O 0.3152(19) 0.5098(7) 0.3541(12) 0.017(5) Uiso 1 1 d . . . . .
O20 O -0.029(3) 0.6614(11) 0.152(2) 0.052(8) Uiso 1 1 d . . . . .
O21 O 0.6177(18) 0.3901(6) 0.4040(11) 0.012(4) Uiso 1 1 d . . . . .
O22 O 0.4502(17) 0.3508(6) 0.2829(11) 0.010(4) Uiso 1 1 d . . . . .
O23 O 0.3829(19) 0.3909(7) 0.1455(12) 0.016(4) Uiso 1 1 d . . . . .
O24 O 0.183(2) 0.3656(7) 0.3937(13) 0.020(5) Uiso 1 1 d . . . . .
O25 O 0.5275(18) 0.4323(7) 0.2640(11) 0.013(4) Uiso 1 1 d . . . . .
O26 O 0.3471(18) 0.4215(6) 0.3505(11) 0.012(4) Uiso 1 1 d . . . . .
O27 O 0.301(2) 0.3008(7) 0.1640(13) 0.018(5) Uiso 1 1 d . . . . .
O28 O 0.053(2) 0.4353(8) 0.1401(13) 0.022(5) Uiso 1 1 d . . . . .
O29 O 0.458(2) 0.4768(7) 0.1026(13) 0.018(5) Uiso 1 1 d . . . . .
O30 O 0.2759(18) 0.3044(7) 0.3077(12) 0.014(4) Uiso 1 1 d . . . . .
O31 O 0.5248(19) 0.2774(7) 0.2100(12) 0.017(5) Uiso 1 1 d . . . . .
O32 O 0.234(2) 0.4437(7) 0.0667(12) 0.018(5) Uiso 1 1 d . . . . .
O33 O 0.783(2) 0.4575(8) 0.4439(13) 0.023(5) Uiso 1 1 d . . . . .
O34 O 0.630(2) 0.2457(9) 0.0913(15) 0.032(6) Uiso 1 1 d . . . . .
O35 O 0.695(2) 0.4495(7) 0.1460(13) 0.021(5) Uiso 1 1 d . . . . .
O36 O 0.423(2) 0.3446(7) 0.4203(13) 0.020(5) Uiso 1 1 d . . . . .
O37 O 0.320(2) 0.3747(8) 0.0022(13) 0.022(5) Uiso 1 1 d . . . . .
O38 O 0.767(2) 0.4033(7) 0.3159(12) 0.018(5) Uiso 1 1 d . . . . .
O39 O 0.542(2) 0.4049(8) 0.0470(14) 0.024(5) Uiso 1 1 d . . . . .
O40 O 0.541(2) 0.4748(7) 0.3874(13) 0.018(5) Uiso 1 1 d . . . . .
O41 O 0.903(4) 0.2585(14) 0.440(3) 0.078(12) Uiso 1 1 d . . . . .
O42 O 0.605(2) 0.3642(7) 0.1913(13) 0.018(5) Uiso 1 1 d . . . . .
O43 O 0.674(2) 0.5878(7) 0.2537(12) 0.017(5) Uiso 1 1 d . . . . .
O44 O 0.698(2) 0.3234(8) 0.3405(13) 0.023(5) Uiso 1 1 d . . . . .
O45 O 0.283(2) 0.4595(7) 0.2181(13) 0.019(5) Uiso 1 1 d . . . . .
O46 O 0.357(2) 0.2246(8) 0.2549(14) 0.023(5) Uiso 1 1 d . . . . .
O47 O 0.928(2) 0.3350(8) 0.3168(15) 0.030(6) Uiso 1 1 d . . . . .
O48 O 0.4653(19) 0.5191(7) 0.2532(12) 0.017(5) Uiso 1 1 d . . . . .
O49 O 0.677(2) 0.3342(8) 0.0747(13) 0.023(5) Uiso 1 1 d . . . . .
O50 O 0.217(2) 0.2951(8) 0.0050(14) 0.028(6) Uiso 1 1 d . . . . .
O51 O 0.452(2) 0.3105(8) 0.0719(14) 0.027(5) Uiso 1 1 d . . . . .
O52 O 0.5010(19) 0.2786(7) 0.3545(12) 0.016(4) Uiso 1 1 d . . . . .
O53 O 0.781(2) 0.4090(8) 0.0360(15) 0.028(6) Uiso 1 1 d . . . . .
O54 O 0.752(2) 0.2966(8) 0.2098(14) 0.025(5) Uiso 1 1 d . . . . .
O55 O 0.827(2) 0.3762(8) 0.1826(14) 0.027(5) Uiso 1 1 d . . . . .
O56 O 0.370(2) 0.4566(7) -0.0489(13) 0.018(5) Uiso 1 1 d . . . . .
O57 O 0.650(2) 0.3122(8) 0.4893(14) 0.025(5) Uiso 1 1 d . . . . .
N1 N 0.623(3) 0.5504(10) 0.4828(17) 0.025(6) Uiso 1 1 d . U . . .
N2 N 0.008(4) 0.4412(13) 0.318(2) 0.045(9) Uiso 1 1 d . U . . .
C1 C 0.074(3) 0.4943(12) 0.419(2) 0.025(7) Uiso 1 1 d . U . . .
C2 C -0.092(3) 0.5523(11) 0.237(2) 0.024(7) Uiso 1 1 d . U . . .
C3 C 0.038(4) 0.5733(14) 0.403(2) 0.037(9) Uiso 1 1 d . U . . .
C4 C -0.038(4) 0.4735(14) 0.271(2) 0.036(9) Uiso 1 1 d . U . . .
C5 C 0.020(3) 0.5278(11) 0.369(2) 0.023(7) Uiso 1 1 d . U . . .
C6 C 0.514(3) 0.5624(10) 0.4877(17) 0.014(6) Uiso 1 1 d . U . . .
C7 C 0.061(3) 0.4518(12) 0.394(2) 0.027(8) Uiso 1 1 d . U . . .
C8 C 0.410(3) 0.6298(11) 0.3175(19) 0.021(7) Uiso 1 1 d . U . . .
C9 C 0.449(3) 0.5863(10) 0.4335(18) 0.016(6) Uiso 1 1 d . U . . .
C10 C 0.497(3) 0.6019(11) 0.3743(19) 0.019(7) Uiso 1 1 d . U . . .
C11 C 0.609(3) 0.5925(11) 0.369(2) 0.023(7) Uiso 1 1 d . U . . .
C12 C -0.031(3) 0.5179(12) 0.294(2) 0.026(8) Uiso 1 1 d . U . . .
C13 C 0.671(3) 0.6112(11) 0.309(2) 0.023(7) Uiso 1 1 d . U . . .
C14 C 0.676(3) 0.5673(11) 0.4261(19) 0.021(7) Uiso 1 1 d . U . . .
O58 O 0.920(2) 0.4498(8) -0.0096(14) 0.024(5) Uiso 1 1 d . . . . .
O59 O 0.093(3) 0.4845(11) -0.0507(19) 0.051(8) Uiso 1 1 d . . . . .
O60 O 0.190(3) 0.6961(13) 0.034(2) 0.063(10) Uiso 1 1 d . . . . .
O61 O -0.170(4) 0.1916(13) 0.037(2) 0.066(10) Uiso 1 1 d . . . . .
O62 O 0.021(4) 0.6205(13) 0.032(2) 0.070(11) Uiso 1 1 d . . . . .
O63 O 0.767(3) 0.4600(10) -0.1135(17) 0.040(7) Uiso 1 1 d . . . . .
O64 O 0.479(4) 0.6667(16) 0.082(3) 0.087(14) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O19 1.74(2) . ?
W1 O25 2.25(2) . ?
W1 O26 2.10(2) . ?
W1 O40 1.95(2) . ?
W1 O45 1.93(2) . ?
W1 O48 1.76(2) . ?
W2 O8 1.78(2) . ?
W2 O21 2.10(2) . ?
W2 O25 2.24(2) . ?
W2 O33 1.73(2) . ?
W2 O38 1.91(2) . ?
W2 O40 1.97(2) . ?
W3 K2 3.924(12) . ?
W3 K4 3.81(2) 1_455 ?
W3 O16 1.93(2) . ?
W3 O22 2.32(2) . ?
W3 O24 1.71(2) . ?
W3 O26 1.80(2) . ?
W3 O30 1.97(2) . ?
W3 O36 1.92(2) . ?
W4 K2 3.855(12) . ?
W4 O9 1.94(2) . ?
W4 O16 1.91(2) . ?
W4 O23 2.32(2) . ?
W4 O28 1.70(2) . ?
W4 O32 1.90(2) . ?
W4 O45 1.89(2) . ?
W5 O23 2.30(2) . ?
W5 O29 1.75(2) . ?
W5 O32 2.02(2) . ?
W5 O37 2.07(2) . ?
W5 O39 1.88(2) . ?
W5 O56 1.74(2) . ?
W6 K1 3.697(15) . ?
W6 O21 1.79(2) . ?
W6 O22 2.349(19) . ?
W6 O36 1.90(2) . ?
W6 O44 1.94(2) . ?
W6 O52 1.98(2) . ?
W6 O57 1.76(2) . ?
W7 K2 3.981(12) . ?
W7 K3 3.90(2) 3_565 ?
W7 O9 1.92(2) . ?
W7 O23 2.41(2) . ?
W7 O27 1.92(2) . ?
W7 O37 1.87(2) . ?
W7 O50 1.67(3) . ?
W7 O51 1.88(3) . ?
W8 K1 3.841(15) . ?
W8 K2 3.994(12) . ?
W8 O22 2.305(19) . ?
W8 O27 1.93(2) . ?
W8 O30 1.92(2) . ?
W8 O31 1.89(2) . ?
W8 O46 1.70(2) . ?
W8 O52 1.88(2) . ?
W9 O35 1.73(2) . ?
W9 O39 1.93(2) . ?
W9 O42 2.37(2) . ?
W9 O49 2.05(2) . ?
W9 O53 1.67(3) . ?
W9 O55 1.91(3) . ?
W10 K1 3.941(15) . ?
W10 K2 3.793(12) 1_655 ?
W10 O38 1.90(2) . ?
W10 O42 2.35(2) . ?
W10 O44 1.90(2) . ?
W10 O47 1.68(3) . ?
W10 O54 1.92(2) . ?
W10 O55 1.96(3) . ?
W11 O31 1.94(2) . ?
W11 O34 1.68(3) . ?
W11 O42 2.39(2) . ?
W11 O49 1.85(2) . ?
W11 O51 1.95(3) . ?
W11 O54 1.93(2) . ?
Pr1 K3 4.12(2) 1_655 ?
Pr1 O2 2.59(2) . ?
Pr1 O8 2.38(2) . ?
Pr1 O12 2.47(3) 1_655 ?
Pr1 O29 2.44(2) . ?
Pr1 O35 2.44(2) . ?
Pr1 O43 2.48(2) . ?
Pr1 O48 2.41(2) . ?
Pr1 O56 2.46(2) 3_665 ?
Pr2 K3 4.34(2) . ?
Pr2 O1 2.42(3) . ?
Pr2 O4 2.49(3) . ?
Pr2 O10 2.60(3) . ?
Pr2 O11 2.53(2) . ?
Pr2 O13 2.58(3) . ?
Pr2 O15 2.42(3) . ?
Pr2 O17 2.50(3) . ?
Pr2 O20 2.52(3) . ?
Pr2 O46 2.57(2) 2 ?
K1 K3 2.72(3) 2_545 ?
K1 O17 3.07(3) 2_545 ?
K1 O20 2.95(4) 2_545 ?
K1 O31 3.12(3) . ?
K1 O41 2.71(5) . ?
K1 O44 2.81(3) . ?
K1 O50 3.02(3) 4_666 ?
K1 O52 2.80(3) . ?
K1 O54 3.21(3) . ?
K2 W10 3.793(12) 1_455 ?
K2 O7 2.73(5) . ?
K2 O9 2.97(2) . ?
K2 O16 2.88(2) . ?
K2 O18 2.69(8) . ?
K2 O27 3.04(3) . ?
K2 O30 2.99(2) . ?
K2 O47 3.01(3) 1_455 ?
K2 O55 3.27(3) 1_455 ?
K3 W7 3.90(2) 3_565 ?
K3 Pr1 4.12(2) 1_455 ?
K3 K1 2.72(3) 2 ?
K3 O6 3.24(3) 1_455 ?
K3 O13 2.98(4) . ?
K3 O17 3.20(4) . ?
K3 O20 2.64(4) . ?
K3 O37 2.71(3) 3_565 ?
K3 O43 2.78(3) 1_455 ?
K3 O50 3.43(3) 3_565 ?
K3 C13 3.31(4) 1_455 ?
K3 O64 3.09(5) 1_455 ?
K4 W3 3.81(2) 1_655 ?
K4 K2 4.27(3) 1_655 ?
K4 O5 3.00(6) . ?
K4 O18 2.78(8) 1_655 ?
K4 O24 2.93(3) 1_655 ?
K4 O30 3.06(3) 1_655 ?
K4 O34 3.02(4) 4_666 ?
K4 O41 2.78(5) . ?
K4 O47 3.34(4) . ?
K4 O60 3.07(5) 2_645 ?
K4 O61 2.83(5) 4_766 ?
Si2 O22 1.67(2) . ?
Si2 O23 1.66(2) . ?
Si2 O25 1.64(2) . ?
Si2 O42 1.62(2) . ?
O1 C8 1.20(4) . ?
O3 C8 1.27(4) . ?
O6 K3 3.24(3) 1_655 ?
O6 C13 1.20(4) . ?
O12 Pr1 2.47(3) 1_455 ?
O12 C2 1.24(4) . ?
O13 C2 1.22(4) . ?
O14 C3 1.32(5) . ?
O15 C3 1.20(5) . ?
O17 K1 3.07(3) 2 ?
O18 K4 2.78(8) 1_455 ?
O20 K1 2.95(4) 2 ?
O24 K4 2.93(3) 1_455 ?
O30 K4 3.06(3) 1_455 ?
O34 K4 3.02(4) 4_565 ?
O37 K3 2.71(3) 3_565 ?
O43 K3 2.78(3) 1_655 ?
O43 C13 1.23(4) . ?
O46 Pr2 2.57(2) 2_545 ?
O47 K2 3.01(3) 1_655 ?
O50 K1 3.02(3) 4_565 ?
O50 K3 3.43(3) 3_565 ?
O55 K2 3.27(3) 1_655 ?
O56 Pr1 2.46(2) 3_665 ?
N1 C6 1.32(4) . ?
N1 C14 1.39(4) . ?
N2 C4 1.33(5) . ?
N2 C7 1.41(5) . ?
C1 C5 1.41(5) . ?
C1 C7 1.37(5) . ?
C2 C12 1.53(5) . ?
C3 C5 1.51(5) . ?
C4 C12 1.41(5) . ?
C5 C12 1.38(5) . ?
C6 C9 1.31(4) . ?
C8 C10 1.53(5) . ?
C9 C10 1.38(4) . ?
C10 C11 1.33(5) . ?
C11 C13 1.51(5) . ?
C11 C14 1.38(5) . ?
C13 K3 3.31(4) 1_655 ?
O60 K4 3.07(5) 2_655 ?
O61 K4 2.83(5) 4_465 ?
O64 K3 3.09(5) 1_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O19 W1 O25 167.6(9) . . ?
O19 W1 O26 89.8(9) . . ?
O19 W1 O40 96.1(10) . . ?
O19 W1 O45 101.1(10) . . ?
O19 W1 O48 103.5(10) . . ?
O26 W1 O25 81.9(8) . . ?
O40 W1 O25 74.1(8) . . ?
O40 W1 O26 84.5(8) . . ?
O45 W1 O25 86.6(8) . . ?
O45 W1 O26 80.6(9) . . ?
O45 W1 O40 157.1(9) . . ?
O48 W1 O25 85.1(9) . . ?
O48 W1 O26 166.7(9) . . ?
O48 W1 O40 94.8(10) . . ?
O48 W1 O45 95.7(10) . . ?
O8 W2 O21 164.7(9) . . ?
O8 W2 O25 84.2(9) . . ?
O8 W2 O38 95.8(10) . . ?
O8 W2 O40 95.2(9) . . ?
O21 W2 O25 80.9(8) . . ?
O33 W2 O8 102.7(10) . . ?
O33 W2 O21 92.6(10) . . ?
O33 W2 O25 169.7(10) . . ?
O33 W2 O38 100.4(10) . . ?
O33 W2 O40 97.7(10) . . ?
O38 W2 O21 80.0(9) . . ?
O38 W2 O25 86.3(8) . . ?
O38 W2 O40 156.1(9) . . ?
O40 W2 O21 83.8(8) . . ?
O40 W2 O25 73.8(8) . . ?
K4 W3 K2 67.0(4) 1_455 . ?
O16 W3 K2 44.5(6) . . ?
O16 W3 K4 109.2(7) . 1_455 ?
O16 W3 O22 86.5(8) . . ?
O16 W3 O30 85.5(8) . . ?
O22 W3 K2 95.8(5) . . ?
O22 W3 K4 120.6(6) . 1_455 ?
O24 W3 K2 82.2(8) . . ?
O24 W3 K4 47.2(8) . 1_455 ?
O24 W3 O16 100.3(10) . . ?
O24 W3 O22 167.5(9) . . ?
O24 W3 O26 104.0(10) . . ?
O24 W3 O30 97.1(10) . . ?
O24 W3 O36 99.0(10) . . ?
O26 W3 K2 132.1(7) . . ?
O26 W3 K4 147.5(7) . 1_455 ?
O26 W3 O16 88.3(9) . . ?
O26 W3 O22 86.6(8) . . ?
O26 W3 O30 158.7(9) . . ?
O26 W3 O36 93.6(9) . . ?
O30 W3 K2 48.1(6) . . ?
O30 W3 K4 53.1(7) . 1_455 ?
O30 W3 O22 72.7(8) . . ?
O36 W3 K2 132.9(7) . . ?
O36 W3 K4 79.5(8) . 1_455 ?
O36 W3 O16 159.5(9) . . ?
O36 W3 O22 73.3(8) . . ?
O36 W3 O30 85.5(9) . . ?
O9 W4 K2 49.2(6) . . ?
O9 W4 O23 74.9(8) . . ?
O16 W4 K2 46.2(6) . . ?
O16 W4 O9 87.8(9) . . ?
O16 W4 O23 88.8(8) . . ?
O23 W4 K2 99.4(6) . . ?
O28 W4 K2 83.0(8) . . ?
O28 W4 O9 98.8(10) . . ?
O28 W4 O16 100.9(10) . . ?
O28 W4 O23 168.3(9) . . ?
O28 W4 O32 96.6(10) . . ?
O28 W4 O45 103.1(10) . . ?
O32 W4 K2 134.7(7) . . ?
O32 W4 O9 86.7(9) . . ?
O32 W4 O16 162.2(9) . . ?
O32 W4 O23 73.4(8) . . ?
O45 W4 K2 133.9(7) . . ?
O45 W4 O9 158.2(9) . . ?
O45 W4 O16 88.3(9) . . ?
O45 W4 O23 83.6(9) . . ?
O45 W4 O32 90.5(9) . . ?
O29 W5 O23 90.9(9) . . ?
O29 W5 O32 91.5(10) . . ?
O29 W5 O37 162.6(10) . . ?
O29 W5 O39 94.9(10) . . ?
O32 W5 O23 72.1(8) . . ?
O32 W5 O37 82.1(9) . . ?
O37 W5 O23 71.8(8) . . ?
O39 W5 O23 84.4(9) . . ?
O39 W5 O32 155.7(10) . . ?
O39 W5 O37 85.0(10) . . ?
O56 W5 O23 162.6(9) . . ?
O56 W5 O29 104.5(10) . . ?
O56 W5 O32 99.0(10) . . ?
O56 W5 O37 92.5(10) . . ?
O56 W5 O39 102.0(10) . . ?
O21 W6 K1 135.2(7) . . ?
O21 W6 O22 85.8(8) . . ?
O21 W6 O36 93.7(9) . . ?
O21 W6 O44 87.9(9) . . ?
O21 W6 O52 157.2(9) . . ?
O22 W6 K1 98.2(5) . . ?
O36 W6 K1 130.2(7) . . ?
O36 W6 O22 72.9(8) . . ?
O36 W6 O44 158.3(10) . . ?
O36 W6 O52 83.4(9) . . ?
O44 W6 K1 48.4(7) . . ?
O44 W6 O22 85.7(8) . . ?
O44 W6 O52 86.7(9) . . ?
O52 W6 K1 48.3(7) . . ?
O52 W6 O22 71.7(8) . . ?
O57 W6 K1 79.0(8) . . ?
O57 W6 O21 104.4(10) . . ?
O57 W6 O22 168.3(9) . . ?
O57 W6 O36 100.1(11) . . ?
O57 W6 O44 100.4(11) . . ?
O57 W6 O52 98.4(10) . . ?
K3 W7 K2 129.6(4) 3_565 . ?
O9 W7 K2 45.6(6) . . ?
O9 W7 K3 100.6(7) . 3_565 ?
O9 W7 O23 73.0(8) . . ?
O23 W7 K2 94.5(5) . . ?
O23 W7 K3 111.2(6) . 3_565 ?
O27 W7 K2 47.6(7) . . ?
O27 W7 K3 163.9(7) . 3_565 ?
O27 W7 O9 86.0(9) . . ?
O27 W7 O23 84.7(8) . . ?
O37 W7 K2 134.1(7) . . ?
O37 W7 K3 38.9(8) . 3_565 ?
O37 W7 O9 88.8(9) . . ?
O37 W7 O23 72.4(9) . . ?
O37 W7 O27 157.0(10) . . ?
O37 W7 O51 89.0(11) . . ?
O50 W7 K2 85.4(9) . . ?
O50 W7 K3 61.4(9) . 3_565 ?
O50 W7 O9 99.5(11) . . ?
O50 W7 O23 168.9(10) . . ?
O50 W7 O27 103.2(11) . . ?
O50 W7 O37 99.7(11) . . ?
O50 W7 O51 101.4(12) . . ?
O51 W7 K2 135.0(8) . . ?
O51 W7 K3 90.6(8) . 3_565 ?
O51 W7 O9 159.1(10) . . ?
O51 W7 O23 86.5(9) . . ?
O51 W7 O27 87.9(10) . . ?
K1 W8 K2 168.8(3) . . ?
O22 W8 K1 95.1(5) . . ?
O22 W8 K2 94.1(5) . . ?
O27 W8 K1 139.9(7) . . ?
O27 W8 K2 47.4(7) . . ?
O27 W8 O22 84.9(8) . . ?
O30 W8 K1 131.8(7) . . ?
O30 W8 K2 45.9(6) . . ?
O30 W8 O22 73.9(8) . . ?
O30 W8 O27 86.8(9) . . ?
O31 W8 K1 53.6(7) . . ?
O31 W8 K2 133.9(7) . . ?
O31 W8 O22 83.7(8) . . ?
O31 W8 O27 86.7(9) . . ?
O31 W8 O30 157.1(9) . . ?
O46 W8 K1 81.8(8) . . ?
O46 W8 K2 88.2(8) . . ?
O46 W8 O22 172.0(9) . . ?
O46 W8 O27 102.2(10) . . ?
O46 W8 O30 102.7(10) . . ?
O46 W8 O31 100.2(10) . . ?
O46 W8 O52 98.5(10) . . ?
O52 W8 K1 43.8(7) . . ?
O52 W8 K2 134.1(7) . . ?
O52 W8 O22 74.4(8) . . ?
O52 W8 O27 159.3(9) . . ?
O52 W8 O30 88.6(9) . . ?
O52 W8 O31 89.7(9) . . ?
O35 W9 O39 90.7(10) . . ?
O35 W9 O42 91.7(9) . . ?
O35 W9 O49 162.2(10) . . ?
O35 W9 O55 95.7(11) . . ?
O39 W9 O42 81.5(9) . . ?
O39 W9 O49 83.2(10) . . ?
O49 W9 O42 70.8(8) . . ?
O53 W9 O35 103.9(12) . . ?
O53 W9 O39 101.5(11) . . ?
O53 W9 O42 164.0(10) . . ?
O53 W9 O49 93.8(11) . . ?
O53 W9 O55 100.2(12) . . ?
O55 W9 O39 155.1(10) . . ?
O55 W9 O42 74.3(9) . . ?
O55 W9 O49 83.4(10) . . ?
K2 W10 K1 94.8(3) 1_655 . ?
O38 W10 K1 128.2(7) . . ?
O38 W10 K2 129.0(7) . 1_655 ?
O38 W10 O42 83.6(9) . . ?
O38 W10 O44 87.4(10) . . ?
O38 W10 O54 159.0(10) . . ?
O38 W10 O55 90.8(10) . . ?
O42 W10 K1 98.1(6) . . ?
O42 W10 K2 120.1(6) . 1_655 ?
O44 W10 K1 41.4(7) . . ?
O44 W10 K2 133.8(7) . 1_655 ?
O44 W10 O42 86.9(9) . . ?
O44 W10 O54 88.5(10) . . ?
O44 W10 O55 160.8(10) . . ?
O47 W10 K1 84.9(9) . . ?
O47 W10 K2 50.1(9) . 1_655 ?
O47 W10 O38 101.9(11) . . ?
O47 W10 O42 170.1(11) . . ?
O47 W10 O44 101.4(11) . . ?
O47 W10 O54 99.1(11) . . ?
O47 W10 O55 97.6(12) . . ?
O54 W10 K1 53.8(8) . . ?
O54 W10 K2 66.4(8) . 1_655 ?
O54 W10 O42 75.6(9) . . ?
O54 W10 O55 86.4(10) . . ?
O55 W10 K1 139.8(8) . . ?
O55 W10 K2 59.6(8) . 1_655 ?
O55 W10 O42 74.0(9) . . ?
O31 W11 O42 81.3(8) . . ?
O31 W11 O51 85.4(10) . . ?
O34 W11 O31 102.0(11) . . ?
O34 W11 O42 173.1(11) . . ?
O34 W11 O49 103.7(12) . . ?
O34 W11 O51 100.9(12) . . ?
O34 W11 O54 99.7(12) . . ?
O49 W11 O31 154.4(10) . . ?
O49 W11 O42 73.3(9) . . ?
O49 W11 O51 89.3(10) . . ?
O49 W11 O54 89.1(10) . . ?
O51 W11 O42 85.3(9) . . ?
O54 W11 O31 87.0(10) . . ?
O54 W11 O42 74.3(9) . . ?
O54 W11 O51 159.1(10) . . ?
O2 Pr1 K3 62.3(6) . 1_655 ?
O8 Pr1 K3 111.5(6) . 1_655 ?
O8 Pr1 O2 135.0(7) . . ?
O8 Pr1 O12 78.1(8) . 1_655 ?
O8 Pr1 O29 116.3(7) . . ?
O8 Pr1 O35 76.9(7) . . ?
O8 Pr1 O43 78.9(7) . . ?
O8 Pr1 O48 74.0(7) . . ?
O8 Pr1 O56 150.4(7) . 3_665 ?
O12 Pr1 K3 56.6(7) 1_655 1_655 ?
O12 Pr1 O2 118.3(8) 1_655 . ?
O12 Pr1 O43 70.3(8) 1_655 . ?
O29 Pr1 K3 131.8(6) . 1_655 ?
O29 Pr1 O2 79.5(7) . . ?
O29 Pr1 O12 139.5(8) . 1_655 ?
O29 Pr1 O35 70.0(7) . . ?
O29 Pr1 O43 146.6(7) . . ?
O29 Pr1 O56 79.2(7) . 3_665 ?
O35 Pr1 K3 128.6(6) . 1_655 ?
O35 Pr1 O2 144.4(8) . . ?
O35 Pr1 O12 77.8(8) . 1_655 ?
O35 Pr1 O43 143.2(7) . . ?
O35 Pr1 O56 86.3(7) . 3_665 ?
O43 Pr1 K3 41.0(6) . 1_655 ?
O43 Pr1 O2 70.0(7) . . ?
O48 Pr1 K3 113.2(6) . 1_655 ?
O48 Pr1 O2 69.8(7) . . ?
O48 Pr1 O12 143.2(8) . 1_655 ?
O48 Pr1 O29 75.7(7) . . ?
O48 Pr1 O35 117.6(7) . . ?
O48 Pr1 O43 81.1(7) . . ?
O48 Pr1 O56 135.6(7) . 3_665 ?
O56 Pr1 K3 61.4(6) 3_665 1_655 ?
O56 Pr1 O2 70.0(7) 3_665 . ?
O56 Pr1 O12 74.6(8) 3_665 1_655 ?
O56 Pr1 O43 102.1(7) 3_665 . ?
O1 Pr2 K3 172.6(7) . . ?
O1 Pr2 O4 75.4(9) . . ?
O1 Pr2 O10 73.1(8) . . ?
O1 Pr2 O11 70.1(8) . . ?
O1 Pr2 O13 141.1(9) . . ?
O1 Pr2 O17 138.2(9) . . ?
O1 Pr2 O20 139.2(10) . . ?
O1 Pr2 O46 83.7(8) . 2 ?
O4 Pr2 K3 102.8(7) . . ?
O4 Pr2 O10 67.5(9) . . ?
O4 Pr2 O11 133.9(9) . . ?
O4 Pr2 O13 72.0(9) . . ?
O4 Pr2 O17 139.7(10) . . ?
O4 Pr2 O20 99.9(10) . . ?
O4 Pr2 O46 136.9(9) . 2 ?
O10 Pr2 K3 99.5(6) . . ?
O11 Pr2 K3 114.9(6) . . ?
O11 Pr2 O10 126.7(8) . . ?
O11 Pr2 O13 120.9(8) . . ?
O11 Pr2 O46 68.3(8) . 2 ?
O13 Pr2 K3 42.0(7) . . ?
O13 Pr2 O10 112.0(9) . . ?
O15 Pr2 K3 106.0(7) . . ?
O15 Pr2 O1 80.6(9) . . ?
O15 Pr2 O4 73.5(9) . . ?
O15 Pr2 O10 137.0(9) . . ?
O15 Pr2 O11 71.5(8) . . ?
O15 Pr2 O13 70.3(9) . . ?
O15 Pr2 O17 89.0(9) . . ?
O15 Pr2 O20 138.0(10) . . ?
O15 Pr2 O46 139.7(8) . 2 ?
O17 Pr2 K3 46.8(7) . . ?
O17 Pr2 O10 132.8(9) . . ?
O17 Pr2 O11 68.2(9) . . ?
O17 Pr2 O13 67.9(9) . . ?
O17 Pr2 O20 69.2(10) . . ?
O17 Pr2 O46 78.6(9) . 2 ?
O20 Pr2 K3 33.6(9) . . ?
O20 Pr2 O10 68.0(10) . . ?
O20 Pr2 O11 126.2(9) . . ?
O20 Pr2 O13 68.2(10) . . ?
O20 Pr2 O46 72.4(9) . 2 ?
O46 Pr2 K3 93.1(6) 2 . ?
O46 Pr2 O10 70.5(8) 2 . ?
O46 Pr2 O13 135.0(8) 2 . ?
W6 K1 W8 53.0(2) . . ?
W6 K1 W10 57.6(2) . . ?
W8 K1 W10 78.8(3) . . ?
K3 K1 W6 153.8(7) 2_545 . ?
K3 K1 W8 124.3(7) 2_545 . ?
K3 K1 W10 147.2(7) 2_545 . ?
K3 K1 O17 66.9(8) 2_545 2_545 ?
K3 K1 O20 55.3(9) 2_545 2_545 ?
K3 K1 O31 126.4(8) 2_545 . ?
K3 K1 O44 169.3(9) 2_545 . ?
K3 K1 O50 73.0(8) 2_545 4_666 ?
K3 K1 O52 132.0(9) 2_545 . ?
K3 K1 O54 126.3(8) 2_545 . ?
O17 K1 W6 121.5(7) 2_545 . ?
O17 K1 W8 68.9(6) 2_545 . ?
O17 K1 W10 108.8(7) 2_545 . ?
O17 K1 O31 59.6(7) 2_545 . ?
O17 K1 O54 81.4(8) 2_545 . ?
O20 K1 W6 106.3(8) 2_545 . ?
O20 K1 W8 72.7(7) 2_545 . ?
O20 K1 W10 151.1(8) 2_545 . ?
O20 K1 O17 56.5(9) 2_545 2_545 ?
O20 K1 O31 90.5(9) 2_545 . ?
O20 K1 O50 70.1(9) 2_545 4_666 ?
O20 K1 O54 134.4(10) 2_545 . ?
O31 K1 W6 66.0(5) . . ?
O31 K1 W8 29.2(4) . . ?
O31 K1 W10 61.6(5) . . ?
O31 K1 O54 49.8(6) . . ?
O41 K1 W6 83.2(10) . . ?
O41 K1 W8 136.0(11) . . ?
O41 K1 W10 72.6(10) . . ?
O41 K1 K3 96.6(12) . 2_545 ?
O41 K1 O17 152.4(13) . 2_545 ?
O41 K1 O20 132.8(13) . 2_545 ?
O41 K1 O31 133.5(11) . . ?
O41 K1 O44 73.4(11) . . ?
O41 K1 O50 65.3(11) . 4_666 ?
O41 K1 O52 112.7(12) . . ?
O41 K1 O54 92.5(11) . . ?
O44 K1 W6 31.2(5) . . ?
O44 K1 W8 66.3(6) . . ?
O44 K1 W10 26.6(5) . . ?
O44 K1 O17 120.7(9) . 2_545 ?
O44 K1 O20 134.6(10) . 2_545 ?
O44 K1 O31 62.2(7) . . ?
O44 K1 O50 105.2(8) . 4_666 ?
O44 K1 O54 52.1(7) . . ?
O50 K1 W6 83.4(6) 4_666 . ?
O50 K1 W8 108.7(6) 4_666 . ?
O50 K1 W10 125.1(7) 4_666 . ?
O50 K1 O17 124.9(9) 4_666 2_545 ?
O50 K1 O31 137.6(8) 4_666 . ?
O50 K1 O54 153.6(8) 4_666 . ?
O52 K1 W6 31.9(5) . . ?
O52 K1 W8 27.7(5) . . ?
O52 K1 W10 79.7(6) . . ?
O52 K1 O17 94.4(8) . 2_545 ?
O52 K1 O20 77.3(9) . 2_545 ?
O52 K1 O31 53.0(6) . . ?
O52 K1 O44 57.3(7) . . ?
O52 K1 O50 85.5(8) . 4_666 ?
O52 K1 O54 90.7(7) . . ?
O54 K1 W6 79.7(5) . . ?
O54 K1 W8 76.6(5) . . ?
O54 K1 W10 28.9(5) . . ?
W3 K2 W7 79.2(2) . . ?
W4 K2 W3 56.32(17) . . ?
W4 K2 W7 50.91(15) . . ?
W10 K2 W3 95.0(3) 1_455 . ?
W10 K2 W4 100.7(3) 1_455 . ?
W10 K2 W7 149.2(3) 1_455 . ?
O7 K2 W3 147.0(11) . . ?
O7 K2 W4 108.9(11) . . ?
O7 K2 W7 70.2(11) . . ?
O7 K2 W10 117.6(11) . 1_455 ?
O7 K2 O9 80.1(11) . . ?
O7 K2 O16 133.7(12) . . ?
O7 K2 O27 82.8(12) . . ?
O7 K2 O30 126.8(12) . . ?
O7 K2 O47 139.0(12) . 1_455 ?
O7 K2 O55 105.8(12) . 1_455 ?
O9 K2 W3 78.2(5) . . ?
O9 K2 W4 29.6(4) . . ?
O9 K2 W7 27.5(4) . . ?
O9 K2 W10 121.8(5) . 1_455 ?
O9 K2 O27 51.7(6) . . ?
O9 K2 O30 89.6(7) . . ?
O9 K2 O47 127.8(7) . 1_455 ?
O9 K2 O55 92.4(7) . 1_455 ?
O16 K2 W3 28.1(4) . . ?
O16 K2 W4 28.6(4) . . ?
O16 K2 W7 65.3(5) . . ?
O16 K2 W10 95.6(5) . 1_455 ?
O16 K2 O9 54.3(6) . . ?
O16 K2 O27 63.7(6) . . ?
O16 K2 O30 53.7(6) . . ?
O16 K2 O47 83.3(7) . 1_455 ?
O16 K2 O55 85.9(7) . 1_455 ?
O18 K2 W3 88.1(17) . . ?
O18 K2 W4 143.0(17) . . ?
O18 K2 W7 118.5(17) . . ?
O18 K2 W10 91.2(17) . 1_455 ?
O18 K2 O7 96(2) . . ?
O18 K2 O9 145.0(18) . . ?
O18 K2 O16 116.1(18) . . ?
O18 K2 O27 93.3(18) . . ?
O18 K2 O30 65.0(17) . . ?
O18 K2 O47 77.0(18) . 1_455 ?
O18 K2 O55 121.9(18) . 1_455 ?
O27 K2 W3 64.3(5) . . ?
O27 K2 W4 64.1(5) . . ?
O27 K2 W7 27.9(4) . . ?
O27 K2 W10 158.6(6) . 1_455 ?
O27 K2 O55 141.8(7) . 1_455 ?
O30 K2 W3 29.4(4) . . ?
O30 K2 W4 78.1(5) . . ?
O30 K2 W7 77.0(5) . . ?
O30 K2 W10 112.1(5) . 1_455 ?
O30 K2 O27 52.1(6) . . ?
O30 K2 O47 87.0(7) . 1_455 ?
O30 K2 O55 126.8(7) . 1_455 ?
O47 K2 W3 73.8(6) 1_455 . ?
O47 K2 W4 99.5(6) 1_455 . ?
O47 K2 W7 148.5(6) 1_455 . ?
O47 K2 W10 25.3(5) 1_455 1_455 ?
O47 K2 O27 137.3(8) 1_455 . ?
O47 K2 O55 51.6(7) 1_455 1_455 ?
O55 K2 W3 99.7(5) 1_455 . ?
O55 K2 W4 78.1(5) 1_455 . ?
O55 K2 W7 119.5(5) 1_455 . ?
O55 K2 W10 31.1(5) 1_455 1_455 ?
W7 K3 Pr1 110.3(5) 3_565 1_455 ?
K1 K3 W7 81.2(6) 2 3_565 ?
K1 K3 Pr1 164.6(9) 2 1_455 ?
K1 K3 O6 88.0(8) 2 1_455 ?
K1 K3 O13 111.8(10) 2 . ?
K1 K3 O17 61.8(8) 2 . ?
K1 K3 O43 130.1(10) 2 1_455 ?
K1 K3 O50 57.6(7) 2 3_565 ?
K1 K3 C13 108.9(10) 2 1_455 ?
K1 K3 O64 89.2(11) 2 1_455 ?
O6 K3 W7 160.8(9) 1_455 3_565 ?
O6 K3 Pr1 78.0(6) 1_455 1_455 ?
O6 K3 O50 145.1(10) 1_455 3_565 ?
O6 K3 C13 21.2(8) 1_455 1_455 ?
O13 K3 W7 129.1(9) . 3_565 ?
O13 K3 Pr1 69.5(7) . 1_455 ?
O13 K3 O6 69.7(9) . 1_455 ?
O13 K3 O17 54.4(9) . . ?
O13 K3 O50 125.5(10) . 3_565 ?
O13 K3 C13 65.8(9) . 1_455 ?
O13 K3 O64 151.8(13) . 1_455 ?
O17 K3 W7 133.5(9) . 3_565 ?
O17 K3 Pr1 112.0(8) . 1_455 ?
O17 K3 O6 50.3(8) . 1_455 ?
O17 K3 O50 109.1(9) . 3_565 ?
O17 K3 C13 66.5(9) . 1_455 ?
O20 K3 W7 83.5(9) . 3_565 ?
O20 K3 Pr1 123.3(10) . 1_455 ?
O20 K3 K1 66.8(10) . 2 ?
O20 K3 O6 106.8(11) . 1_455 ?
O20 K3 O13 60.8(10) . . ?
O20 K3 O17 57.4(10) . . ?
O20 K3 O37 97.0(12) . 3_565 ?
O20 K3 O43 121.9(12) . 1_455 ?
O20 K3 O50 67.4(10) . 3_565 ?
O20 K3 C13 117.7(12) . 1_455 ?
O20 K3 O64 147.4(14) . 1_455 ?
O37 K3 W7 25.6(5) 3_565 3_565 ?
O37 K3 Pr1 84.7(7) 3_565 1_455 ?
O37 K3 K1 106.5(10) 3_565 2 ?
O37 K3 O6 155.6(11) 3_565 1_455 ?
O37 K3 O13 119.9(11) 3_565 . ?
O37 K3 O17 154.1(11) 3_565 . ?
O37 K3 O43 119.3(10) 3_565 1_455 ?
O37 K3 O50 50.6(7) 3_565 3_565 ?
O37 K3 C13 137.7(11) 3_565 1_455 ?
O37 K3 O64 67.8(11) 3_565 1_455 ?
O43 K3 W7 144.2(9) 1_455 3_565 ?
O43 K3 Pr1 35.9(5) 1_455 1_455 ?
O43 K3 O6 42.2(7) 1_455 1_455 ?
O43 K3 O13 61.9(9) 1_455 . ?
O43 K3 O17 81.9(9) 1_455 . ?
O43 K3 O50 168.9(10) 1_455 3_565 ?
O43 K3 C13 21.1(8) 1_455 1_455 ?
O43 K3 O64 90.3(12) 1_455 1_455 ?
O50 K3 W7 25.3(5) 3_565 3_565 ?
O50 K3 Pr1 135.2(8) 3_565 1_455 ?
C13 K3 W7 158.5(9) 1_455 3_565 ?
C13 K3 Pr1 56.8(7) 1_455 1_455 ?
C13 K3 O50 163.8(10) 1_455 3_565 ?
O64 K3 W7 70.7(10) 1_455 3_565 ?
O64 K3 Pr1 85.2(10) 1_455 1_455 ?
O64 K3 O6 93.5(12) 1_455 1_455 ?
O64 K3 O17 130.8(13) 1_455 . ?
O64 K3 O50 81.3(11) 1_455 3_565 ?
O64 K3 C13 90.2(12) 1_455 1_455 ?
W3 K4 K2 57.8(4) 1_655 1_655 ?
O5 K4 W3 94.3(12) . 1_655 ?
O5 K4 K2 103.4(12) . 1_655 ?
O5 K4 O30 122.5(14) . 1_655 ?
O5 K4 O34 64.9(13) . 4_666 ?
O5 K4 O47 59.7(12) . . ?
O5 K4 O60 141.6(16) . 2_645 ?
O18 K4 W3 89.2(17) 1_655 1_655 ?
O18 K4 K2 38.0(16) 1_655 1_655 ?
O18 K4 O5 126(2) 1_655 . ?
O18 K4 O24 103.0(18) 1_655 1_655 ?
O18 K4 O30 63.1(17) 1_655 1_655 ?
O18 K4 O34 140.1(19) 1_655 4_666 ?
O18 K4 O47 70.3(17) 1_655 . ?
O18 K4 O60 85.7(18) 1_655 2_645 ?
O18 K4 O61 144(2) 1_655 4_766 ?
O24 K4 W3 25.4(5) 1_655 1_655 ?
O24 K4 K2 65.7(6) 1_655 1_655 ?
O24 K4 O5 68.8(13) 1_655 . ?
O24 K4 O30 55.1(7) 1_655 1_655 ?
O24 K4 O34 115.6(10) 1_655 4_666 ?
O24 K4 O47 58.9(8) 1_655 . ?
O24 K4 O60 130.7(12) 1_655 2_645 ?
O30 K4 W3 31.1(4) 1_655 1_655 ?
O30 K4 K2 44.5(5) 1_655 1_655 ?
O30 K4 O47 80.2(8) 1_655 . ?
O30 K4 O60 89.6(10) 1_655 2_645 ?
O34 K4 W3 130.2(9) 4_666 1_655 ?
O34 K4 K2 164.5(9) 4_666 1_655 ?
O34 K4 O30 150.0(11) 4_666 1_655 ?
O34 K4 O47 121.6(10) 4_666 . ?
O34 K4 O60 76.8(11) 4_666 2_645 ?
O41 K4 W3 134.4(12) . 1_655 ?
O41 K4 K2 94.8(11) . 1_655 ?
O41 K4 O5 54.2(15) . . ?
O41 K4 O18 86(2) . 1_655 ?
O41 K4 O24 113.2(13) . 1_655 ?
O41 K4 O30 139.3(13) . 1_655 ?
O41 K4 O34 70.2(12) . 4_666 ?
O41 K4 O47 63.6(11) . . ?
O41 K4 O60 115.7(14) . 2_645 ?
O41 K4 O61 129.1(15) . 4_766 ?
O47 K4 W3 72.1(6) . 1_655 ?
O47 K4 K2 44.5(6) . 1_655 ?
O60 K4 W3 109.2(10) 2_645 1_655 ?
O60 K4 K2 114.7(10) 2_645 1_655 ?
O60 K4 O47 156.0(12) 2_645 . ?
O61 K4 W3 69.0(9) 4_766 1_655 ?
O61 K4 K2 126.5(11) 4_766 1_655 ?
O61 K4 O5 85.1(15) 4_766 . ?
O61 K4 O24 69.1(10) 4_766 1_655 ?
O61 K4 O30 86.2(11) 4_766 1_655 ?
O61 K4 O34 64.8(11) 4_766 4_666 ?
O61 K4 O47 124.3(12) 4_766 . ?
O61 K4 O60 76.1(12) 4_766 2_645 ?
O23 Si2 O22 109.0(11) . . ?
O25 Si2 O22 108.4(10) . . ?
O25 Si2 O23 111.1(11) . . ?
O42 Si2 O22 109.4(11) . . ?
O42 Si2 O23 106.9(11) . . ?
O42 Si2 O25 112.0(11) . . ?
C8 O1 Pr2 135(2) . . ?
C13 O6 K3 83(2) . 1_655 ?
W2 O8 Pr1 137.1(11) . . ?
W4 O9 K2 101.2(8) . . ?
W7 O9 W4 121.4(11) . . ?
W7 O9 K2 106.9(9) . . ?
C2 O12 Pr1 131(2) . 1_455 ?
Pr2 O13 K3 102.7(10) . . ?
C2 O13 Pr2 141(3) . . ?
C2 O13 K3 108(2) . . ?
C3 O15 Pr2 132(3) . . ?
W3 O16 K2 107.4(8) . . ?
W4 O16 W3 145.2(12) . . ?
W4 O16 K2 105.2(8) . . ?
Pr2 O17 K1 111.8(11) . 2 ?
Pr2 O17 K3 98.5(10) . . ?
K1 O17 K3 51.4(7) 2 . ?
K2 O18 K4 103(3) . 1_455 ?
Pr2 O20 K1 115.0(13) . 2 ?
Pr2 O20 K3 114.5(14) . . ?
K3 O20 K1 57.9(9) . 2 ?
W6 O21 W2 153.1(11) . . ?
W3 O22 W6 91.5(7) . . ?
W8 O22 W3 93.6(7) . . ?
W8 O22 W6 92.7(7) . . ?
Si2 O22 W3 122.9(10) . . ?
Si2 O22 W6 121.3(10) . . ?
Si2 O22 W8 125.8(10) . . ?
W4 O23 W7 90.7(7) . . ?
W5 O23 W4 94.4(8) . . ?
W5 O23 W7 93.8(8) . . ?
Si2 O23 W4 122.8(11) . . ?
Si2 O23 W5 123.4(12) . . ?
Si2 O23 W7 123.1(11) . . ?
W3 O24 K4 107.3(11) . 1_455 ?
W2 O25 W1 94.8(8) . . ?
Si2 O25 W1 126.9(11) . . ?
Si2 O25 W2 127.6(11) . . ?
W3 O26 W1 152.2(11) . . ?
W7 O27 W8 149.3(13) . . ?
W7 O27 K2 104.5(9) . . ?
W8 O27 K2 104.7(9) . . ?
W5 O29 Pr1 155.5(12) . . ?
W3 O30 K2 102.4(8) . . ?
W3 O30 K4 95.8(9) . 1_455 ?
W8 O30 W3 119.7(11) . . ?
W8 O30 K2 106.7(8) . . ?
W8 O30 K4 135.1(10) . 1_455 ?
K2 O30 K4 89.7(7) . 1_455 ?
W8 O31 W11 153.6(13) . . ?
W8 O31 K1 97.2(9) . . ?
W11 O31 K1 108.5(9) . . ?
W4 O32 W5 119.8(11) . . ?
W11 O34 K4 128.4(14) . 4_565 ?
W9 O35 Pr1 161.1(13) . . ?
W6 O36 W3 121.8(12) . . ?
W5 O37 K3 122.4(11) . 3_565 ?
W7 O37 W5 122.0(12) . . ?
W7 O37 K3 115.5(11) . 3_565 ?
W10 O38 W2 155.3(13) . . ?
W5 O39 W9 144.8(14) . . ?
W1 O40 W2 114.7(11) . . ?
K1 O41 K4 133.7(18) . . ?
W9 O42 W11 92.4(8) . . ?
W10 O42 W9 91.0(8) . . ?
W10 O42 W11 89.6(7) . . ?
Si2 O42 W9 124.2(12) . . ?
Si2 O42 W10 123.1(12) . . ?
Si2 O42 W11 126.4(12) . . ?
Pr1 O43 K3 103.1(9) . 1_655 ?
C13 O43 Pr1 151(2) . . ?
C13 O43 K3 105(2) . 1_655 ?
W6 O44 K1 100.4(10) . . ?
W10 O44 W6 146.4(13) . . ?
W10 O44 K1 111.9(11) . . ?
W4 O45 W1 154.1(13) . . ?
W8 O46 Pr2 152.6(13) . 2_545 ?
W10 O47 K2 104.6(11) . 1_655 ?
W10 O47 K4 155.1(14) . . ?
K2 O47 K4 84.4(8) 1_655 . ?
W1 O48 Pr1 135.7(11) . . ?
W11 O49 W9 123.5(12) . . ?
W7 O50 K1 137.6(13) . 4_565 ?
W7 O50 K3 93.4(11) . 3_565 ?
K1 O50 K3 49.4(6) 4_565 3_565 ?
W7 O51 W11 150.1(15) . . ?
W6 O52 K1 99.8(9) . . ?
W8 O52 W6 121.2(11) . . ?
W8 O52 K1 108.5(9) . . ?
W10 O54 W11 120.6(13) . . ?
W10 O54 K1 97.3(9) . . ?
W11 O54 K1 105.6(10) . . ?
W9 O55 W10 120.5(13) . . ?
W9 O55 K2 135.4(11) . 1_655 ?
W10 O55 K2 89.2(9) . 1_655 ?
W5 O56 Pr1 165.5(12) . 3_665 ?
C6 N1 C14 120(3) . . ?
C4 N2 C7 118(4) . . ?
C7 C1 C5 118(3) . . ?
O12 C2 C12 113(3) . . ?
O13 C2 O12 128(3) . . ?
O13 C2 C12 119(3) . . ?
O14 C3 C5 113(3) . . ?
O15 C3 O14 126(4) . . ?
O15 C3 C5 121(4) . . ?
N2 C4 C12 122(4) . . ?
C1 C5 C3 114(3) . . ?
C12 C5 C1 120(3) . . ?
C12 C5 C3 126(3) . . ?
C9 C6 N1 120(3) . . ?
C1 C7 N2 122(3) . . ?
O1 C8 O3 123(3) . . ?
O1 C8 C10 122(3) . . ?
O3 C8 C10 115(3) . . ?
C6 C9 C10 120(3) . . ?
C9 C10 C8 113(3) . . ?
C11 C10 C8 125(3) . . ?
C11 C10 C9 122(3) . . ?
C10 C11 C13 125(3) . . ?
C10 C11 C14 117(3) . . ?
C14 C11 C13 118(3) . . ?
C4 C12 C2 118(3) . . ?
C5 C12 C2 123(3) . . ?
C5 C12 C4 119(3) . . ?
O6 C13 K3 76(2) . 1_655 ?
O6 C13 O43 130(3) . . ?
O6 C13 C11 114(3) . . ?
O43 C13 K3 54.3(18) . 1_655 ?
O43 C13 C11 117(3) . . ?
C11 C13 K3 165(2) . 1_655 ?
C11 C14 N1 119(3) . . ?


_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_ma18005_0m
_database_code_depnum_ccdc_archive 'CCDC 1857778'
_audit_update_record             
;
2018-07-24 deposited with the CCDC.
2018-08-23 downloaded from the CCDC.
;
_audit_creation_date             2018-06-24
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'C14 K4.5 La2 N2 O63.06 Si W11, 0.44(O)'
_chemical_formula_sum            'C14 K4.50 La2 N2 O63.50 Si W11'
_chemical_formula_weight         3716.37
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   11.5296(10)
_cell_length_b                   30.702(3)
_cell_length_c                   17.9958(14)
_cell_angle_alpha                90
_cell_angle_beta                 101.940(3)
_cell_angle_gamma                90
_cell_volume                     6232.3(9)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    9564
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      36.221
_cell_measurement_theta_min      2.302
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    21.995
_exptl_absorpt_correction_T_max  0.7471
_exptl_absorpt_correction_T_min  0.4028
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1708 before and 0.0669 after correction. The Ratio of minimum to maximum transmission is 0.5392. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            white
_exptl_crystal_colour_primary    white
_exptl_crystal_density_diffrn    3.961
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plates
_exptl_crystal_F_000             6534
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.04
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0488
_diffrn_reflns_av_unetI/netI     0.0244
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       38
_diffrn_reflns_limit_k_min       -38
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            110257
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.372
_diffrn_reflns_theta_min         3.514
_diffrn_ambient_temperature      150.0
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                11831
_reflns_number_total             12731
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_refine_diff_density_max         3.548
_refine_diff_density_min         -2.730
_refine_diff_density_rms         0.239
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.083
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     886
_refine_ls_number_reflns         12731
_refine_ls_number_restraints     6
_refine_ls_R_factor_all          0.0292
_refine_ls_R_factor_gt           0.0259
_refine_ls_restrained_S_all      1.083
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0152P)²+122.8405P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0579
_refine_ls_wR_factor_ref         0.0593
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(W5) \\sim Ueq, Uanis(W5) \\sim Ueq: with sigma of 0.1 and sigma for
terminal atoms of 0.2
2. Others
 Sof(O65)=1-FVAR(1)
 Sof(O63)=FVAR(1)
 Fixed Sof: K4(0.25) O62(0.5) K5(0.5) K6(0.75)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.18272(3) 0.55379(2) 0.36029(2) 0.00835(6) Uani 1 1 d . . . . .
W2 W 0.07619(3) 0.66654(2) 0.40047(2) 0.00943(6) Uani 1 1 d . . . . .
W3 W -0.10614(3) 0.72114(2) 0.26023(2) 0.00943(6) Uani 1 1 d . . . . .
W4 W 0.30200(3) 0.41610(2) -0.15482(2) 0.00790(6) Uani 1 1 d . . . . .
W5 W -0.09554(3) 0.52161(2) 0.30440(2) 0.00751(6) Uani 1 1 d . U . . .
W6 W -0.20449(3) 0.63401(2) 0.34276(2) 0.00813(6) Uani 1 1 d . . . . .
W7 W 0.10231(3) 0.43255(2) -0.04346(2) 0.00788(6) Uani 1 1 d . . . . .
W8 W -0.20445(3) 0.67050(2) 0.06986(2) 0.00952(6) Uani 1 1 d . . . . .
W9 W 0.10730(3) 0.70613(2) 0.13289(2) 0.01109(7) Uani 1 1 d . . . . .
W10 W 0.20340(3) 0.60251(2) 0.10550(2) 0.01032(7) Uani 1 1 d . . . . .
W11 W 0.28690(3) 0.65286(2) 0.27403(2) 0.01092(7) Uani 1 1 d . . . . .
La1 La 0.12037(4) 0.48042(2) 0.17858(2) 0.00824(9) Uani 1 1 d . . . . .
La2 La -0.11188(4) 0.85674(2) 0.22292(3) 0.01324(9) Uani 1 1 d . . . . .
Si14 Si -0.00570(17) 0.61510(7) 0.22259(11) 0.0068(4) Uani 1 1 d . . . . .
K1 K 0.5524(2) 0.69125(9) 0.19355(14) 0.0382(6) Uani 1 1 d . . . . .
O1 O -0.1952(5) 0.69895(18) 0.1664(3) 0.0127(11) Uani 1 1 d . . . . .
O2 O 0.2802(5) 0.5435(2) 0.4446(3) 0.0166(12) Uani 1 1 d . . . . .
O3 O 0.2943(5) 0.38042(18) -0.2425(3) 0.0112(11) Uani 1 1 d . . . . .
O4 O -0.3339(5) 0.63714(18) 0.0958(3) 0.0110(11) Uani 1 1 d . . . . .
O5 O 0.2144(5) 0.45873(18) -0.2180(3) 0.0108(11) Uani 1 1 d . . . . .
O6 O -0.0356(5) 0.48152(17) 0.2536(3) 0.0109(11) Uani 1 1 d . . . . .
O7 O 0.2591(5) 0.44248(17) -0.0677(3) 0.0097(11) Uani 1 1 d . . . . .
O8 O 0.1077(5) 0.63642(17) 0.1937(3) 0.0101(11) Uani 1 1 d . . . . .
O9 O 0.0395(5) 0.47577(19) -0.1021(3) 0.0130(11) Uani 1 1 d . . . . .
O10 O 0.1948(5) 0.67637(18) 0.3408(3) 0.0130(11) Uani 1 1 d . . . . .
O11 O 0.0034(5) 0.72119(18) 0.3543(3) 0.0113(11) Uani 1 1 d . . . . .
O12 O 0.2622(5) 0.85574(18) 0.3533(3) 0.0138(12) Uani 1 1 d . . . . .
O13 O -0.0379(5) 0.41830(19) 0.1343(3) 0.0181(12) Uani 1 1 d . . . . .
O14 O 0.2617(5) 0.5388(2) -0.1125(3) 0.0205(13) Uani 1 1 d . . . . .
O15 O -0.1486(5) 0.57912(18) 0.3505(3) 0.0104(11) Uani 1 1 d . . . . .
O16 O 0.2673(5) 0.59771(18) 0.3165(3) 0.0123(11) Uani 1 1 d . . . . .
O17 O 0.4441(5) 0.43523(19) -0.1395(3) 0.0144(12) Uani 1 1 d . . . . .
O18 O -0.0424(5) 0.40296(18) -0.0480(3) 0.0125(11) Uani 1 1 d . . . . .
O19 O -0.0786(5) 0.65491(18) 0.4222(3) 0.0125(11) Uani 1 1 d . . . . .
O20 O 0.0791(5) 0.8214(2) 0.1994(4) 0.0210(13) Uani 1 1 d . . . . .
O21 O 0.1806(5) 0.37352(18) -0.0048(3) 0.0106(11) Uani 1 1 d . . . . .
O22 O -0.2216(5) 0.69525(18) 0.3081(3) 0.0109(11) Uani 1 1 d . . . . .
O23 O 0.4822(5) 0.6230(2) -0.0240(3) 0.0230(14) Uani 1 1 d . . . . .
O24 O 0.3353(5) 0.4636(2) 0.1843(3) 0.0168(12) Uani 1 1 d . . . . .
O25 O -0.4478(5) 0.8640(2) 0.2446(3) 0.0186(13) Uani 1 1 d . . . . .
O26 O 0.1308(5) 0.45508(19) 0.0480(3) 0.0145(12) Uani 1 1 d . . . . .
O27 O 0.0243(5) 0.72344(18) 0.2102(3) 0.0126(11) Uani 1 1 d . . . . .
O28 O 0.3253(5) 0.62556(19) 0.1864(3) 0.0149(12) Uani 1 1 d . . . . .
O29 O 0.0426(5) 0.52675(17) 0.3868(3) 0.0103(11) Uani 1 1 d . . . . .
O30 O 0.0276(4) 0.56837(17) 0.2636(3) 0.0084(10) Uani 1 1 d . . . . .
O31 O 0.0382(6) 0.9191(2) 0.0553(4) 0.0296(15) Uani 1 1 d . . . . .
O32 O 0.1451(5) 0.68725(19) 0.4873(3) 0.0148(12) Uani 1 1 d . . . . .
O33 O -0.3238(5) 0.8544(2) 0.1648(3) 0.0179(13) Uani 1 1 d . . . . .
O34 O 0.5852(5) 0.5192(2) -0.0487(3) 0.0244(14) Uani 1 1 d . . . . .
N1 N -0.5152(6) 0.9397(2) 0.0119(4) 0.0146(14) Uani 1 1 d . . . . .
O35 O 0.4286(5) 0.6664(2) 0.3184(3) 0.0211(13) Uani 1 1 d . . . . .
O36 O -0.1493(5) 0.77503(18) 0.2544(3) 0.0140(12) Uani 1 1 d . . . . .
C1 C -0.4926(7) 0.8980(3) 0.1238(4) 0.0114(15) Uani 1 1 d . . . . .
O37 O 0.2832(5) 0.5929(2) 0.0365(3) 0.0176(12) Uani 1 1 d . . . . .
O38 O 0.2477(5) 0.70483(18) 0.2122(3) 0.0136(11) Uani 1 1 d . . . . .
O39 O 0.1765(5) 0.41230(18) 0.2560(3) 0.0131(11) Uani 1 1 d . . . . .
O40 O 0.1272(5) 0.7559(2) 0.0929(3) 0.0194(13) Uani 1 1 d . . . . .
O41 O -0.3146(5) 0.63355(19) 0.3938(3) 0.0150(12) Uani 1 1 d . . . . .
N2 N 0.5125(7) 0.5590(3) 0.3219(5) 0.0292(19) Uani 1 1 d . . . . .
O42 O -0.1138(6) 0.9045(2) 0.1119(3) 0.0221(14) Uani 1 1 d . . . . .
O43 O 0.0285(6) 0.8416(2) 0.3494(4) 0.0285(15) Uani 1 1 d . . . . .
O44 O -0.2837(5) 0.70724(19) 0.0076(3) 0.0156(12) Uani 1 1 d . . . . .
O45 O -0.1473(5) 0.8087(2) 0.1011(3) 0.0209(13) Uani 1 1 d . . . . .
O46 O -0.0477(5) 0.64892(17) 0.2826(3) 0.0090(11) Uani 1 1 d . . . . .
O47 O 0.1773(5) 0.66788(18) 0.0762(3) 0.0125(11) Uani 1 1 d . . . . .
C2 C -0.4470(7) 0.9138(3) 0.0648(4) 0.0134(16) Uani 1 1 d . . . . .
O48 O 0.1986(5) 0.55107(19) 0.1487(3) 0.0139(12) Uani 1 1 d . . . . .
O49 O 0.2136(5) 0.51046(19) 0.3030(3) 0.0122(11) Uani 1 1 d . . . . .
C3 C 0.4701(7) 0.4837(3) 0.2964(5) 0.0182(18) Uani 1 1 d . . . . .
O50 O -0.7158(5) 0.85286(19) 0.1712(3) 0.0169(12) Uani 1 1 d . . . . .
O51 O 0.1171(5) 0.60965(18) 0.4047(3) 0.0103(11) Uani 1 1 d . . . . .
C4 C -0.6779(7) 0.9353(3) 0.0726(4) 0.0143(16) Uani 1 1 d . . . . .
C5 C -0.6261(7) 0.9509(3) 0.0151(4) 0.0151(17) Uani 1 1 d . . . . .
C6 C -0.6096(7) 0.9089(3) 0.1281(4) 0.0126(16) Uani 1 1 d . . . . .
O52 O -0.0461(5) 0.69072(18) 0.0756(3) 0.0137(11) Uani 1 1 d . . . . .
O53 O -0.1142(5) 0.61035(17) 0.1483(3) 0.0079(10) Uani 1 1 d . . . . .
O54 O -0.1829(5) 0.49099(18) 0.3522(3) 0.0130(11) Uani 1 1 d . . . . .
C7 C 0.5239(7) 0.4742(3) 0.3710(5) 0.0171(17) Uani 1 1 d . . . . .
C8 C 0.4623(7) 0.5282(3) 0.2724(5) 0.0186(18) Uani 1 1 d . . . . .
O55 O -0.2251(5) 0.8516(2) 0.3331(3) 0.0197(13) Uani 1 1 d . . . . .
O56 O 0.4398(6) 0.4106(2) 0.2533(3) 0.0225(14) Uani 1 1 d . . . . .
O57 O -0.1903(6) 0.9303(2) 0.2531(4) 0.0247(14) Uani 1 1 d . . . . .
C9 C 0.5704(8) 0.5082(3) 0.4210(5) 0.0200(18) Uani 1 1 d . . . . .
C10 C -0.4154(7) 0.8699(3) 0.1827(4) 0.0133(16) Uani 1 1 d . . . . .
C11 C 0.5616(7) 0.5497(3) 0.3951(5) 0.0175(17) Uani 1 1 d . . . . .
C12 C -0.6701(7) 0.8899(3) 0.1870(4) 0.0121(16) Uani 1 1 d . . . . .
C13 C 0.4120(7) 0.4497(3) 0.2404(5) 0.0182(18) Uani 1 1 d . . . . .
C14 C -0.0339(8) 0.9285(3) 0.0970(5) 0.0211(19) Uani 1 1 d . . . . .
K2 K -0.3602(3) 0.72645(16) 0.4260(2) 0.0929(15) Uani 1 1 d . . . . .
K3 K 0.4207(4) 0.54990(14) -0.0066(2) 0.0787(11) Uani 1 1 d . . . . .
O58 O 0.4932(8) 0.7387(3) 0.0584(5) 0.052(2) Uani 1 1 d . . . . .
K4 K 0.3677(9) 0.7820(4) 0.2597(6) 0.040(2) Uiso 0.25 1 d . . P . .
O59 O 0.3387(8) 0.8061(3) 0.0414(5) 0.0409(19) Uani 1 1 d . . . . .
O60 O -0.5931(8) 0.7421(3) 0.4427(5) 0.058(3) Uani 1 1 d . . . . .
O61 O -0.1964(8) 0.8040(3) 0.4669(5) 0.048(2) Uani 1 1 d . . . . .
O62 O -0.2487(15) 0.6852(5) 0.5258(8) 0.031(3) Uani 0.5 1 d . . P A .
O63 O 0.4142(18) 0.6481(6) 0.4787(10) 0.040(6) Uiso 0.44(3) 1 d . . P A 1
O64 O 0.6012(10) 0.7638(4) 0.2854(9) 0.095(5) Uani 1 1 d . . . . .
K5 K -0.0263(7) 0.3335(3) 0.0804(4) 0.076(2) Uiso 0.5 1 d . . P . .
K6 K 0.1999(2) 0.77010(8) 0.34733(14) 0.0171(5) Uiso 0.75 1 d . . P . .
O65 O -0.5094(16) 0.6618(5) 0.4956(9) 0.047(6) Uiso 0.56(3) 1 d . . P A 2


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O2 1.721(6) . ?
W1 O16 1.926(6) . ?
W1 O29 1.961(5) . ?
W1 O30 2.266(5) . ?
W1 O49 1.764(5) . ?
W1 O51 2.098(5) . ?
W2 O10 1.929(5) . ?
W2 O11 1.980(5) . ?
W2 O19 1.938(6) . ?
W2 O32 1.722(5) . ?
W2 O46 2.362(5) . ?
W2 O51 1.807(5) . ?
W2 K6 3.691(3) . ?
W3 K1 3.979(3) 1_455 ?
W3 O1 1.912(5) . ?
W3 O11 1.891(5) . ?
W3 O22 1.902(5) . ?
W3 O27 1.907(5) . ?
W3 O36 1.725(5) . ?
W3 O46 2.328(5) . ?
W3 K6 3.858(2) . ?
W4 K1 3.828(3) 3_665 ?
W4 O3 1.907(5) . ?
W4 O4 1.943(5) 3_565 ?
W4 O5 1.884(5) . ?
W4 O7 1.919(5) . ?
W4 O17 1.709(5) . ?
W4 O53 2.338(5) 3_565 ?
W4 K3 3.988(4) 3_665 ?
W5 O5 1.944(5) 3_565 ?
W5 O6 1.758(5) . ?
W5 O15 2.095(5) . ?
W5 O29 1.945(5) . ?
W5 O30 2.246(5) . ?
W5 O54 1.731(6) . ?
W6 K1 3.879(2) 1_455 ?
W6 O3 1.937(5) 3_565 ?
W6 O15 1.799(5) . ?
W6 O19 1.924(5) . ?
W6 O22 1.978(5) . ?
W6 O41 1.715(6) . ?
W6 O46 2.336(5) . ?
W6 K2 3.826(4) . ?
W7 O7 1.969(5) . ?
W7 O9 1.755(6) . ?
W7 O18 1.887(5) . ?
W7 O21 2.079(5) . ?
W7 O26 1.752(5) . ?
W7 O53 2.328(5) 3_565 ?
W8 K1 3.975(2) 1_455 ?
W8 O1 1.927(5) . ?
W8 O4 1.944(5) . ?
W8 O21 1.846(5) 3_565 ?
W8 O44 1.715(5) . ?
W8 O52 1.911(6) . ?
W8 O53 2.424(5) . ?
W9 O8 2.404(5) . ?
W9 O27 1.920(5) . ?
W9 O38 1.924(6) . ?
W9 O40 1.724(6) . ?
W9 O47 1.847(5) . ?
W9 O52 1.913(5) . ?
W9 K4 4.100(11) . ?
W9 K5 3.950(8) 3_565 ?
W10 O8 2.355(5) . ?
W10 O18 1.937(6) 3_565 ?
W10 O28 1.936(6) . ?
W10 O37 1.716(6) . ?
W10 O47 2.081(6) . ?
W10 O48 1.766(6) . ?
W10 K3 3.878(4) . ?
W10 K5 4.050(8) 3_565 ?
W11 K1 3.833(3) . ?
W11 O8 2.319(5) . ?
W11 O10 1.903(5) . ?
W11 O16 1.891(6) . ?
W11 O28 1.917(6) . ?
W11 O35 1.715(6) . ?
W11 O38 1.944(6) . ?
W11 K4 4.093(11) . ?
W11 K6 4.031(3) . ?
La1 O6 2.462(5) . ?
La1 O9 2.460(5) 3_565 ?
La1 O13 2.646(6) . ?
La1 O24 2.512(6) . ?
La1 O26 2.502(5) . ?
La1 O39 2.522(6) . ?
La1 O48 2.451(6) . ?
La1 O49 2.455(5) . ?
La2 O20 2.566(6) . ?
La2 O33 2.452(6) . ?
La2 O36 2.627(6) . ?
La2 O42 2.475(6) . ?
La2 O43 2.548(6) . ?
La2 O45 2.603(6) . ?
La2 O55 2.594(6) . ?
La2 O56 2.550(6) 2 ?
La2 O57 2.533(6) . ?
Si14 O8 1.640(6) . ?
Si14 O30 1.623(5) . ?
Si14 O46 1.642(5) . ?
Si14 O53 1.637(5) . ?
K1 W4 3.828(3) 3_665 ?
K1 W6 3.878(2) 1_655 ?
K1 O1 3.058(6) 1_655 ?
K1 O3 2.845(6) 3_665 ?
K1 O4 2.921(6) 1_655 ?
K1 O22 2.972(6) 1_655 ?
K1 O28 3.286(6) . ?
K1 O35 2.999(7) . ?
K1 O58 2.797(9) . ?
K1 K4 3.841(11) . ?
K1 O64 2.762(14) . ?
O1 K1 3.058(6) 1_455 ?
O3 W6 1.937(5) 3_565 ?
O3 K1 2.846(6) 3_665 ?
O4 W4 1.943(5) 3_565 ?
O4 K1 2.921(6) 1_455 ?
O5 W5 1.944(5) 3_565 ?
O9 La1 2.460(5) 3_565 ?
O10 K6 2.880(6) . ?
O11 K6 2.742(6) . ?
O12 K4 3.208(12) . ?
O12 K5 3.108(10) 2 ?
O12 K6 2.722(6) . ?
O13 K5 2.793(10) . ?
O14 K3 2.380(7) . ?
O17 K3 2.802(7) 3_665 ?
O18 W10 1.937(5) 3_565 ?
O18 K5 3.122(10) . ?
O20 K6 3.158(7) . ?
O21 W8 1.846(5) 3_565 ?
O21 K5 3.327(10) . ?
O22 K1 2.972(6) 1_455 ?
O22 K2 3.063(6) . ?
O23 K3 2.393(8) . ?
O24 C13 1.270(10) . ?
O25 C10 1.260(10) . ?
O25 K4 3.343(12) 1_455 ?
O25 K5 3.358(10) 2_455 ?
O27 K6 3.189(6) . ?
O31 C14 1.264(11) . ?
O33 C10 1.259(10) . ?
O34 K3 2.351(8) 3_665 ?
O34 K3 2.378(7) . ?
N1 C2 1.360(11) . ?
N1 C5 1.337(11) . ?
O35 K2 3.335(7) 1_655 ?
C1 C2 1.368(11) . ?
C1 C6 1.407(11) . ?
C1 C10 1.506(11) . ?
O37 K3 2.316(7) . ?
O38 K4 2.787(12) . ?
O38 K6 3.284(6) . ?
O39 C12 1.250(10) 2_445 ?
O40 K2 3.084(7) 4_675 ?
O41 K2 2.979(7) . ?
N2 C8 1.345(12) . ?
N2 C11 1.352(12) . ?
O42 C14 1.252(11) . ?
O43 K6 2.959(7) . ?
O44 K6 2.934(6) 4_575 ?
O47 K5 2.991(10) 3_565 ?
C3 C7 1.389(12) . ?
C3 C8 1.430(13) . ?
C3 C13 1.506(12) . ?
O50 C12 1.262(10) . ?
O50 K4 2.750(12) 1_455 ?
C4 C5 1.385(11) . ?
C4 C6 1.396(11) . ?
C6 C12 1.502(11) . ?
O52 K5 3.178(10) 3_565 ?
O53 W4 2.338(5) 3_565 ?
O53 W7 2.328(5) 3_565 ?
C7 C9 1.408(12) . ?
C7 C14 1.510(12) 2_545 ?
O56 La2 2.550(6) 2_545 ?
O56 C13 1.253(11) . ?
C9 C11 1.353(12) . ?
C12 O39 1.250(10) 2_455 ?
C14 C7 1.510(12) 2 ?
K2 O35 3.335(7) 1_455 ?
K2 O40 3.084(7) 4_576 ?
K2 O59 2.933(10) 4_576 ?
K2 O60 2.804(10) . ?
K2 O61 3.033(11) . ?
K2 O62 2.351(15) . ?
K2 O64 2.729(15) 1_455 ?
K2 K5 3.529(9) 2_455 ?
K2 O65 3.060(18) . ?
K3 W4 3.988(4) 3_665 ?
K3 O17 2.801(7) 3_665 ?
K3 O34 2.351(8) 3_665 ?
K3 K3 3.551(8) 3_665 ?
K4 O25 3.343(12) 1_655 ?
K4 O50 2.750(12) 1_655 ?
K4 K2 4.221(11) 1_655 ?
K4 O64 2.694(15) . ?
K4 K5 3.456(13) 2 ?
K4 K6 2.762(11) . ?
O59 K2 2.933(10) 4_675 ?
O59 O62 1.024(16) 4_675 ?
O60 K5 3.189(14) 2_455 ?
O60 K6 2.772(9) 1_455 ?
O61 K5 3.261(11) 2_455 ?
O62 O59 1.024(16) 4_576 ?
O64 K2 2.729(15) 1_655 ?
K5 W9 3.950(8) 3_565 ?
K5 O12 3.109(10) 2_545 ?
K5 O25 3.358(10) 2_445 ?
K5 O47 2.991(10) 3_565 ?
K5 O52 3.178(10) 3_565 ?
K5 K2 3.529(9) 2_445 ?
K5 K4 3.456(13) 2_545 ?
K5 O60 3.188(14) 2_445 ?
K5 O61 3.261(11) 2_445 ?
K6 O44 2.934(6) 4_676 ?
K6 O60 2.772(9) 1_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 W1 O16 101.3(3) . . ?
O2 W1 O29 97.4(2) . . ?
O2 W1 O30 168.8(2) . . ?
O2 W1 O49 101.6(3) . . ?
O2 W1 O51 92.1(2) . . ?
O16 W1 O29 155.3(2) . . ?
O16 W1 O30 86.2(2) . . ?
O16 W1 O51 80.6(2) . . ?
O29 W1 O30 73.2(2) . . ?
O29 W1 O51 82.7(2) . . ?
O49 W1 O16 96.2(2) . . ?
O49 W1 O29 95.7(2) . . ?
O49 W1 O30 85.6(2) . . ?
O49 W1 O51 166.3(2) . . ?
O51 W1 O30 80.89(19) . . ?
O10 W2 O11 85.5(2) . . ?
O10 W2 O19 158.4(2) . . ?
O10 W2 O46 84.4(2) . . ?
O10 W2 K6 50.54(17) . . ?
O11 W2 O46 72.1(2) . . ?
O11 W2 K6 46.70(16) . . ?
O19 W2 O11 85.0(2) . . ?
O19 W2 O46 74.2(2) . . ?
O19 W2 K6 129.23(17) . . ?
O32 W2 O10 101.6(3) . . ?
O32 W2 O11 98.3(2) . . ?
O32 W2 O19 99.0(2) . . ?
O32 W2 O46 168.4(2) . . ?
O32 W2 O51 104.5(3) . . ?
O32 W2 K6 77.7(2) . . ?
O46 W2 K6 99.15(13) . . ?
O51 W2 O10 88.1(2) . . ?
O51 W2 O11 157.1(2) . . ?
O51 W2 O19 93.3(2) . . ?
O51 W2 O46 85.5(2) . . ?
O51 W2 K6 137.07(17) . . ?
O1 W3 K1 48.24(17) . 1_455 ?
O1 W3 O46 84.1(2) . . ?
O1 W3 K6 140.99(17) . . ?
O11 W3 K1 134.93(17) . 1_455 ?
O11 W3 O1 158.2(2) . . ?
O11 W3 O22 89.7(2) . . ?
O11 W3 O27 88.6(2) . . ?
O11 W3 O46 74.3(2) . . ?
O11 W3 K6 41.45(17) . . ?
O22 W3 K1 45.47(16) . 1_455 ?
O22 W3 O1 87.3(2) . . ?
O22 W3 O27 157.4(2) . . ?
O22 W3 O46 74.2(2) . . ?
O22 W3 K6 130.23(16) . . ?
O27 W3 K1 133.95(17) . 1_455 ?
O27 W3 O1 85.9(2) . . ?
O27 W3 O46 83.6(2) . . ?
O27 W3 K6 55.45(17) . . ?
O36 W3 K1 87.01(19) . 1_455 ?
O36 W3 O1 101.1(2) . . ?
O36 W3 O11 100.7(2) . . ?
O36 W3 O22 102.0(2) . . ?
O36 W3 O27 100.5(3) . . ?
O36 W3 O46 173.6(2) . . ?
O36 W3 K6 83.07(19) . . ?
O46 W3 K1 93.75(14) . 1_455 ?
O46 W3 K6 95.34(14) . . ?
K6 W3 K1 167.81(5) . 1_455 ?
K1 W4 K3 92.42(7) 3_665 3_665 ?
O3 W4 K1 45.73(16) . 3_665 ?
O3 W4 O4 86.6(2) . 3_565 ?
O3 W4 O7 160.5(2) . . ?
O3 W4 O53 87.5(2) . 3_565 ?
O3 W4 K3 130.21(17) . 3_665 ?
O4 W4 K1 48.30(16) 3_565 3_665 ?
O4 W4 O53 75.7(2) 3_565 3_565 ?
O4 W4 K3 77.84(17) 3_565 3_665 ?
O5 W4 K1 133.52(16) . 3_665 ?
O5 W4 O3 88.4(2) . . ?
O5 W4 O4 158.7(2) . 3_565 ?
O5 W4 O7 90.2(2) . . ?
O5 W4 O53 83.4(2) . 3_565 ?
O5 W4 K3 120.43(17) . 3_665 ?
O7 W4 K1 135.16(16) . 3_665 ?
O7 W4 O4 87.7(2) . 3_565 ?
O7 W4 O53 73.00(19) . 3_565 ?
O7 W4 K3 66.27(16) . 3_665 ?
O17 W4 K1 83.3(2) . 3_665 ?
O17 W4 O3 102.1(2) . . ?
O17 W4 O4 97.7(3) . 3_565 ?
O17 W4 O5 103.6(3) . . ?
O17 W4 O7 97.1(2) . . ?
O17 W4 O53 168.1(2) . 3_565 ?
O17 W4 K3 36.35(19) . 3_665 ?
O53 W4 K1 98.96(13) 3_565 3_665 ?
O53 W4 K3 131.73(13) 3_565 3_665 ?
O5 W5 O15 80.8(2) 3_565 . ?
O5 W5 O29 156.2(2) 3_565 . ?
O5 W5 O30 86.0(2) 3_565 . ?
O6 W5 O5 95.2(2) . 3_565 ?
O6 W5 O15 167.0(2) . . ?
O6 W5 O29 96.0(2) . . ?
O6 W5 O30 86.3(2) . . ?
O15 W5 O30 81.2(2) . . ?
O29 W5 O15 83.7(2) . . ?
O29 W5 O30 74.0(2) . . ?
O54 W5 O5 100.3(2) . 3_565 ?
O54 W5 O6 102.1(2) . . ?
O54 W5 O15 90.8(2) . . ?
O54 W5 O29 97.7(2) . . ?
O54 W5 O30 168.9(2) . . ?
O3 W6 K1 44.60(17) 3_565 1_455 ?
O3 W6 O22 85.6(2) 3_565 . ?
O3 W6 O46 85.9(2) 3_565 . ?
O3 W6 K2 109.30(17) 3_565 . ?
O15 W6 K1 132.37(17) . 1_455 ?
O15 W6 O3 88.4(2) . 3_565 ?
O15 W6 O19 93.0(2) . . ?
O15 W6 O22 157.7(2) . . ?
O15 W6 O46 85.4(2) . . ?
O15 W6 K2 148.68(18) . . ?
O19 W6 K1 133.56(17) . 1_455 ?
O19 W6 O3 160.7(2) . 3_565 ?
O19 W6 O22 85.9(2) . . ?
O19 W6 O46 75.0(2) . . ?
O19 W6 K2 78.73(18) . . ?
O22 W6 K1 48.72(16) . 1_455 ?
O22 W6 O46 72.8(2) . . ?
O22 W6 K2 52.71(17) . . ?
O41 W6 K1 82.27(19) . 1_455 ?
O41 W6 O3 100.7(2) . 3_565 ?
O41 W6 O15 104.1(3) . . ?
O41 W6 O19 97.6(2) . . ?
O41 W6 O22 98.1(2) . . ?
O41 W6 O46 168.4(2) . . ?
O41 W6 K2 48.4(2) . . ?
O46 W6 K1 96.21(13) . 1_455 ?
O46 W6 K2 120.45(15) . . ?
K2 W6 K1 66.69(7) . 1_455 ?
O7 W7 O21 81.6(2) . . ?
O7 W7 O53 72.41(19) . 3_565 ?
O9 W7 O7 91.9(2) . . ?
O9 W7 O18 95.0(2) . . ?
O9 W7 O21 163.1(2) . . ?
O9 W7 O53 91.5(2) . 3_565 ?
O18 W7 O7 155.4(2) . . ?
O18 W7 O21 85.0(2) . . ?
O18 W7 O53 83.8(2) . 3_565 ?
O21 W7 O53 71.59(19) . 3_565 ?
O26 W7 O7 98.3(2) . . ?
O26 W7 O9 103.9(3) . . ?
O26 W7 O18 102.9(2) . . ?
O26 W7 O21 92.6(2) . . ?
O26 W7 O53 162.4(2) . 3_565 ?
O1 W8 K1 48.43(17) . 1_455 ?
O1 W8 O4 85.7(2) . . ?
O1 W8 O53 83.3(2) . . ?
O4 W8 K1 44.36(16) . 1_455 ?
O4 W8 O53 73.6(2) . . ?
O21 W8 K1 133.43(17) 3_565 1_455 ?
O21 W8 O1 156.4(2) 3_565 . ?
O21 W8 O4 89.4(2) 3_565 . ?
O21 W8 O52 90.4(2) 3_565 . ?
O21 W8 O53 73.1(2) 3_565 . ?
O44 W8 K1 85.3(2) . 1_455 ?
O44 W8 O1 102.3(3) . . ?
O44 W8 O4 99.9(3) . . ?
O44 W8 O21 101.3(3) . 3_565 ?
O44 W8 O52 101.3(3) . . ?
O44 W8 O53 171.2(2) . . ?
O52 W8 K1 133.96(17) . 1_455 ?
O52 W8 O1 86.0(2) . . ?
O52 W8 O4 158.5(2) . . ?
O52 W8 O53 85.7(2) . . ?
O53 W8 K1 93.64(12) . 1_455 ?
O8 W9 K4 108.68(19) . . ?
O8 W9 K5 98.41(17) . 3_565 ?
O27 W9 O8 82.6(2) . . ?
O27 W9 O38 86.4(2) . . ?
O27 W9 K4 81.8(2) . . ?
O27 W9 K5 137.4(2) . 3_565 ?
O38 W9 O8 73.8(2) . . ?
O38 W9 K4 36.1(2) . . ?
O38 W9 K5 135.1(2) . 3_565 ?
O40 W9 O8 172.4(2) . . ?
O40 W9 O27 100.8(3) . . ?
O40 W9 O38 99.5(3) . . ?
O40 W9 O47 102.8(3) . . ?
O40 W9 O52 100.5(3) . . ?
O40 W9 K4 65.4(3) . . ?
O40 W9 K5 83.8(2) . 3_565 ?
O47 W9 O8 74.1(2) . . ?
O47 W9 O27 156.4(2) . . ?
O47 W9 O38 90.0(2) . . ?
O47 W9 O52 90.3(2) . . ?
O47 W9 K4 108.4(2) . . ?
O47 W9 K5 46.4(2) . 3_565 ?
O52 W9 O8 86.5(2) . . ?
O52 W9 O27 85.1(2) . . ?
O52 W9 O38 159.5(2) . . ?
O52 W9 K4 158.3(2) . . ?
O52 W9 K5 52.7(2) . 3_565 ?
K5 W9 K4 135.58(19) 3_565 . ?
O8 W10 K3 167.89(14) . . ?
O8 W10 K5 96.65(17) . 3_565 ?
O18 W10 O8 82.4(2) 3_565 . ?
O18 W10 O47 82.9(2) 3_565 . ?
O18 W10 K3 109.67(17) 3_565 . ?
O18 W10 K5 48.5(2) 3_565 3_565 ?
O28 W10 O8 72.5(2) . . ?
O28 W10 O18 154.2(2) . 3_565 ?
O28 W10 O47 83.2(2) . . ?
O28 W10 K3 95.55(17) . . ?
O28 W10 K5 127.4(2) . 3_565 ?
O37 W10 O8 163.6(2) . . ?
O37 W10 O18 101.3(3) . 3_565 ?
O37 W10 O28 101.1(3) . . ?
O37 W10 O47 93.1(3) . . ?
O37 W10 O48 103.5(3) . . ?
O37 W10 K3 18.5(2) . . ?
O37 W10 K5 75.0(2) . 3_565 ?
O47 W10 O8 71.39(19) . . ?
O47 W10 K3 110.20(16) . . ?
O47 W10 K5 45.65(19) . 3_565 ?
O48 W10 O8 92.1(2) . . ?
O48 W10 O18 92.5(2) . 3_565 ?
O48 W10 O28 94.6(2) . . ?
O48 W10 O47 163.3(2) . . ?
O48 W10 K3 86.50(19) . . ?
O48 W10 K5 137.9(2) . 3_565 ?
K3 W10 K5 92.41(13) . 3_565 ?
K1 W11 K4 57.88(15) . . ?
K1 W11 K6 96.97(5) . . ?
O8 W11 K1 120.64(14) . . ?
O8 W11 K4 110.90(19) . . ?
O8 W11 K6 98.54(13) . . ?
O10 W11 K1 135.70(17) . . ?
O10 W11 O8 86.2(2) . . ?
O10 W11 O28 159.9(2) . . ?
O10 W11 O38 87.5(2) . . ?
O10 W11 K4 80.6(2) . . ?
O10 W11 K6 41.02(17) . . ?
O16 W11 K1 126.84(17) . . ?
O16 W11 O8 83.8(2) . . ?
O16 W11 O10 87.5(2) . . ?
O16 W11 O28 90.5(2) . . ?
O16 W11 O38 159.0(2) . . ?
O16 W11 K4 160.2(2) . . ?
O16 W11 K6 127.52(17) . . ?
O28 W11 K1 59.02(17) . . ?
O28 W11 O8 73.7(2) . . ?
O28 W11 O38 87.4(2) . . ?
O28 W11 K4 106.1(2) . . ?
O28 W11 K6 140.82(18) . . ?
O35 W11 K1 48.9(2) . . ?
O35 W11 O8 169.5(2) . . ?
O35 W11 O10 102.5(3) . . ?
O35 W11 O16 102.2(3) . . ?
O35 W11 O28 97.4(3) . . ?
O35 W11 O38 98.9(3) . . ?
O35 W11 K4 65.6(3) . . ?
O35 W11 K6 84.8(2) . . ?
O38 W11 K1 68.95(16) . . ?
O38 W11 O8 75.5(2) . . ?
O38 W11 K4 36.7(2) . . ?
O38 W11 K6 53.88(17) . . ?
K6 W11 K4 39.74(15) . . ?
O6 La1 O13 68.81(18) . . ?
O6 La1 O24 143.76(18) . . ?
O6 La1 O26 134.57(18) . . ?
O6 La1 O39 80.88(17) . . ?
O9 La1 O6 75.64(17) 3_565 . ?
O9 La1 O13 80.53(19) 3_565 . ?
O9 La1 O24 138.89(18) 3_565 . ?
O9 La1 O26 79.64(18) 3_565 . ?
O9 La1 O39 147.08(18) 3_565 . ?
O24 La1 O13 118.49(19) . . ?
O24 La1 O39 70.67(19) . . ?
O26 La1 O13 69.95(18) . . ?
O26 La1 O24 74.67(18) . . ?
O26 La1 O39 101.78(18) . . ?
O39 La1 O13 69.54(18) . . ?
O48 La1 O6 116.86(18) . . ?
O48 La1 O9 70.15(18) . 3_565 ?
O48 La1 O13 146.52(18) . . ?
O48 La1 O24 77.65(19) . . ?
O48 La1 O26 88.73(19) . . ?
O48 La1 O39 142.29(18) . . ?
O48 La1 O49 75.88(18) . . ?
O49 La1 O6 74.12(17) . . ?
O49 La1 O9 116.19(18) . 3_565 ?
O49 La1 O13 133.64(18) . . ?
O49 La1 O24 78.34(18) . . ?
O49 La1 O26 151.24(18) . . ?
O49 La1 O39 78.10(18) . . ?
O20 La2 O36 79.46(19) . . ?
O20 La2 O45 67.22(19) . . ?
O20 La2 O55 133.2(2) . . ?
O33 La2 O20 136.94(19) . . ?
O33 La2 O36 82.54(19) . . ?
O33 La2 O42 80.3(2) . . ?
O33 La2 O43 140.2(2) . . ?
O33 La2 O45 69.83(19) . . ?
O33 La2 O55 73.11(18) . . ?
O33 La2 O56 139.7(2) . 2 ?
O33 La2 O57 75.5(2) . . ?
O42 La2 O20 89.0(2) . . ?
O42 La2 O36 139.97(19) . . ?
O42 La2 O43 136.6(2) . . ?
O42 La2 O45 71.5(2) . . ?
O42 La2 O55 136.9(2) . . ?
O42 La2 O56 68.1(2) . 2 ?
O42 La2 O57 72.6(2) . . ?
O43 La2 O20 70.2(2) . . ?
O43 La2 O36 74.7(2) . . ?
O43 La2 O45 127.5(2) . . ?
O43 La2 O55 68.5(2) . . ?
O43 La2 O56 68.9(2) . 2 ?
O45 La2 O36 68.68(18) . . ?
O55 La2 O36 69.31(18) . . ?
O55 La2 O45 126.4(2) . . ?
O56 La2 O20 68.7(2) 2 . ?
O56 La2 O36 137.74(19) 2 . ?
O56 La2 O45 119.3(2) 2 . ?
O56 La2 O55 114.1(2) 2 . ?
O57 La2 O20 140.2(2) . . ?
O57 La2 O36 136.34(19) . . ?
O57 La2 O43 99.2(2) . . ?
O57 La2 O45 133.2(2) . . ?
O57 La2 O55 68.4(2) . . ?
O57 La2 O56 71.7(2) . 2 ?
O8 Si14 O46 108.6(3) . . ?
O30 Si14 O8 111.6(3) . . ?
O30 Si14 O46 109.5(3) . . ?
O30 Si14 O53 111.2(3) . . ?
O53 Si14 O8 107.5(3) . . ?
O53 Si14 O46 108.3(3) . . ?
W4 K1 W6 56.94(4) 3_665 1_655 ?
W4 K1 W11 102.64(6) 3_665 . ?
W4 K1 K4 166.63(17) 3_665 . ?
W11 K1 W6 96.80(6) . 1_655 ?
W11 K1 K4 64.46(16) . . ?
O1 K1 W4 64.51(11) 1_655 3_665 ?
O1 K1 W6 64.56(11) 1_655 1_655 ?
O1 K1 W11 160.91(13) 1_655 . ?
O1 K1 O28 144.88(17) 1_655 . ?
O1 K1 K4 126.9(2) 1_655 . ?
O3 K1 W4 28.68(11) 3_665 3_665 ?
O3 K1 W6 28.56(11) 3_665 1_655 ?
O3 K1 W11 97.98(13) 3_665 . ?
O3 K1 O1 63.80(16) 3_665 1_655 ?
O3 K1 O4 54.48(15) 3_665 1_655 ?
O3 K1 O22 54.41(16) 3_665 1_655 ?
O3 K1 O28 88.65(16) 3_665 . ?
O3 K1 O35 86.16(17) 3_665 . ?
O3 K1 K4 144.4(2) 3_665 . ?
O4 K1 W4 29.78(11) 1_655 3_665 ?
O4 K1 W6 79.00(12) 1_655 1_655 ?
O4 K1 W11 123.10(14) 1_655 . ?
O4 K1 O1 52.18(15) 1_655 1_655 ?
O4 K1 O22 90.15(16) 1_655 1_655 ?
O4 K1 O28 94.64(16) 1_655 . ?
O4 K1 O35 130.50(19) 1_655 . ?
O4 K1 K4 161.0(2) 1_655 . ?
O22 K1 W4 78.88(12) 1_655 3_665 ?
O22 K1 W6 30.02(11) 1_655 1_655 ?
O22 K1 W11 113.89(12) 1_655 . ?
O22 K1 O1 51.74(15) 1_655 1_655 ?
O22 K1 O28 129.04(17) 1_655 . ?
O22 K1 O35 88.61(16) 1_655 . ?
O22 K1 K4 102.6(2) 1_655 . ?
O28 K1 W4 80.82(11) . 3_665 ?
O28 K1 W6 101.83(12) . 1_655 ?
O28 K1 W11 30.01(10) . . ?
O28 K1 K4 88.23(19) . . ?
O35 K1 W4 102.24(14) . 3_665 ?
O35 K1 W6 75.74(13) . 1_655 ?
O35 K1 W11 25.54(11) . . ?
O35 K1 O1 139.07(17) . 1_655 ?
O35 K1 O28 51.29(15) . . ?
O35 K1 K4 64.7(2) . . ?
O58 K1 W4 109.1(2) . 3_665 ?
O58 K1 W6 148.17(19) . 1_655 ?
O58 K1 W11 114.76(19) . . ?
O58 K1 O1 83.6(2) . 1_655 ?
O58 K1 O3 134.1(2) . 3_665 ?
O58 K1 O4 80.3(2) . 1_655 ?
O58 K1 O22 127.1(2) . 1_655 ?
O58 K1 O28 103.7(2) . . ?
O58 K1 O35 135.7(2) . . ?
O58 K1 K4 80.8(3) . . ?
K4 K1 W6 118.79(17) . 1_655 ?
O64 K1 W4 139.5(3) . 3_665 ?
O64 K1 W6 85.5(3) . 1_655 ?
O64 K1 W11 95.8(2) . . ?
O64 K1 O1 87.2(2) . 1_655 ?
O64 K1 O3 113.7(3) . 3_665 ?
O64 K1 O4 139.3(3) . 1_655 ?
O64 K1 O22 60.7(3) . 1_655 ?
O64 K1 O28 125.5(3) . . ?
O64 K1 O35 80.0(3) . . ?
O64 K1 O58 94.8(3) . . ?
O64 K1 K4 44.5(3) . . ?
W3 O1 W8 151.3(3) . . ?
W3 O1 K1 104.0(2) . 1_455 ?
W8 O1 K1 103.4(2) . 1_455 ?
W4 O3 W6 145.7(3) . 3_565 ?
W4 O3 K1 105.6(2) . 3_665 ?
W6 O3 K1 106.8(2) 3_565 3_665 ?
W4 O4 W8 120.4(3) 3_565 . ?
W4 O4 K1 101.9(2) 3_565 1_455 ?
W8 O4 K1 107.9(2) . 1_455 ?
W4 O5 W5 154.1(3) . 3_565 ?
W5 O6 La1 134.8(3) . . ?
W4 O7 W7 121.3(3) . . ?
W10 O8 W9 92.50(18) . . ?
W11 O8 W9 90.42(18) . . ?
W11 O8 W10 92.00(18) . . ?
Si14 O8 W9 125.0(3) . . ?
Si14 O8 W10 123.6(3) . . ?
Si14 O8 W11 123.7(3) . . ?
W7 O9 La1 156.6(3) . 3_565 ?
W2 O10 K6 98.3(2) . . ?
W11 O10 W2 147.6(3) . . ?
W11 O10 K6 113.3(2) . . ?
W2 O11 K6 101.6(2) . . ?
W3 O11 W2 121.4(3) . . ?
W3 O11 K6 111.4(2) . . ?
K5 O12 K4 66.3(3) 2 . ?
K6 O12 K4 54.8(2) . . ?
K6 O12 K5 91.8(2) . 2 ?
La1 O13 K5 134.2(3) . . ?
W6 O15 W5 152.6(3) . . ?
W11 O16 W1 154.9(3) . . ?
W4 O17 K3 122.5(3) . 3_665 ?
W7 O18 W10 143.7(3) . 3_565 ?
W7 O18 K5 112.4(3) . . ?
W10 O18 K5 103.9(3) 3_565 . ?
W6 O19 W2 119.7(3) . . ?
La2 O20 K6 108.4(2) . . ?
W7 O21 K5 100.0(2) . . ?
W8 O21 W7 122.5(3) 3_565 . ?
W8 O21 K5 103.7(3) 3_565 . ?
W3 O22 W6 120.4(3) . . ?
W3 O22 K1 107.4(2) . 1_455 ?
W3 O22 K2 134.2(3) . . ?
W6 O22 K1 101.3(2) . 1_455 ?
W6 O22 K2 96.4(2) . . ?
K1 O22 K2 89.14(16) 1_455 . ?
C13 O24 La1 128.3(5) . . ?
C10 O25 K4 119.4(5) . 1_455 ?
C10 O25 K5 166.0(5) . 2_455 ?
K4 O25 K5 62.1(2) 1_455 2_455 ?
W7 O26 La1 165.6(3) . . ?
W3 O27 W9 153.1(3) . . ?
W3 O27 K6 95.0(2) . . ?
W9 O27 K6 110.7(2) . . ?
W10 O28 K1 134.6(3) . . ?
W11 O28 W10 121.6(3) . . ?
W11 O28 K1 91.0(2) . . ?
W5 O29 W1 115.8(3) . . ?
W5 O30 W1 94.30(19) . . ?
Si14 O30 W1 126.8(3) . . ?
Si14 O30 W5 127.4(3) . . ?
C10 O33 La2 134.0(5) . . ?
K3 O34 K3 97.3(3) 3_665 . ?
C5 N1 C2 122.8(7) . . ?
W11 O35 K1 105.5(3) . . ?
W11 O35 K2 156.2(3) . 1_655 ?
K1 O35 K2 83.75(17) . 1_655 ?
W3 O36 La2 150.6(3) . . ?
C2 C1 C6 119.1(7) . . ?
C2 C1 C10 118.8(7) . . ?
C6 C1 C10 122.1(7) . . ?
W10 O37 K3 147.9(4) . . ?
W9 O38 W11 120.1(3) . . ?
W9 O38 K4 119.9(3) . . ?
W9 O38 K6 107.0(2) . . ?
W11 O38 K4 118.7(3) . . ?
W11 O38 K6 97.6(2) . . ?
K4 O38 K6 53.4(2) . . ?
C12 O39 La1 149.0(5) 2_445 . ?
W9 O40 K2 126.9(3) . 4_675 ?
W6 O41 K2 106.0(3) . . ?
C8 N2 C11 122.2(8) . . ?
C14 O42 La2 129.6(6) . . ?
La2 O43 K6 115.2(2) . . ?
W8 O44 K6 135.7(3) . 4_575 ?
W3 O46 W2 92.11(18) . . ?
W3 O46 W6 92.46(18) . . ?
W6 O46 W2 90.64(17) . . ?
Si14 O46 W2 122.0(3) . . ?
Si14 O46 W3 127.0(3) . . ?
Si14 O46 W6 122.9(3) . . ?
W9 O47 W10 122.0(3) . . ?
W9 O47 K5 107.1(3) . 3_565 ?
W10 O47 K5 104.5(3) . 3_565 ?
N1 C2 C1 119.4(7) . . ?
W10 O48 La1 159.1(3) . . ?
W1 O49 La1 135.5(3) . . ?
C7 C3 C8 118.6(8) . . ?
C7 C3 C13 123.4(8) . . ?
C8 C3 C13 117.9(7) . . ?
C12 O50 K4 120.3(5) . 1_455 ?
W2 O51 W1 152.3(3) . . ?
C5 C4 C6 118.0(8) . . ?
N1 C5 C4 120.5(8) . . ?
C1 C6 C12 122.5(7) . . ?
C4 C6 C1 120.3(7) . . ?
C4 C6 C12 116.9(7) . . ?
W8 O52 W9 151.2(3) . . ?
W8 O52 K5 107.4(3) . 3_565 ?
W9 O52 K5 98.7(3) . 3_565 ?
W4 O53 W8 90.19(17) 3_565 . ?
W7 O53 W4 93.13(18) 3_565 3_565 ?
W7 O53 W8 92.82(17) 3_565 . ?
Si14 O53 W4 123.3(3) . 3_565 ?
Si14 O53 W7 123.3(3) . 3_565 ?
Si14 O53 W8 124.8(3) . . ?
C3 C7 C9 119.8(8) . . ?
C3 C7 C14 123.1(8) . 2_545 ?
C9 C7 C14 117.1(8) . 2_545 ?
N2 C8 C3 118.7(8) . . ?
C13 O56 La2 144.5(6) . 2_545 ?
C11 C9 C7 119.1(8) . . ?
O25 C10 C1 117.7(7) . . ?
O33 C10 O25 126.1(8) . . ?
O33 C10 C1 116.2(7) . . ?
N2 C11 C9 121.4(8) . . ?
O39 C12 O50 126.0(7) 2_455 . ?
O39 C12 C6 118.8(7) 2_455 . ?
O50 C12 C6 115.1(7) . . ?
O24 C13 C3 116.1(8) . . ?
O56 C13 O24 125.4(8) . . ?
O56 C13 C3 118.5(7) . . ?
O31 C14 C7 115.6(8) . 2 ?
O42 C14 O31 126.5(9) . . ?
O42 C14 C7 117.8(8) . 2 ?
O22 K2 W6 30.93(11) . . ?
O22 K2 O35 81.25(17) . 1_455 ?
O22 K2 O40 150.0(2) . 4_576 ?
O22 K2 K5 120.8(2) . 2_455 ?
O35 K2 W6 73.02(13) 1_455 . ?
O35 K2 K5 105.9(2) 1_455 2_455 ?
O40 K2 W6 129.21(19) 4_576 . ?
O40 K2 O35 119.1(2) 4_576 1_455 ?
O40 K2 K5 77.07(19) 4_576 2_455 ?
O41 K2 W6 25.52(11) . . ?
O41 K2 O22 55.08(16) . . ?
O41 K2 O35 59.67(17) . 1_455 ?
O41 K2 O40 113.8(2) . 4_576 ?
O41 K2 O61 132.3(2) . . ?
O41 K2 K5 164.6(2) . 2_455 ?
O41 K2 O65 66.1(3) . . ?
O59 K2 W6 70.32(17) 4_576 . ?
O59 K2 O22 86.6(2) 4_576 . ?
O59 K2 O35 126.4(3) 4_576 1_455 ?
O59 K2 O40 63.7(2) 4_576 4_576 ?
O59 K2 O41 70.6(2) 4_576 . ?
O59 K2 O61 74.9(2) 4_576 . ?
O59 K2 K5 124.8(2) 4_576 2_455 ?
O59 K2 O65 85.0(4) 4_576 . ?
O60 K2 W6 135.0(2) . . ?
O60 K2 O22 140.9(2) . . ?
O60 K2 O35 63.7(2) . 1_455 ?
O60 K2 O40 68.1(2) . 4_576 ?
O60 K2 O41 113.4(3) . . ?
O60 K2 O59 127.5(3) . 4_576 ?
O60 K2 O61 113.6(3) . . ?
O60 K2 K5 59.1(3) . 2_455 ?
O60 K2 O65 55.7(4) . . ?
O61 K2 W6 110.98(18) . . ?
O61 K2 O22 91.5(2) . . ?
O61 K2 O35 156.6(3) . 1_455 ?
O61 K2 O40 77.2(2) . 4_576 ?
O61 K2 K5 59.0(2) . 2_455 ?
O61 K2 O65 141.7(4) . . ?
O62 K2 W6 70.9(3) . . ?
O62 K2 O22 94.6(4) . . ?
O62 K2 O35 111.4(5) . 1_455 ?
O62 K2 O40 58.6(4) . 4_576 ?
O62 K2 O41 62.8(4) . . ?
O62 K2 O59 18.5(4) . 4_576 ?
O62 K2 O60 113.3(5) . . ?
O62 K2 O61 91.3(5) . . ?
O62 K2 O64 153.2(5) . 1_455 ?
O62 K2 K5 131.8(4) . 2_455 ?
O62 K2 O65 66.6(5) . . ?
O64 K2 W6 87.0(2) 1_455 . ?
O64 K2 O22 59.8(3) 1_455 . ?
O64 K2 O35 74.6(3) 1_455 1_455 ?
O64 K2 O40 142.9(3) 1_455 4_576 ?
O64 K2 O41 102.9(3) 1_455 . ?
O64 K2 O59 138.9(3) 1_455 4_576 ?
O64 K2 O60 92.9(3) 1_455 . ?
O64 K2 O61 82.5(3) 1_455 . ?
O64 K2 K5 65.8(3) 1_455 2_455 ?
O64 K2 O65 130.9(4) 1_455 . ?
K5 K2 W6 151.5(2) 2_455 . ?
O65 K2 W6 91.6(3) . . ?
O65 K2 O22 119.9(3) . . ?
O65 K2 O35 58.3(3) . 1_455 ?
O65 K2 O40 64.7(3) . 4_576 ?
O65 K2 K5 112.4(3) . 2_455 ?
W10 K3 W4 91.10(9) . 3_665 ?
O14 K3 W4 171.6(2) . 3_665 ?
O14 K3 W10 90.18(19) . . ?
O14 K3 O17 164.1(3) . 3_665 ?
O14 K3 O23 103.2(3) . . ?
O14 K3 K3 103.3(2) . 3_665 ?
O17 K3 W4 21.19(12) 3_665 3_665 ?
O17 K3 W10 74.83(14) 3_665 . ?
O17 K3 K3 84.22(19) 3_665 3_665 ?
O23 K3 W4 68.63(17) . 3_665 ?
O23 K3 W10 85.33(19) . . ?
O23 K3 O17 81.3(2) . 3_665 ?
O23 K3 K3 130.9(3) . 3_665 ?
O34 K3 W4 76.32(18) . 3_665 ?
O34 K3 W4 90.99(19) 3_665 3_665 ?
O34 K3 W10 167.0(2) . . ?
O34 K3 W10 94.46(19) 3_665 . ?
O34 K3 O14 97.2(3) 3_665 . ?
O34 K3 O14 102.7(3) . . ?
O34 K3 O17 92.2(2) . 3_665 ?
O34 K3 O17 79.0(2) 3_665 3_665 ?
O34 K3 O23 93.0(3) . . ?
O34 K3 O23 159.6(3) 3_665 . ?
O34 K3 O34 82.7(3) 3_665 . ?
O34 K3 K3 41.04(18) . 3_665 ?
O34 K3 K3 41.62(18) 3_665 3_665 ?
O37 K3 W4 96.22(19) . 3_665 ?
O37 K3 W10 13.61(15) . . ?
O37 K3 O14 83.3(2) . . ?
O37 K3 O17 83.1(2) . 3_665 ?
O37 K3 O23 75.6(2) . . ?
O37 K3 O34 106.9(3) . 3_665 ?
O37 K3 O34 168.2(3) . . ?
O37 K3 K3 148.0(3) . 3_665 ?
K3 K3 W4 81.55(14) 3_665 3_665 ?
K3 K3 W10 134.75(18) 3_665 . ?
W9 K4 K2 121.1(3) . 1_655 ?
W11 K4 W9 48.31(12) . . ?
W11 K4 K2 73.11(19) . 1_655 ?
K1 K4 W9 78.7(2) . . ?
K1 K4 W11 57.67(16) . . ?
K1 K4 K2 63.17(17) . 1_655 ?
O12 K4 W9 112.3(3) . . ?
O12 K4 W11 122.3(3) . . ?
O12 K4 K1 165.7(3) . . ?
O12 K4 O25 80.1(3) . 1_655 ?
O12 K4 K2 102.7(3) . 1_655 ?
O12 K4 K5 55.5(2) . 2 ?
O25 K4 W9 142.0(3) 1_655 . ?
O25 K4 W11 153.1(3) 1_655 . ?
O25 K4 K1 96.8(3) 1_655 . ?
O25 K4 K2 88.3(3) 1_655 1_655 ?
O25 K4 K5 59.2(2) 1_655 2 ?
O38 K4 W9 24.01(15) . . ?
O38 K4 W11 24.63(16) . . ?
O38 K4 K1 63.9(2) . . ?
O38 K4 O12 122.9(4) . . ?
O38 K4 O25 154.0(4) . 1_655 ?
O38 K4 K2 97.1(3) . 1_655 ?
O38 K4 K5 142.0(4) . 2 ?
O50 K4 W9 89.9(3) 1_655 . ?
O50 K4 W11 138.3(4) 1_655 . ?
O50 K4 K1 123.0(3) 1_655 . ?
O50 K4 O12 67.7(3) 1_655 . ?
O50 K4 O25 60.6(3) 1_655 1_655 ?
O50 K4 O38 113.8(4) 1_655 . ?
O50 K4 K2 148.2(4) 1_655 1_655 ?
O50 K4 K5 100.5(4) 1_655 2 ?
O50 K4 K6 103.4(4) 1_655 . ?
O64 K4 W9 124.7(4) . . ?
O64 K4 W11 91.2(4) . . ?
O64 K4 K1 46.0(3) . . ?
O64 K4 O12 122.0(5) . . ?
O64 K4 O25 62.6(3) . 1_655 ?
O64 K4 O38 107.0(5) . . ?
O64 K4 O50 118.7(5) . 1_655 ?
O64 K4 K2 39.2(3) . 1_655 ?
O64 K4 K5 67.3(4) . 2 ?
O64 K4 K6 131.9(5) . . ?
K5 K4 W9 157.4(3) 2 . ?
K5 K4 W11 118.6(3) 2 . ?
K5 K4 K1 111.0(3) 2 . ?
K5 K4 K2 53.6(2) 2 1_655 ?
K6 K4 W9 74.0(2) . . ?
K6 K4 W11 68.9(2) . . ?
K6 K4 K1 125.4(3) . . ?
K6 K4 O12 53.6(2) . . ?
K6 K4 O25 132.7(4) . 1_655 ?
K6 K4 O38 72.6(3) . . ?
K6 K4 K2 92.7(3) . 1_655 ?
K6 K4 K5 84.1(3) . 2 ?
O62 O59 K2 46.7(9) 4_675 4_675 ?
K2 O60 K5 71.8(3) . 2_455 ?
K6 O60 K2 135.0(4) 1_455 . ?
K6 O60 K5 89.2(3) 1_455 2_455 ?
K2 O61 K5 68.1(2) . 2_455 ?
O59 O62 K2 114.9(12) 4_576 . ?
K2 O64 K1 100.9(4) 1_655 . ?
K4 O64 K1 89.5(5) . . ?
K4 O64 K2 102.2(4) . 1_655 ?
O12 K5 W9 117.2(2) 2_545 3_565 ?
O12 K5 O18 92.1(3) 2_545 . ?
O12 K5 O21 49.95(18) 2_545 . ?
O12 K5 O25 81.3(2) 2_545 2_445 ?
O12 K5 O52 88.6(2) 2_545 3_565 ?
O12 K5 K2 123.0(3) 2_545 2_445 ?
O12 K5 K4 58.2(2) 2_545 2_545 ?
O12 K5 O60 80.1(3) 2_545 2_445 ?
O12 K5 O61 172.2(3) 2_545 2_445 ?
O13 K5 W9 127.3(3) . 3_565 ?
O13 K5 O12 77.0(3) . 2_545 ?
O13 K5 O18 67.6(2) . . ?
O13 K5 O21 84.6(3) . . ?
O13 K5 O25 52.7(2) . 2_445 ?
O13 K5 O47 106.3(3) . 3_565 ?
O13 K5 O52 124.4(3) . 3_565 ?
O13 K5 K2 146.7(3) . 2_445 ?
O13 K5 K4 101.1(3) . 2_545 ?
O13 K5 O60 156.7(4) . 2_445 ?
O13 K5 O61 103.6(3) . 2_445 ?
O18 K5 W9 61.66(17) . 3_565 ?
O18 K5 O21 49.06(18) . . ?
O18 K5 O25 120.0(3) . 2_445 ?
O18 K5 O52 59.5(2) . 3_565 ?
O18 K5 K2 130.3(3) . 2_445 ?
O18 K5 K4 150.3(3) . 2_545 ?
O18 K5 O60 117.7(3) . 2_445 ?
O18 K5 O61 95.3(3) . 2_445 ?
O21 K5 W9 73.37(18) . 3_565 ?
O21 K5 O25 122.7(3) . 2_445 ?
O21 K5 K2 128.7(3) . 2_445 ?
O21 K5 K4 104.3(3) . 2_545 ?
O25 K5 W9 161.5(3) 2_445 3_565 ?
O25 K5 K2 100.7(2) 2_445 2_445 ?
O25 K5 K4 58.7(2) 2_445 2_545 ?
O47 K5 W9 26.55(13) 3_565 3_565 ?
O47 K5 O12 134.2(3) 3_565 2_545 ?
O47 K5 O18 51.55(19) 3_565 . ?
O47 K5 O21 84.5(2) 3_565 . ?
O47 K5 O25 137.8(3) 3_565 2_445 ?
O47 K5 O52 51.12(19) 3_565 3_565 ?
O47 K5 K2 79.5(2) 3_565 2_445 ?
O47 K5 K4 152.0(4) 3_565 2_545 ?
O47 K5 O60 92.7(3) 3_565 2_445 ?
O47 K5 O61 53.3(2) 3_565 2_445 ?
O52 K5 W9 28.61(12) 3_565 3_565 ?
O52 K5 O21 48.30(18) 3_565 . ?
O52 K5 O25 169.8(3) 3_565 2_445 ?
O52 K5 K2 85.2(2) 3_565 2_445 ?
O52 K5 K4 116.0(3) 3_565 2_545 ?
O52 K5 O60 58.7(2) 3_565 2_445 ?
O52 K5 O61 97.3(3) 3_565 2_445 ?
K2 K5 W9 70.75(16) 2_445 3_565 ?
K4 K5 W9 130.3(3) 2_545 3_565 ?
K4 K5 K2 74.4(2) 2_545 2_445 ?
O60 K5 W9 67.9(2) 2_445 3_565 ?
O60 K5 O21 84.0(3) 2_445 . ?
O60 K5 O25 119.5(3) 2_445 2_445 ?
O60 K5 K2 49.0(2) 2_445 2_445 ?
O60 K5 K4 62.5(3) 2_445 2_545 ?
O60 K5 O61 98.5(3) 2_445 2_445 ?
O61 K5 W9 68.8(2) 2_445 3_565 ?
O61 K5 O21 137.7(3) 2_445 . ?
O61 K5 O25 92.9(3) 2_445 2_445 ?
O61 K5 K2 52.9(2) 2_445 2_445 ?
O61 K5 K4 114.3(3) 2_445 2_545 ?
W2 K6 W3 53.09(3) . . ?
O10 K6 W2 31.15(11) . . ?
O10 K6 W3 65.47(12) . . ?
O10 K6 O20 117.55(17) . . ?
O10 K6 O27 61.01(15) . . ?
O10 K6 O38 50.61(15) . . ?
O10 K6 O43 137.18(19) . . ?
O10 K6 O44 105.88(17) . 4_676 ?
O11 K6 W2 31.70(12) . . ?
O11 K6 W3 27.16(11) . . ?
O11 K6 O10 56.26(16) . . ?
O11 K6 O20 95.00(17) . . ?
O11 K6 O27 52.50(15) . . ?
O11 K6 O38 88.07(16) . . ?
O11 K6 O43 81.11(19) . . ?
O11 K6 O44 88.32(17) . 4_676 ?
O11 K6 K4 141.4(3) . . ?
O11 K6 O60 114.6(3) . 1_655 ?
O12 K6 W2 159.22(14) . . ?
O12 K6 W3 127.16(14) . . ?
O12 K6 O10 165.88(19) . . ?
O12 K6 O11 137.80(19) . . ?
O12 K6 O20 67.52(16) . . ?
O12 K6 O27 125.75(17) . . ?
O12 K6 O38 122.35(17) . . ?
O12 K6 O43 56.93(19) . . ?
O12 K6 O44 76.68(17) . 4_676 ?
O12 K6 K4 71.6(3) . . ?
O12 K6 O60 95.1(3) . 1_655 ?
O20 K6 W2 121.43(13) . . ?
O20 K6 W3 69.21(12) . . ?
O20 K6 O27 58.23(15) . . ?
O20 K6 O38 78.05(16) . . ?
O27 K6 W2 66.18(11) . . ?
O27 K6 W3 29.51(10) . . ?
O27 K6 O38 47.92(14) . . ?
O38 K6 W2 78.42(11) . . ?
O38 K6 W3 74.97(10) . . ?
O43 K6 W2 109.92(15) . . ?
O43 K6 W3 74.75(14) . . ?
O43 K6 O20 57.38(17) . . ?
O43 K6 O27 91.39(17) . . ?
O43 K6 O38 132.58(18) . . ?
O44 K6 W2 84.22(13) 4_676 . ?
O44 K6 W3 111.05(13) 4_676 . ?
O44 K6 O20 129.58(18) 4_676 . ?
O44 K6 O27 140.20(17) 4_676 . ?
O44 K6 O38 152.35(18) 4_676 . ?
O44 K6 O43 73.68(18) 4_676 . ?
K4 K6 W2 128.0(2) . . ?
K4 K6 W3 120.6(2) . . ?
K4 K6 O10 96.9(3) . . ?
K4 K6 O20 72.0(2) . . ?
K4 K6 O27 91.4(2) . . ?
K4 K6 O38 54.1(2) . . ?
K4 K6 O43 117.2(3) . . ?
K4 K6 O44 128.3(3) . 4_676 ?
K4 K6 O60 77.3(3) . 1_655 ?
O60 K6 W2 84.4(2) 1_655 . ?
O60 K6 W3 136.8(2) 1_655 . ?
O60 K6 O10 74.0(2) 1_655 . ?
O60 K6 O20 148.2(3) 1_655 . ?
O60 K6 O27 131.9(2) 1_655 . ?
O60 K6 O38 90.9(2) 1_655 . ?
O60 K6 O43 135.5(2) 1_655 . ?
O60 K6 O44 66.0(2) 1_655 4_676 ?


_olex2_submission_special_instructions 'No special instructions were received'
